STRENGTH OF MATERIALS
No part of this digital document may be reproduced, stored in a retrieval system or transmitted ...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

STRENGTH OF MATERIALS

No part of this digital document may be reproduced, stored in a retrieval system or transmitted in any form or by any means. The publisher has taken reasonable care in the preparation of this digital document, but makes no expressed or implied warranty of any kind and assumes no responsibility for any errors or omissions. No liability is assumed for incidental or consequential damages in connection with or arising out of information contained herein. This digital document is sold with the clear understanding that the publisher is not engaged in rendering legal, medical or any other professional services.

STRENGTH OF MATERIALS

GUSTAVO MENDES AND

BRUNO LAGO EDITORS

Nova Science Publishers, Inc. New York

Copyright © 2009 by Nova Science Publishers, Inc. All rights reserved. No part of this book may be reproduced, stored in a retrieval system or transmitted in any form or by any means: electronic, electrostatic, magnetic, tape, mechanical photocopying, recording or otherwise without the written permission of the Publisher. For permission to use material from this book please contact us: Telephone 631-231-7269; Fax 631-231-8175 Web Site: http://www.novapublishers.com NOTICE TO THE READER The Publisher has taken reasonable care in the preparation of this book, but makes no expressed or implied warranty of any kind and assumes no responsibility for any errors or omissions. No liability is assumed for incidental or consequential damages in connection with or arising out of information contained in this book. The Publisher shall not be liable for any special, consequential, or exemplary damages resulting, in whole or in part, from the readers’ use of, or reliance upon, this material. Any parts of this book based on government reports are so indicated and copyright is claimed for those parts to the extent applicable to compilations of such works. Independent verification should be sought for any data, advice or recommendations contained in this book. In addition, no responsibility is assumed by the publisher for any injury and/or damage to persons or property arising from any methods, products, instructions, ideas or otherwise contained in this publication. This publication is designed to provide accurate and authoritative information with regard to the subject matter covered herein. It is sold with the clear understanding that the Publisher is not engaged in rendering legal or any other professional services. If legal or any other expert assistance is required, the services of a competent person should be sought. FROM A DECLARATION OF PARTICIPANTS JOINTLY ADOPTED BY A COMMITTEE OF THE AMERICAN BAR ASSOCIATION AND A COMMITTEE OF PUBLISHERS. LIBRARY OF CONGRESS CATALOGING-IN-PUBLICATION DATA Strength of materials / edited by Gustavo Mendes and Bruno Lago. p. cm. Includes bibliographical references. ISBN 978-1-61728-584-4 (E-Book) 1. Strength of materials. 2. Composite materials. I. Mendes, Gustavo. II. Lago, Bruno. TA405.S765 2009 620.1'12--dc22 2009013535

Published by Nova Science Publishers, Inc.

New York

CONTENTS Preface

vii

Chapter 1

High Temperature Mechanical Properties and Microstructure of Sic-Based Fibers under Severe Environments Jianjun Sha

Chapter 2

Ionomers as Candidates for Structural Materials Daniel J. Klein

61

Chapter 3

Failure of Layered Composites Subject to Impacts: Constitutive Modeling and Parameter Identification Issues Stefano Mariani

97

Chapter 4

Current State of the Art of the Ceramic Composite Material BIOLOX®delta Meinhard Kuntz, Bernard Masson and Thomas Pandorf

133

Chapter 5

Particle Modeling and Its Current Success in the Simulations of Dynamics Fragmentation of Solids G. Wang, A. Al-Ostaz, A.H.D. Cheng and P. Radziszewski

157

Chapter 6

Non-Oriented Electrical Steels: Materials for Saving Energy and Conserving the Environment Taisei Nakayama

183

Chapter 7

Influence of Luting Cement Application Technique on Quartz Fiber Post Regional Bond Strengths Camillo D’Arcangelo, Francesco De Angelis, Maurizio D’Amario, Simone Zazzeroni, Mirco Vadini and Sergio Caputi

217

Chapter 8

Microstructural Influence on Flexure Strength of a Ceromer Reinforced by Two Types of Fibers (Polyethylene and Glass) Silvana Marques Miranda Spyrides and Fernando Luiz Bastian

233

1

vi Chapter 9

Index

Contents Influence on Strength Properties of Anisotropy Planes in Slates Samples in the NW of Spain M.A. Rodríguez-Sastre, M. Gutiérrez-Claverol, M. Torres-Alonso and L. Calleja

247

261

PREFACE The strength of a material refers to the material's ability to withstand an applied stress without failure. The applied stress may be tensile, compressive, or shear. A material's strength is dependent on its microstructure. The engineering processes to which a material is subjected can alter this microstructure. This book provides a variety of material strength research including an extensive overview on the state of the art ceramic composite material BIOLOX delta which, since 2001, has successfully implanted more than 500,000 artificial hip joints. Due to the unique strength and toughness of this material, the risk of fracture has been substantially reduced when compared to conventional ceramic materials. Several different aspects of ionomer research from a physical property standpoint is discussed as well, including the history and current trends in ionomer research and a discussion on the immediate needs in this field. Furthermore, particle modeling (PM) as an innovative particulate dynamics based modeling approach is examined as a robust tool for simulating fracture problems of solids under extreme loading conditions, including situations of collapse, impact, blasting or high strain rate tension/compression. This book includes research on the ability of particle modeling to correctly predict dynamic fragmentation of materials with good accuracy. Ceramic-matrix composites (CMCs) have been considering as potential structural materials for advanced energy-generation systems and propulsion systems. SiC fibers with low oxygen content and high crystallinity, which derived from polycarbonsilane, are the backbone as reinforcements in load-bearing CMCs. For high temperature application, the most desired critical properties of SiC fibers are high strength and stiffness as well as the reliable retention of these properties throughout the service life of application. Low fiber strength and thermal stability could result in low fracture toughness and accelerate sub-critical crack propagation in CMCs. Thus, the mechanical durability and microstructure stability of SiC fibers are major concerns under severe environments. Furthermore, in practical service environments, rarely is one degradation mechanism operative, but several mechanisms operate simultaneously, leading to the environment-pertinent degradation mechanism is complex for the SiC materials. In order to enhance the understanding of reliability and durability of CMCs applied to high temperature and oxidative environments, the investigations on the high temperature mechanical properties and microstructure for SiCbased fibers subjected to severe environments were integrated into Chapter 1. The field of ionomers is an often overlooked and under-utilized branch of polymer research. Although ionomers can be broadly described as a class of polymers that contain any

viii

Gustavo Mendes and Bruno Lago

number of ionic groups, from a structural property standpoint only a low percent of ionic groups are necessary to impart significantly improved properties over the nonionic version of the same polymer. Current trends in the field of ionomers are highly focused on the field of fuel cell technology. There appears to be a significant hole remaining in the study of imparting strength to materials using ionic groups. This hole is very significant from an industrial point of view, and has a large commercial potential. There are very few commercially available ionomers, which shows how little this field has been explored to date. Chapter 2 will focus on several aspects of ionomer research from a physical property standpoint: 1) A history of ionomer research, 2) Current trends in ionomer research - a) standalone polymers, b) nanocomposites, c) blends; 3) A commentary on the immediate needs in the field of ionomer research. Layered composites subject to impacts can fail by delamination, i.e. by debonding between laminae, if the stress waves cause damaging phenomena to take place mainly within the resin-enriched interlaminar phases. To simulate delamination at the structural level, processes dissipating energy are lumped onto fictitious zero-thickness interlaminar surfaces, and softening interface constitutive laws are adopted to describe the progressive failure of the interlaminar phases. Since delamination occurs inside very narrow regions, results of experimental testing on whole composites need to be accurately and reliably filtered to calibrate the interface constitutive laws. To this aim, Chapter 3 proposes a sigma-point Kalman filter approach. The performances of the proposed methodology, in terms of constitutive parameter estimations and dynamic delamination tracking, are assessed through pseudoexperimental testings on a two-layer composite, and real testings on multi-layer glass fiber reinforced plastic composites. An extensive overview about the state of the art of the ceramic composite material BIOLOX®delta is given. The unique properties rely on a well defined alumina based fine composite microstructure which is mainly achieved by high temperature solid body reaction of the different ceramic phases during sintering. Zirconia comprises 17 % of the total volume. The tetragonal phase of zirconia is stabilized chemically and mechanically. The high strength and toughness of the material depend on transformation toughening of the zirconia which is clearly shown by various experimental results. The excellent mechanical properties are reproduced batch by batch with a very low scatter. As presented in Chapter 4, the outstanding properties of the material BIOLOX®delta support advantageous properties of the final product, e.g. ceramic hard-hard bearings for hip arthroplasty. The burst load of the components is significantly increased. It is shown that the design of the components is also very important for the reliability and the ultimate properties of the system. Wear properties at severe conditions are significantly improved by using the new composite material BIOLOX®delta in comparison to pure alumina. Phase transformation of zirconia from the tetragonal to the monoclinic phase due to hydrothermal aging is extensively discussed. Due to the particular distribution and stabilization of the zirconia particles instable aging effects are not possible in this material. After very long time of accelerated aging conditions an increase of monoclinic phase is found – however, it is shown that dynamic and static properties of BIOLOX®delta are not influenced by this effect.

Preface

ix

Chapter 5 studies particle modeling (PM), which is an innovative particulate dynamics based modeling approach. It has been demonstrated as a robust tool for simulating fracture problems of solids with dynamic fragmentation under extreme loading conditions. These loading conditions can include situations of collapse, impact, blasting or high strain rate tension/compression, as well as thermally-induced breakage problems. Initially, PM was developed for the purpose of mimicking the microscopic material process at macroscopic level. This method can be conceptually illustrated by fully dynamic particles (or “quasi-particles”) placed at the nodes of a lattice network without explicitly considering their geometric size. The potential can be specified for particle-particle interactions via axial springs. Theoretically, PM is an upscale of the molecular dynamics (MD) model applicable to various length scale problems. This is possible if a proper equivalent macroscopic potential is found, and, in case of lattice spacing decreasing to a few Angstroms, a MD model at zero Kelvin with, say, Leonard-Jones potential is recovered. In its current form, PM has been developed as a tool applicable to real engineering problems. The advantages of PM over the existing discrete element based methods can be summarized as follows: (1) Sample in theory. Four conservative/equivalent rules (mass, potential energy, Young’s modulus and tensile/compression strength) are applied to preserve the equivalent material properties. (2) Easy for implementation. Since the physical size of each particle is ignored other than its equivalent mass, the algorithm of coding a PM computation is fairly easy. Current research work has exhibited that PM is able to correctly predict dynamic fragmentation of materials with a good accuracy. In modeling an epoxy plate with randomly distributed holes in tension, the PM result of the final crack pattern compared favorably with the associate experiment; for the simulations of impact study of two polymeric materials (nylon, 6-6 and vinyl ester) subject to a rigid falling indenter, the modeling results of resistant force, energy, deflection and drop speed of indenter vs. time quantitatively agree fairly well with the according empirical observations. Electrical steels are the core materials for electrical motors or transformers. Those materials for motors are played an energy conversion roll from electricity to motion. However, energy losses are accompanied with this conversion. To minimize these losses is a key technology to conserve our environment. Numerous researches on the grain-oriented electrical steels reported. Those researches especially for transformers are focused on the reducing the losses at supplying the electricity from power plants. On the other hand, home or industrial appliances are the power consuming devices, and the most effective point on the energy loss reduction. These home appliances are used small motors using non-oriented electrical steels. In Chapter 6, several researches on the non-oriented electrical steels are discussed and focused on the metallurgical control of the steels to reduce the core loss for generating waste heats and motor building innovation technologies for decreasing the building factor of the core losses. In the metallurgical part, some additive elements as phosphorus, aluminum and manganese for improving magnetic properties reviewed. Moreover some contaminating elements as vanadium, titanium and zirconium are discussed especially for precipitation studies in the steels have been done. These precipitations are inhibited the grain growth at final annealing or stress relief annealing. These inhibited small grains increase the core losses.

x

Gustavo Mendes and Bruno Lago

For studying motor building technologies, compression stress effect, shearing stress effect are discussed. Even though the best core materials are used for manufacturing motors, those building deteriorations make worse for the motor efficiency. Therefore, those technologies are also important for reducing the carbon dioxide emission. The aim of Chapter 7 was to investigate regional root canal push-out bond strengths for a fiber-reinforced post system varying the application method of the luting agent. Recently extracted maxillary incisors (n=30) were sectioned transversally at the labial cemento-enamel junction, and the roots treated endodontically. Following post space preparations, fiber-reinforced posts (Endo Light-Post; RTD) were placed using adhesive system and resin cement provided by the manufacturer. Three equal groups (n=10) were assessed according to the technique used to place the luting agent into post space: using a lentulo spiral, applying the cement onto the post surface, injecting the material with a specific syringe. Each root was sliced into three discs (2 mm thick) representing the coronal, middle and apical part of the bonded fiber post. Push-out tests were performed for each specimen to measure regional bond strengths. Results were statistically analyzed using two-way ANOVA and Tukey tests (α = 0.05). All fractured specimens were observed using a scanning electron microscope to identify the types of failure. The results indicated that bond strength values were significantly affected by the application method of the resin cement (p < 0.05). The "syringe technique" and the "lentulo technique" showed higher bond strength values compared with the "post technique". No significant differences were recorded among the post space thirds. Microscopic analysis revealed a prevalence of post/cement and mixed failures. The best performance in terms of push-out bond strengths for the post system tested was obtained when the luting agent was applied into the post space either with a specific syringe or using a lentulo spiral. There were not differences in bond strength among root thirds. In Chapter 8, the microstructures of a ceromer (Artglass®) reinforced by either glass fibers (GlasSpan®) or polyethylene fibers (Connect®) were characterized and compared and the influence of the fiber reinforcement on the flexural strength of the resulting products evaluated. With this objective, seven bars of each material were produced. One bar of each material was separated for microstructural analysis. The microstructural samples were subjected to metallographic polishing and finishing, and then analyzed using optical microscopy at different magnifications. The images obtained were treated using an image processing computer program (Image Pro Plus) in order to quantify the microstructure by calculating the mean diameter and mean volume fraction of fibers. The flexure tests were made by three-point bending, using six samples of each material. After statistical analysis, the results showed that the mean diameter of the glass fibers (4μm) was smaller than the polyethylene ones (23.6 μm). The mean volume fraction of glass fibers (0.42) was larger than that of the polyethylene fibers (0.28) and the mean center-to-center distance between fibers was smaller in the glass fibers material (33 μm) than in the polyethylene fibers material (61 μm). The flexural strength of both glass and polyethylene fiber-reinforced materials was statistically equal, despite the fiber volume fraction being statistically larger in the fiber glass material. The purpose of Chapter 9 is to describe the influence of anisotropy on the geomechanical strength properties of two Spanish slates with different chemical and physical characteristics. From laboratory testing results of slates under point load and uniaxial compression and the use of indirect methods, as it is the measurement of P velocities, principal parameters were

Preface

xi

calculated for this rock material. As it is well known under uniaxial compressive strength slates are strong and also very strong rock when loading is parallel (90o) o perpendicular (0o) to the main anisotropic planes. In contrast it is a weak rock with minimum strength values for angles between 45 to 60o of inclination of anisotropy planes. The correlation equations were calculated between different parameters. Despite weak correlation between different geotechnical properties were found and when all lithologies are considered together correlation of geomechanical properties is weak. However when each lithology is considered separately the geomechanical properties can be coherently defined. Linear and polynomial equations were found for the point load and uniaxial strength correlations with the inclination of the anisotropy. Different strength fields were calculated when uniaxial strength and point load test plot and its comparison include the inclination of the anisotropy planes on slates. Uniaxial compressive strength and P wave velocity appears to be strongly influenced by uniaxial strength and good polynomial correlations resulted. Plots of slates with other sedimentary type of rocks from Cantabrian Zone, CZ, revealed the hardness and highest strength of slates when loading is perpendicular to the main anisotropy planes.

In: Strength of Materials Editors: G. Mendes and B. Lago, pp. 1-60

ISBN: 978-1-60741-500-8 © 2009 Nova Science Publishers, Inc.

Chapter 1

HIGH TEMPERATURE MECHANICAL PROPERTIES AND MICROSTRUCTURE OF SIC-BASED FIBERS UNDER SEVERE ENVIRONMENTS Jianjun Sha1,2* 1

Shool of Aeronautics and Astronautics, Dalian University of Technology 116024, Dalian, China 2 Ceramic Materials Engineering, University of Bayreuth, D-95440 Bayreuth, Germany

Abstract Ceramic-matrix composites (CMCs) have been considering as potential structural materials for advanced energy-generation systems and propulsion systems. SiC fibers with low oxygen content and high crystallinity, which derived from polycarbonsilane, are the backbone as reinforcements in load-bearing CMCs. For high temperature application, the most desired critical properties of SiC fibers are high strength and stiffness as well as the reliable retention of these properties throughout the service life of application. Low fiber strength and thermal stability could result in low fracture toughness and accelerate sub-critical crack propagation in CMCs. Thus, the mechanical durability and microstructure stability of SiC fibers are major concerns under severe environments. Furthermore, in practical service environments, rarely is one degradation mechanism operative, but several mechanisms operate simultaneously, leading to the environment-pertinent degradation mechanism is complex for the SiC materials. In order to enhance the understanding of reliability and durability of CMCs applied to high temperature and oxidative environments, the investigations on the high temperature mechanical properties and microstructure for SiC-based fibers subjected to severe environments were integrated into this review.

*

Corresponding address: School of Aeronautics and Astronautics, Dalian University of Technology, 116024, Dalian, China

2

Jianjun Sha

1. Introduction Non-oxide Ceramic-matrix Composites (CMCs), have been extensively studied during the last two decades. Currently, CMCs have been proposed to use as the structural materials in application of high temperature technologies, such as advanced nuclear energy systems [13], various stationary gas turbine engines and aerospace propulsion systems [4-6]. As structural engineering materials, one of the important advantages of CMCs is the significant improvement of toughness by using continuous ceramic fibers compared to their monolithic ceramics. In continuous ceramic fiber reinforced CMCs, the improved toughness is attributed to several energy dissipating mechanisms when the matrix crack is occurring under applied stress, such as crack deflection, fiber bridging and fiber sliding [7]. The energy dissipation procedure can be illustrated schematically in Figure 1. These energy dissipations enhanced the fracture toughness and resulted in a non-catastrophic failure mode. If the conditions for de-bonding are satisfied, fibers bridge the crack faces in the wake of the crack tip, subsequent to matrix cracking. The stress bore by bridge fibers applies traction forces to the crack faces that reduce the stress intensity at the crack tip. Under specific condition crack propagation does not occur without additional applied stress. The performance of CMCs could be improved through the optimization of fiber/interface/matrix, and now the fabrication process is still in developing and progressing.

σ

σ Fiber bridging

Fiber fracture

Interface Fibers

Crack tip Crack

crack

Crack deflection Matrix

σ Monolithic

σ composite

Figure 1. Schematic of crack propagation and principle for improved toughness in CMCs.

Based on the simple theory of mixture for the ultimate tensile strength (UTS) calculation of continuous fiber reinforced ceramic matrix composites [8], in the case of CMCs with I-D reinforcement alignment, when the reinforced fiber has a smaller modulus and a similar or even large strength, significant matrix cracks must be occurred before reaching the UTS of

High Temperature Mechanical Properties and Microstructure…

3

fiber. In other words, when the applied stress is beyond that of the crack initiation of matrix, the residual stress is mainly carried by the fiber alone. Pull out of the fiber can significantly improve the fracture toughness. The fibers are backbone in CMCs and play a very important role on the mechanical properties of CMCs. Among of CMCs, SiC fiber reinforced SiC matrix composite (SiC/SiC) has been considered as one of the most potential candidate materials, because it possessed many attractive properties for structural engineering applications under severe environments, such as excellent mechanical and chemical stability. It is well know, the fracture behavior of monolithic silicon carbide is brittle and fails catastrophically. However, if the SiC fibers with an appropriate coating as reinforcement are incorporated with the silicon carbide matrix by specific fabrication process to form the ceramic matrix composite, the fracture characteristics of silicon carbide materials can be significantly improved. Figure 2 shows the typical polished morphologies and the fracture surface of near-net shape SiC/SiC composite. It is apparent that reinforcing fibers incorporated with dense matrix through an appropriate interphase. The significant fibers pull out could improve the fracture toughness and result in a pseudo-ductile fracture behavior. The tough ceramics as structural materials have the potential for being used up to about 1500 °C which is much higher than the operation temperature of superalloy (maximum 1100 °C close to the melting point). In different fields, such as advanced nuclear energy system, gas turbines for power/steam co-generation, heat exchangers and so on, they give different requirements for materials performance, but common features for high temperature technologies are excellent mechanical performance and environmental durability.

Figure 2. Typical polished morphology of SiC/SiC composite and its fracture surface with long fiber pull out.

The major advantages for SiC/SiC composite applied to engineering are: (i) high specific strength, (ii) superior high temperature strength and creep resistance, (iii) low thermal expansion coefficient and high thermal conductivity, (iv) low neutron irradiation-induced radioactivity in nuclear environments.

4

Jianjun Sha

SiC fibers with low oxygen content and high crystallinity, which derived from polycarbonsilane, are the backbone as reinforcements in load-bearing CMCs. For high temperature application, the most desired critical properties of SiC fibers are high strength and stiffness as well as the reliable retention of these properties throughout the service life of application. Low fiber strength and thermal stability could result in low fracture toughness and accelerate sub-critical crack propagation in CMCs. The key to the successful application of high temperature ceramic matrix composites (CMC) is the judicious selection and incorporation of ceramic fiber reinforcement with the proper chemical, physical and mechanical properties. Thus, the mechanical durability and the microstructure stability of SiC fibers are major concerns under severe environments. In practical service environments, rarely is one degradation mechanism operative, but several mechanisms operate simultaneously, which leading to the environment-pertinent degradation mechanism is complex for the SiC materials. For understanding the environmental durability and describing the response of reinforced fibers to service environments and further evaluation of reliability of CMCs, the investigation of thermal mechanical properties on SiC-based fibers in complex situation is essential. In this chapter, the investigations on mechanical properties and microstructure of SiC-based fibers are reviewed in terms of varied environments; some issues concerning the environmentpertinent properties are discussed.

2. Materials System and Characterization Technique 2.1. Materials System The first SiC-based Nicalon fiber was produced by Nippon Carbon which allowed nonoxide ceramic matrix composites to be developed. It made possible to use the SiC fiber as the reinforcement for high temperature structural materials in very severe environments. In order to improve the flexibility and strength so that the preform can be woven in complex shape, the fine diameter SiC fibers were developed. However the first SiC-based fibers are inherently limited by oxidation at very high temperatures. As a result of this limitation a renewal of interest has occurred in oxide resistance of SiC fibers by approaching to the near stoichiometric composition or addition of small amount additives to improve thermal stability at elevated temperatures. Efforts have been made to improve the high temperature properties of fine diameter SiC fibers by making them with compositions increasingly approaching stoichiometry. Based on the chemical composition and the fabrication process, the development of SiC-based fibers could be categorized into three generations as illustrated in Figure 3. The first fine diameter SiC fiber (Nicalon NL200) was synthesized by Yajima in Japan in 1970 [9]. The Nicalon fiber could be viewed as the representative of the first generation of SiC fibers (Figure 3). This fiber is thermodynamically unstable at high temperature, because it consists of SiC-nanocrystals (average size: 1-2 nm) and free carbon embedded in an amorphous SiCxOy matrix. The amorphous SiCxOy phase decomposes at temperature beyond 1300 ˚C [10-11], with a significant gaseous species evolution and SiC crystal growth [11-12]. In order to improve the high temperature resistance of the Si-C-O fiber, a new fabrication

High Temperature Mechanical Properties and Microstructure…

5

process of the fiber, radiation curing method [13-15], has been developed. Irradiation curing with an electron beam was applied to make the fiber infusible and cross linking. β-SiC crystallite (~2 nm)

Amorphous (Si-C-O)

Stoichiometric Crystallized

Reduced oxygen

Low thermal stability Low strength Low stiffness

Amorphous Si-C-O Fibers NicalonTM TyrannoTM-LoxM, etc.

β-SiC crystallite (>20 nm)

β-SiC crystallite (~5 nm)

Improved thermal stability Modest oxidation resistance

Increased elastic modulus Enhanced creep resistance Enhanced oxidation resistance

Low-Oxygen Si-C Fibers Hi-NicalonTM TyrannoTM-ZMI, etc.

Crystalline SiC Fibers NicalonTM Type-S TyrannoTM-SA

Figure 3. Illustration of R&D of SiC-based Fibers.

To avoid the thermal instability caused by the decomposition of oxycarbide phase (SiCxOy), in 1990, a nearly oxygen-free SiC fiber, Hi-Nicalon (Nippon-Carbon) was developed by melt spinning, electron beam curing and pyrolysis of a polycarbosilane precursor (PCS) under anaerobic conditions [15-16]. This fiber had a much higher thermal stability than the standard Nicalon fiber and was viewed as the representative of the second generation. However, the Hi-Nicalon fiber consists of not only SiC nanocrystals (average crystal size: 5 nm) but also excess of free carbon which affects its oxidation and creep resistance. To reduce the free carbon content and eventually improve the high temperature properties of the fibers, extensive efforts have been devoted to develop near stoichiometric and high crystallized SiC fibers. The precursor fiber can be sintered at high temperatures that excess carbon and oxygen are lost as volatile species to yield polycrystalline and near-stoichiometric SiC fiber. These fibers are advanced SiC fibers and generally called the third generation of SiC fibers (Figure 3), including Hi-Nicalon type S fiber [17], Tyranno SA fibers [18] and Sylramic SiC fiber [19]. The third generation of SiC fibers is oxygen-free and nearstoichiometric (atomic ratio: C/Si=1.00–1.08). Furthermore, their grain size is relatively large (20–200 nm) and their thermal stability is excellent. For enhancing the environmental durability of CMCs, SiC-based fibers with high crystallinity and near stoichiometry would be preferential. Based on this standing point, the following SiC-based fibers were used for the work presented in this chapter (Table 1).

6

Jianjun Sha Table 1. SiC-based fibers used for the work in this chapter and their properties provided by manufacture

SiC fiber HNL HNLS TySA

C/Si

Oxygen (wt%)

Strength (Gpa)

Modulus (Gpa)

Density (g/cm3)

Diameter (μm)

1.39 1.05 1.07

0.5 0.2 [u]e

where ς is a model parameter that allows to match the slope of the softening branch just beyond the attainment of the peak traction τM . Sometimes, a smooth transition from the elastic regime to the softening one turns out to be more representative of the actual interphase response. The nonlinear binding model, originally proposed in [30, 31] for metals and bimetallic compounds and later adopted also in nonlinear fracture mechanics [20, 21, 32], allows to describe such smooth transition through the following exponential (EXP) law (see Figure 2(c)): [u] τ = K[u] exp − (14) [u]e Besides the effective stiffness K and strength τM , a full characterization of the nonlinear behavior of the interface has to match the fracture energy, or work of separation G. In terms of effective quantities, G is defined as the amount of energy required to annihilate the interaction between the opening/sliding crack faces, i.e.: G=

Z∞

τ d[u]

(15)

0

From a model calibration perspective, parameters Q and ς in (12) and (13) can be tuned to accurately match the actual G, since they do affect only the softening branch of the interface law. On the other hand, after having assigned K in (14), only [u]e can be adjusted: therefore, both τM and G can not be accurately matched. In the exponential law, in fact, the following constraint holds: s KG (16) 2 =e τM

104

Stefano Mariani

e being the Nepero number. To avoid problems related to this fictitious constraint, a modified exponential law is here formulated as follows (see Figure 3): [u] q τ = K[u] exp − (17) [u]e where q shows up as an additional constitutive parameter. In law (17): K still represents the initial elastic stiffness; [u]e is a reference effective displacement discontinuity, while peak traction τM is attained at [¯ u] ≡ (1/q)1/q [u]e . The effective peak traction and fracture energy are affected by q, according to: 1/q 1 1 exp − τM =K[u]e q q K 2 G = [u]2e γf q q

(18)

γf being the gamma function. The dependence of τM and G on the parameter q is depicted in Figure 4: it can be seen that G is a monotonically decreasing function of q, whereas τM is lower-bounded by the value corresponding to q = 1. Having tuned K, this law thus allows the calibration of both τM and G. All the above laws but the piecewise linear one, assume that the interaction between the opening interface sides continues up to [u] → ∞, which seems not physical at the macroscale. To simulate delamination growth a breakdown threshold therefore needs to be introduced [33, 34]: as soon as the current traction τ reduces to a small fraction (say 5-10 %) of the peak value τM , the interaction is suddenly assumed to vanish. When unloading from the tensile envelope occurs, i.e. when [u] ˙ < 0, the above interface models can be viewed as either reversible, if τ always belongs to the envelope (leading to interface healing if softening has already started), or irreversible, if τ decreases following a radial path to the origin of the τ − [u] plane. These two alternative constitutive assumptions lead to different entries in the interface tangent stiffness matrix E Γ , linking rates of τ and [u] in the local n − sj1 − sj2 reference frame according to: τ˙ = E Γ [u] ˙

(19)

For additional details, readers are referred to [27, 28].

2.3.

Finite Element Formulation

The weak form of the equilibrium equations (1)-(3) reads: Z

Ω\Γ

T

εv σ dΩ =

Z

Ω\Γ

¯ − ̺¨ v (b u) dΩ + T

Z

Γτ

T

v τ¯ dΓτ −

nΓ Z X j=1 Γ

[v]T τ dΓj

∀v ∈ U0 (20)

j

where: v is the test function; εv = Cv; U is the trial solution space, collecting displacement fields u continuous in Ω\Γ, possibly discontinuous along each Γj and fulfilling the boundary condition (5) on Γu ; U0 is the relevant variation space, with zero prescribed

Failure of Layered Composites Subject to Impacts

105

Figure 3. effect of q on the modified exponential traction-displacement discontinuity law (17).

(a)

(b)

Figure 4. modified exponential law (17). Effects of q on (a) the effective peak traction τM and on (b) the effective fracture energy G. displacements on Γu . In (20), in view of the assumed linearized kinematics, the relation − Γj ≡ Γ+ j ≡ Γj for each interface has been exploited. Allowing for the elastic bulk constitutive law (8), the following variational statement is arrived at: Z Z nΓ Z X T T ¨ dΩ + find u ∈ U : ̺v u εv E Ω ε dΩ + [v]T τ dΓj Ω\Γ

j=1 Γ

Ω\Γ

=

Z

Ω\Γ

j

T¯

v b dΩ +

Z

Γτ

T

v τ¯ dΓτ

(21)

∀v ∈ U0

106

Stefano Mariani

Now, let the finite element approximation of the displacement and deformation fields in Ω\Γ be (see [35] for the notation): u∼ = Φuh

(22)

ε∼ = CΦuh = B Ω uh

(23)

where matrix Φ gathers the nodal shape functions, and vector uh collects the nodal displacements. If delamination is allowed to occur only along element boundaries, the discrete displacement jump field can be written: [u]

Γj

∼ = B Γj uh

j = 1, ..., nΓ

(24)

Owing to the discrete interpolation fields defined above, the semi-discretized equations of motion of the composite turn out to be: ¨ h + K Ω uh + Mu

nΓ X

Rj = F

(25)

j=1

where the mass matrix M , the bulk stiffness matrix K Ω , the internal force vectors Rj and the external load vector F are, respectively: M=

Z

̺ ΦT Φ dΩ

Z

B TΩ E Ω B Ω dΩ

Ω\Γ

KΩ =

Ω\Γ

Rj =

Z

(26)

B TΓj τ dΓj

Γj

F =

Z

Ω\Γ

T¯

Φ b dΩ +

Z

ΦT τ¯ dΓτ

Γτ

Smarter finite element formulations, like the extended or generalized ones [36,37], have been recently formulated to simulate mixed-mode crack growth in homogeneous solids, see e.g. [27, 38, 39]. These methodologies allow cracks to propagate not only along interelement edges, but also inside the elements; possible constraints imposed by the mesh layout on crack trajectories, evidenced e.g. in [40], can be therefore alleviated. When dealing with delamination in layered continua, where debonding occurs only along the a-priori known interlaminar surfaces, crack description looks simple and the aforementioned feature of the extended finite element method looses much of its advantages.

Failure of Layered Composites Subject to Impacts

2.4.

107

Time Integration

In our previous works [11, 15] it was shown that the time integration scheme can strongly affect the stability of the filtering procedure and, therefore, the accuracy of model parameter estimates. In case of impact loadings, which cause the propagation of shock waves inside the composite, the time marching algorithm has to dump the spurious high frequency oscillations linked to space discretization. Otherwise, the numerically computed displacement and velocity fields do not prove reliable enough to be compared to the experimental data. We adopt here the explicit α−method [41, 42] to advance in time the solution of the equations of motion (25), see also [19]. After having partitioned the time interval of interest Nt −1 according to [t0 tN ] = ∪i=0 [ti ti+1 ], at the end of the generic time step [ti ti+1 ] the solution to (25) is obtained according to the following predictor-integrator-corrector splitting: • predictor: 1 ˜ i+1 =ui + ∆t u˙ i + ∆t2 ( − β)¨ u ui 2 ˜˙ i+1 =u˙ i + ∆t(1 − γ)¨ ui u

(27) (28)

where ∆t = ti+1 − ti ; • explicit integrator:

¨ i+1 = M −1 F i+1+α − (1 + α) K u ˜ i+1 + u

where: F i+1+α = F (ti + (1 + α)∆t); R T B Γj τ˜ i+1 dΓj ;

X

Rji

j

˜ j + α Kui + R i+1

=

R

Γj

B TΓj τ i dΓj

X j

Rji

(29) j ˜ and Ri+1 =

Γj

• corrector: ¨ i+1 ui+1 =˜ ui+1 + ∆t2 β u ˜ ¨ i+1 u˙ i+1 =u ˙ i+1 + ∆tγ u

(30) (31)

In the above equations α, β and γ are algorithmic coefficients. To get a non-oscillatory velocity field, α = −0.3 has been adopted in all the forthcoming simulations; furthermore, β and γ have been finely tuned around the values allowing second-order accuracy in linear elasto-dynamics. To ensure accuracy of the filtering procedure, the time step size ∆t has been always set so as to fulfill the Courant condition in the bulk of the composite. Moreover, to speed up the explicit integrator phase (29), the mass matrix M has been diagonalized by means of a standard row-sum lumping procedure [42].

108

Stefano Mariani

Account taken of the explicit format of the integrator stage, the space-time discretized equations of motion of the laminate (state equations) can be formally written: ui+1 (32) z i+1 = u˙ i+1 = f zi (z i ) ¨ i+1 u where z is the structural state vector, and mapping f z turns out to be nonlinear because of the softening interface behavior.

3. 3.1.

Constrained Sigma-point Kalman Filtering Parameter Identification via Joint Kalman Filtering

According to a standard methodology [43], the calibration of constitutive laws can be pursued by Kalman filtering if a state vector x is obtained by joining the structural state vector z (see Eq. 32) with a vector ϑ gathering all the model parameters to be tuned. At time ti this can be written: zi xi = (33) ϑi While the current structural state z is always at least partially observed, model parameters to be identified can not be directly measured; by joining z and ϑ, state tracking can consistently improve model calibration. In case of irreversible constitutive laws, internal state variables must be gathered by x too, see e.g. [12, 19]. Allowing for model and measurement errors, the state-space model describing the evolution within the time interval [ti ti+1 ] of the joint state vector and its link with observations turns out to be: ( xi+1 = f i (xi ) + v i (34) = Hxi + wi yi where: y is the observation vector, which collects the measured components of the state vector; v is the process noises; w is the measurement noise. v, w are assumed to be additive, uncorrelated white and Gaussian processes, with zero mean and covariances V and W [44, 45]. Since z is defined according to Eq. (32), the observation equation in (34) shows up as a linear relation between y and x. On the contrary, the interface behavior renders the evolution equation f nonlinear. By way of the EKF [12, 46], within the time step the nonlinear mapping f is expanded in Taylor series, up to the first order, around the current estimates of the state vector and of model parameters. Bounds on the required accuracy of the initialization of x, and on the statistics of noises v and w to assure filter stability were provided for linear systems in [47] and, more recently, for nonlinear systems in [48]. Even in the absence of filter instabilities, the softening response of the interlaminar surfaces does not always guarantee the achievement of an accurate model calibration, see [15, 19].

Failure of Layered Composites Subject to Impacts

109

Table 1. Sigma-point Kalman filter. • Initialization at t0 : ˆ 0 =E[x0 ] x ˆ 0 ) (x0 − x ˆ 0 )T ] P 0 =E[(x0 − x • At ti , for i = 0, ..., N 1. Predictor phase: χ ˆi,j =ˆ xi + ∆χi,j

j = 0, ..., Nχ

ˆ− ˆ i,j ) χ i+1,j =f i (χ ˆ− x i+1 P− i+1

=

Nχ X

ˆ− ωj χ i+1,j

j=0 =R− i+1

+V

where R− i+1

=

Nχ X j=0

T ˆ− ˆ− ˆ− ˆ− χ ωj χ i+1 i+1 i+1,j − x i+1,j − x

2. Corrector phase: U ˆ− ˆ i =ˆ x x− i i + Gi y i − H x

− U P i =P − i − Gi HRi

where − T T GU HR− i =Ri H i H +W

−1

To improve the results when nonlinearities become dominant, the SPKF has been recently proposed [16, 49–51]. At the beginning of the time step, the probability distribution of x is deterministically sampled through a set of sigma-points χ ˆj , j = 0, ..., Nχ . These sigma-points are then allowed to evolve according to the nonlinear mapping f . The statistics of x at the end of the time step are finally obtained through a proper weighted averaging scheme [18]. This filtering procedure is detailed in Table 1, where E[2] represents the expected value of 2. The number of sigma-points and their location in the state vector space are accurately chosen, so as to achieve high accuracy in the estimated probability distribution of x at the end of each time step; when compared to the EKF, a better performance of the SPKF, also in terms of model calibration, is therefore expected [16]. The enhanced accuracy of the

110

Stefano Mariani

SPKF is discussed next; even though these results have been already presented elsewhere, they are here collected to show how possible constraints on parameter estimates, not dealt with by the standard SPKF, can be managed.

3.2.

Accuracy of a Constrained Sigma-point Transformation

In this Section we focus on the time interval [ti ti+1 ], but we avoid using indexes i and i + 1 to simplify the notation. Let x be a random vector, featuring at the beginning of the time step mean x ˆ and covariance P . We conceive x as the sum of the mean x ˆ and a zero-mean disturbance ∆x = x − x ˆ. If x undergoes a nonlinear transformation, governed by a mapping f analytic everywhere so that it can be expanded in Taylor series about x ˆ, at the end of the time step we get: ∞ X 1 n x = f (x) = f (ˆ x + ∆x) =f (ˆ x) + D n! ∆x n=1 −

(35)

n in the series expansion is: where, with a slight abuse in notation, the n−th order term D∆x

n D∆x

≡

!n Nx X ∂f ∆xℓ ∂xℓ x=ˆ x

(36)

ℓ=1

Nx being the number of components of the state vector x. Since the derivatives of f in (36) are evaluated at x = x ˆ, they are not random variables. The expected value of x− therefore reads: "∞ # X 1 x ˆ− = E[x− ] =E [f (ˆ x)] + E Dn n! ∆x n=1 (37) ∞ X 1 n =f (ˆ x) + E D∆x n! n=1

The relevant error covariance matrix is: h T i P − =E x− − x ˆ − x− − x ˆ− ! ∞ X 1 n n D∆x − E D∆x =E n! n=1

∞ X m 1 m D∆x − E D∆x m!

m=1

∞ X ∞ i X n h m T i 1 1 h n m T E D∆xD∆x − E D∆x E D∆x = n! m!

!T

(38)

n=1 m=1

Now, let us suppose to sample the probability distribution of x through a set of sigmapoints χ ˆj , j = 0, ..., Nχ , chosen around the current mean x ˆ according to: χ ˆj = x ˆ + ∆χj ,

j = 0, ..., Nχ

(39)

Failure of Layered Composites Subject to Impacts

111

where the terms ∆χj need to be determined. Similarly to x, within the time step each sigma-point undergoes the transformation: χ ˆ− j

∞ X 1 n = f (χ ˆj ) = f (ˆ x) + D n! ∆χj n=1

(40)

where: Dn ∆χj

≡

!n Nx X ∂f ∆χj ℓ ∂xℓ x=ˆ x

(41)

ℓ=1

At the end of the time step, the information in the evolved sigma-points are collected via a weighted averaging procedure to obtain: x ˆ− SPT

=

Nχ X

ωj χ ˆ− j

j=0

=

Nχ X j=0

(42)

Nχ ∞ X X 1 ωj D n ωj f (ˆ x) + ∆χj n!

n=1

j=0

where ωj are the weights of the sigma-point transformation relevant to the mean of x. The corresponding error covariance matrix is given by: P− SPT

=

Nχ X j=0

=

Nχ X j=0

T − − − ωj⋆ χ ˆ− − x ˆ − x ˆ χ ˆ SPT SPT j j

T Nχ Nχ ∞ ∞ X X X X 1 1 n D m ωj⋆ D ∆χj − ωr D n ωs D m ∆χr ∆χj − ∆χs n! m! n=1 m=1 r=0

s=0

(43)

where ωj⋆ are the weights of the sigma-point transformation relevant to the covariance of x. If x is a Gaussian random vector, its probability distribution is symmetric with respect n , n = 1, 3, 5, ..., are zero. To be to the mean x ˆ; therefore, all the odd central moments D∆x compliant with this condition, couples of sigma-points are symmetrically placed around x ˆ, according to [16]: ∆χ0 ∆χk ∆χ Nχ +k 2

=0 √ = +ψ P 1k √ = −ψ P 1k

k = 1, ...,

Nχ 2

(44)

√ Here: P represents the square root of matrix P , computed e.g. through a Cholesky factorization; ψ is a scaling parameter; 1k is a unit vector aligned with component k in the

112

Stefano Mariani

state vector space. The series expansions (37) and (42) agree up to third order if: P Nχ j=0 ωj = 1 P χ 1 N j=0 ωj D ∆χj = 0 2 PNχ 2 j=0 ωj D ∆χj = E D∆x PNχ ωj D 3 = 0

(45)

∆χj

j=0

To simplify the matter, let us assume ωj = ω for j = 1, ..., Nχ ; relations involving the first and third order terms in (45) are then automatically satisfied. Relations involving the zeroth and second order terms in (45) then furnish: ( ω0 + Nχ ω = 1 (46) 2ψ 2 ω = 1 A further condition to set ω0 , ω and ψ can be furnished by matching the diagonal entries of the fourth order terms (kurtoses) in (37) and (42). This leads to [19]: ω0 = 1 −

Nχ , 6

1 ω= , 6

ψ=

√

3

(47)

Here we propose an alternative condition to determine ω0 , ω and ψ, partially exploiting the features of the so-called scaled unscented transformation [52]. Let us assume that model parameters have to satisfy the constraints: ϑm ≤ ϑ ≤ ϑM

(48)

where ϑm and ϑM respectively gather the minimum and maximum (if any) allowed values of model parameters. This requirement must be fulfilled by each sigma-point χ ˆ− j , j = ˆ (and, therefore, 0, ..., Nχ . For j = 0 the conditions (48) are automatically satisfied, since x ˆ is computed at the end of the previous time step by averaging sigma-points all fulfilling ϑ) the constraints. Further, if ϑ = B ϑ x, B ϑ being a Boolean matrix, conditions (48) are satisfied by all the sigma-points if: ( ) M −ϑ ˆℓ ϑˆℓ − ϑm ϑ Nχ ℓ ℓ ; ℓ = 1, ..., Nϑ (49) ψ ≤ min , , k = 1, ..., ℓ ℓ 2 ak ak √ where ak = B ϑ P 1k , and Nϑ is the√number of model parameters in ϑ. In the forthcoming examples, we initially assume ψ = 3 (according to what reported in 47) and reduce its value if necessary, according to relation (49). ⋆ As for the error covariance matrix P − SPT , by letting ωj = ωj = ω for j = 1, ..., Nχ , we get: Nχ Nχ Nχ ∞ X ∞ X X X X 1 1 T ⋆ m T P− ωk D m ωj D n ωj D n ∆χk ∆χj D ∆χj + (ω0 + Nχ ω − 2) ∆χj SPT = n! m! n=1 m=1 j=0

j=0

k=0

(50)

Failure of Layered Composites Subject to Impacts

113

In case of Gaussian random variables, independently of the value of ω0⋆ , (38) and (50) agree up to the third order. Weight ω0⋆ can be set by matching part of the fourth order terms T (specifically those involving D 2∆χj D 2∆χk in 50), thereby obtaining (see also [52]): ω0⋆ = 4 −

Nχ − ψ2 ψ2

(51)

In what precedes we have assumed the mapping f to be analytic everywhere in the x space. If f is not differentiable, low order terms of the Taylor series expansions of mean and covariance get affected. It is difficult to quantify the discrepancies with respect to the analytic case, because they depend on whether the sigma-points sample the loci of nondifferentiability. However, it can be generally said that the order of accuracy is detrimentally affected.

4.

Results

To assess the performances of the proposed filtering approach in calibrating the interlaminar constitutive law while detecting impact-induced delamination, we first study a simple problem consisting of a two-layer composite stricken by a homogeneous impactor. Hence, two different impact tests on GRP composites [14, 53] are considered to mainly show the accuracy in detecting delamination in real-time. In all the cases, it is assumed that the contact between specimen and impactor is perfect (i.e. distributed all over their approaching surfaces) and that failure of the laminate occurs because of the propagation of dilatational plane waves in the through-the-thickness direction: the interlaminar surfaces are therefore subject to pure mode I loading.

4.1.

Pseudo-experimental Testings

As a starting benchmark, a pseudo-experimental testing condition is conceived. The pseudo-experimental response of the laminate to the impact loading has been computed by adding a white noise (of assigned variance) to sampled outcomes of finite element analyses. Even though this approach is sometimes criticized, being not clear whether one is testing with it the filtering approach or its implementation, it helps in getting insights into the performance of the filter in terms of stability and convergence rate. Indeed, calibration of interlaminar constitutive models may become difficult if delamination occurs almost instantaneously: the filter has to be highly sensitive to model parameters to promptly react to the information conveyed by measurements. This requires a careful setting of filter parameters, like P 0 and V . It is worth mentioning that, to further complicate the problem, the effects of the shape of the tensile envelope of interlaminar laws (at assigned strength and toughness) on the overall response of a laminate subject to impacts have not been thoroughly understood yet: depending on the loading and boundary conditions, on the composite geometry and on the stacking sequence, in some circumstances the shape affects the response, whereas in others it does not [54]. The capabilities of the SPKF are therefore first assessed through a simple test: a twolayer composite is stricken by a homogeneous impactor. The laminae and the impactor are

114

Stefano Mariani

Figure 5. impact on a two-layer composite. Space-time diagram (the vertical dashed line here represents the possibly debonding surface when a brittle, homogeneous material is subject to the same impact). assumed to be isotropic and elastic, featuring Young’s modulus E = 10 GPa, Poisson’s ratio ν = 0.35 and mass density ̺ = 1500 kg/m3 (see also [11]). Each lamina and the impactor are 0.75 mm in thickness. Target mechanical properties of the interlaminar surfaces are assumed: 2K =277.09 (N/mm3 ) τM =75 G =0.15

(MPa)

(52)

(N/mm)

According to the space-time diagram of Figure 5, failure can occur only along the interlaminar surface because of the interaction of the two release waves propagating inwards from the free surfaces of impactor and specimen. Two different values of the velocity v of the impactor are considered. In a first case v = 10.19 m/s leads to the propagation in the through-the-thickness direction of a compressive/tensile wave of amplitude τ¯ = 50 MPa, which does not cause interface failure. In a second case v = 20.38 m/s causes laminate failure, i.e. whole delamination, because of the propagation of a compressive/tensile wave of amplitude τ¯ = 100 MPa. Outcomes of the two tests are respectively reported in Figures 6 and 7, in terms of time evolution of the free surface velocity velocity u˙ r at the rear laminate surface, of the opening displacement discontinuity [u] and of the normal traction τ (here and in what follows the subscript n has been dropped to simplify the notation). Results are shown for all the constitutive models described in Section 2.2., having assumed q = 1 for the modified exponential interface law (17). For comparison purposes, the response of an interface-free specimen is reported too; in such a case, the purely elastic behavior of the material leads to the propagation of sharp fronts of a shock wave. If delamination is not incepted (¯ τ = 50 MPa), the response is almost independent of the shape of the interface law. Only in the presence of an interface that behaves according to the exponential model, the pre-peak nonlinearity of the constitutive law (see Figure 2(a))

Failure of Layered Composites Subject to Impacts

115

(a)

(b)

(c)

Figure 6. impact on a two-layer composite, τ¯ = 50 MPa. Effects of the interlaminar laws on the time evolution of (a) the free surface velocity u˙ r , of (b) the displacement discontinuity [u] and (c) relevant traction τ along the interface. leads to a larger opening [u] of the interlaminar surface when subject to a tensile stress. For any constitutive model, the signature of the interface is shown in Figure 6(a) by the delay in the sudden changes of u˙ r with respect to the reference, interface-free solution. This delay, which grows in time, is caused by the compliance of the interface, that is additional to the bulk one. In case of failure (¯ τ = 100 MPa), the free surface velocity u˙ r is affected by the interface model only when the waves, traveling across the interlaminar surface while softening is taking place, reach the rear surface; this occurs in the present case around 1µs after the impact, see Figure 7(a). After failure, the rear lamina detaches from the front one and freely flies off, as testified by the diverging [u] history in Figure 7(b). Part of the shock waves then get confined inside the back lamina: this explains the subsequent doubling of the drops in the u˙ r evolution. It is worth noting that the time elapsed between softening

116

Stefano Mariani

(a)

(b)

(c)

Figure 7. impact on a two-layer composite, τ¯ = 100 MPa. Effects of the interlaminar laws on the time evolution of (a) the free surface velocity u˙ r , of (b) the displacement discontinuity [u] and (c) relevant traction τ along the interface. inception (t ∼ = 0.72 µs) and whole failure of the interface (t ∼ = 0.9 µs), see Figure 7(c), is very short; only the information on this failure event, constituting the so-called pull-back signal (PBS), conveyed by the shock waves to the free laminate surface, can be used by the filter to calibrate the interface law. The effects on the PBS of the shape of the tensile envelope and of the strength τM and toughness G values need to be assessed. In the absence of any dissipation mechanisms, in this test the free surface velocity u˙ r would drop to zero at t = 0.917 µs (see Figure 6(a)); in case of delamination, the minimum attained velocity after the arrival of the unloading tensile wave and the shape of the PBS do furnish information on the interface response. To understand the roles of interface law, strength and toughness, the results of a parametric analysis are shown in Figure 8: for any interface model, τM and G are varied by 20% at most with respect to the target values (52). The piecewise linear and linear-exponential

Failure of Layered Composites Subject to Impacts

(a)

(b)

(c)

(d)

(e)

(f)

117

Figure 8. impact on a two-layer composite, τ¯ = 100 MPa. Effects of the interface strength τM (left column) and toughness G (right column) on the pull-back signal. (a-b) piecewise linear law (12); (c-d) linear-exponential law (13); (e-f) exponential law (14).

118

Stefano Mariani

laws, having a common initial elastic phase in tension, lead to a common descending branch in the PBS. At variance, the local tangent stiffness of the exponential law in the hardening phase is affected by τM and G: the slope of the descending branch of the PBS is therefore affected by τM and G too. Independently of the interface law, τM turns out to affect the starting stage of debonding, whereas G affects its tail and the time needed to complete it; this is clearly evidenced by the PBS, since τM modifies the minimum attained velocity, whereas G influences only the ascending branch with no effects on the pull-back velocity. From a model calibration perspective, it is clear that the SPKF has chances to improve parameter estimates only in the time interval 0.9 ≤ t ≤ 1.2 µs. It is therefore hard to figure out from the previous plots whether the effects of tensile envelope, τM and G can be actually interpreted by the filter to improve model calibration. The performances of the SPKF are hence tested here not only looking at parameter estimates, but also checking its capability to detect whether a laminate is failing and, in case of delamination, where it actually takes place. Typical results of the filtering procedure are depicted in Figures 9 and 10; in this case the pseudo-experimental data, which consist in the free surface velocity alone, have been supposed very accurate, featuring a standard deviation δ = 0.33 m/s (the measurement error covariance matrix W becomes scalar-valued, with entry W = δ 2 ). As far as the process covariance matrix V is concerned, in case of pseudo-experimental testing it can be assumed to be vanishing, since the filter employs the same structural model adopted to get the pseudo-experimental data. Components of P 0 instead need to be finely tuned to enhance filter convergence [11, 15]. Figure 9 shows the obtained estimates of τM and G as a function of their initial guess in ˆ 0 (here respectively denoted by τM,0 and G0 ), for all the interface models. These estimates x evolve from τM,0 and G0 once the PBS is processed by the filter; after that, they become stationary. The tracked state of the laminate is shown in Figure 10 in terms of predicted interface opening [u] and free surface velocity u˙ r . Knowing the target response of the composite to the impact, here denoted by the dashed lines, allows to certify stability and convergence of the SPKF, no matter if displacement is diverging in a part of the system and what kind of interface constitutive law has been adopted. It can be seen that estimates get enhanced as soon as the filter senses the PBS: in fact, the sudden changes in the estimate of [u] show up only while processing the PBS, starting from t ∼ = 0.9 µs. These outcomes testify that the SPKF is very efficient in tracking the state of the laminate, i.e. in understanding whether the structure is failing or not. Model calibration is instead less accurately accomplished: independently of the interface law, τM is quite precisely estimated, provided the initial guess τM,0 is not too far from the target value, whereas G can be hardly inferred. These conclusions are in agreement with the results of the parametric analysis: while τM affects the whole PBS, G affects only its ascending branch. Therefore, filtering out from u˙ r the effects of G alone turns out to be extremely difficult. In case of a much higher scattering of pseudo-experimental data (δ = 3.3 m/s), see Figure 11, results loose accuracy as for the calibration task. Contrariwise, state tracking maintain accuracy: even though measurements contain poor information, the SPKF is again able to provide the evolution of the free surface velocity in the PBS.

Failure of Layered Composites Subject to Impacts

(a)

(b)

(c)

(d)

(e)

(f)

119

Figure 9. impact on a two-layer composite, τ¯ = 100 MPa (W=10−1 m2 /s2 ). Effects of the initialization values τM,0 and G0 on the converged estimates of τM (left column) and G (right column). (a-b) piecewise linear law; (c-d) linear-exponential law; (e-f) exponential law.

120

Stefano Mariani

(a)

(b)

(c)

(d)

(e)

(f)

Figure 10. impact on a two-layer composite, τ¯ = 100 MPa (W=10−1 m2 /s2 ). Evolution in time of interface opening [u] (left column) and free surface velocity u˙ r (right column), and comparison among tracked state (orange squares), actual state (dashed lines) and pseudoexperimental data (blue circles). (a-b) piecewise linear law; (c-d) linear-exponential law; (e-f) exponential law.

Failure of Layered Composites Subject to Impacts

(a)

(b)

(c)

(d)

(e)

(f)

121

Figure 11. impact on a two-layer composite, τ¯ = 100 MPa (W=10 m2 /s2 ). Evolution in time of interface opening [u] (left column) and free surface velocity u˙ r (right column), and comparison among tracked state (orange squares), actual state (dashed lines) and pseudoexperimental data (blue circles). (a-b) piecewise linear law; (c-d) linear-exponential law; (e-f) exponential law.

122

Stefano Mariani

(a)

(b)

Figure 12. impact on a 7-layer composite [53]. (a) space-time diagram (the vertical dashed line here represents the possibly debonding surface when a brittle, homogeneous material is subject to the same impact), and (b) experimentally measured free surface velocity.

4.2.

Actual Experimental Testings

To finally check the performances of the SPKF when dealing with multi-layered composites, we consider two of the experiments reported in [53] and [14]. In the first experiment (experiment FY06001 in [53]), the specimen is a 7-layer composite plate; each lamina is 1.37 mm in thickness, and is made of a balanced 5-harness satin weave E-glass and LY564 epoxy. The wave speed in the through-the-thickness direction is 3.34 km/s, while the mass density is ̺ = 1885 kg/m3 [53]. This laminate was subject to a plane impact, stricken by an aluminum impactor (12.5 mm thick) flying at velocity v = 71 m/s. The relevant space-time diagram is shown in Figure 12, along with the free surface velocity profile measured via a velocity interferometer for any reflector (VISAR). Account taken of the high accuracy of the experimentally measured u˙ r , the identification procedure have furnished the results reported in Figure 13 in terms of time evolution of estimates of τM and G as a function of their initialization values within the domain: Cϑ = {50 ≤ τM,0 ≤ 250 (MPa), 0.5 ≤ G0 ≤ 2.5 (N/mm)}

(53)

Failure of Layered Composites Subject to Impacts

(a)

(b)

(c)

(d)

(e)

(f)

123

Figure 13. impact on a 7-layer composite [53]. Evolution in time of the estimated values of τM (left column) and G (right column). (a-b) piecewise linear law; (c-d) linear-exponential law; (e-f) exponential law.

124

Stefano Mariani

(a)

(b)

(c)

(d)

(e)

(f)

(g)

Figure 14. impact on a 7-layer composite [53]. Evolution in time of (a) free surface velocity u˙ r and (b-g) estimated interface openings [u]1 − [u]6 .

Failure of Layered Composites Subject to Impacts

125

(a)

(b)

Figure 15. impact on a 11+11-layer composite [14]. (a) space-time diagram (the vertical dashed line here represents the possibly debonding surface when a brittle, homogeneous material is subject to the same impact), and (b) experimentally measured free surface velocity. Converged estimates of τM are in good agreement with the spall strength of 119.5 MPa reported in [53]; on the other hand, final estimates of G are well representative for this kind of composites. Figure 14 reports the estimated state of the specimen: the capability to track the measured free surface velocity and to foresee delamination along the third interlaminar surface away from the impact plane, is evidenced. This latter result, allowing also for wave dispersion caused by interlaminar surfaces and inner inhomogeneities of the composite, well agrees with the state-space diagram of Figure 12(a). In the second experiment (experiment 1 in [14]), a GRP specimen, 7.02 mm thick, is backed by another GRP plate, 6.91 mm thick; both laminates are made of 11 plies. The wave speed in the through-the-thickness direction now amounts to 3.19 km/s, and the mass density to ̺ = 1867 kg/m3 [14]. The specimen is stricken by a 5-layer GRP flyer, 2.96 mm in thickness, flying at velocity v = 85 m/s. The corresponding space-time diagram, and the free surface velocity profile measured via a VISAR are reported in Figure 15. Because of the test set-up, the release waves interact causing delamination inside the back plate.

126

Stefano Mariani

(a)

(b)

(c)

(d)

(e)

(f)

(g)

(h)

(i)

(j)

(k)

Figure 16. Impact on a 11+11-layer composite [14]. Evolution in time of (a) free surface velocity u˙ r and (b-k) estimated interface openings [u]1 − [u]10 in the back plate.

Results of the filtering process are reported in Figure 16 is terms of tracked free surface velocity and estimated displacement jumps along all the interfaces inside the back plate (sequence starts at the specimen-back plate contact surface). These estimations turn out once again to be independent of the interface law and of the initialization values of τM and

Failure of Layered Composites Subject to Impacts

127

G inside the domain: Cϑ = {25 ≤ τM,0 ≤ 100 (MPa), 0.1 ≤ G0 ≤ 0.6 (N/mm)}

(54)

While the free surface velocity is accurately tracked, delamination is foreseen to take place along the 7-th interlaminar surfaces, in agreement with the results of [11, 14]. As far as model calibration is concerned, outcomes turn out to be qualitatively in agreement with those already reported for the previous tests.

5.

Conclusion

In this Chapter we have addressed some issues related to constitutive modeling and parameter identification in finite element simulations of layered composites subject to impacts. Assuming the impact energy to be high enough to cause damage spreading inside the interlaminar resin-enriched phases, but not high enough to result in penetration of the impactor accompanied by intralaminar damage, a numerical scheme for structural-level analyses has been revised. Within this scheme the laminae are assumed to behave elastically, whereas dissipation mechanisms are lumped onto zero-thickness interlaminar surfaces. Along these interlaminar surfaces strength reduction, eventually leading to delamination, is governed by softening interface constitutive laws linking tractions to displacement jumps. Interface laws are known to be difficult to calibrate, since direct testing on a single interlaminar phase can not be devised. Here we have offered a sigma-point Kalman filtering approach to estimate uncertain model parameters of the aforementioned interface laws. This technique outperforms most of the customarily adopted ones, since it efficiently deals with nonlinearities, which are a result of interlaminar strength degradation in the case under study. The performances of the filtering procedure have been assessed through pseudoexperimental testings on a two-layer composite, and through real testings on multi-layer glass fiber reinforced plastic composites. It has been shown that the state of the composite, including delamination inception and growth, is always tracked with a noteworthy level of accuracy. Due to the fast failure events, model calibration is instead less accurately performed and sometimes requires initialization values of uncertain model parameters to be appropriately chosen to avoid biased estimates.

References [1] S. Abrate. Impact on composite structures. Cambridge University Press, 1998. [2] H.D. Espinosa, S. Dwivedi, P.D. Zavattieri, and G. Yuan. A numerical investigation of penetration in multilayered material/structure systems. International Journal of Solids and Structures, 35:2975–3001, 1998. [3] O. Allix and P. Ladev´eze. Interlaminar interface modelling for the prediction of delamination. Composite Structures, 22:235–242, 1992.

128

Stefano Mariani

[4] A. Corigliano. Formulation, identification and use of interface elements in the numerical analysis of composite delamination. International Journal of Solids and Structures, 30:2779–2811, 1993. [5] A. Corigliano and O. Allix. Some aspects of interlaminar degradation in composites. Computer Methods in Applied Mechanics and Engineering, 185:203–224, 2000. [6] A. Corigliano and S. Mariani. Simulation of damage in composites by means of interface models: parameter identification. Composites Science and Technology, 61:2299– 2315, 2001. [7] G. Alfano and M.A. Crisfield. Finite element interface models for the delamination analysis of laminated composites: mechanical and computational issues. International Journal for Numerical Methods in Engineering, 50:1701–1736, 2001. [8] A. Corigliano. Damage and fracture mechanics techniques for composite structures. In I. Milne, R.O. Ritchie, and B. Karihaloo, editors, Comprehensive Structural Integrity, volume 3, chapter 9, pages 459–539. Elsevier Science, 2003. [9] A. Corigliano and S. Mariani. Parameter identification of a time-dependent elasticdamage interface model for the simulation of debonding in composites. Composites Science and Technology, 61:191–203, 2001. [10] A. Corigliano and S. Mariani. Identification of a constitutive model for the simulation of time-dependent interlaminar debonding processes in composites. Computer Methods in Applied Mechanics and Engineering, 191:1861–1894, 2002. [11] S. Mariani and A. Corigliano. Impact induced composite delamination: state and parameter identification via joint and dual extended Kalman filters. Computer Methods in Applied Mechanics and Engineering, 194:5242–5272, 2005. [12] S. Bittanti, G. Maier, and A. Nappi. Inverse problems in structural elastoplasticity: a Kalman filter approach. In A. Sawczuk and G. Bianchi, editors, Plasticity today. Modelling, Methods and Applications, pages 311–329. Elsevier Applied Science Publishers, 1984. [13] A. Corigliano, S. Mariani, and B. Orsatti. Identification of Gurson-Tvergaard material model parameters via Kalman filtering technique - I. Theory. International Journal of Fracture, 104:349–373, 2000. [14] H.D. Espinosa, S. Dwivedi, and H.-C. Lu. Modeling impact induced delamination of woven fiber reinforced composites with contact/cohesive laws. Computer Methods in Applied Mechanics and Engineering, 183:259–290, 2000. [15] A. Corigliano and S. Mariani. Parameter identification in explicit structural dynamics: performance of the extended Kalman filter. Computer Methods in Applied Mechanics and Engineering, 193:3807–3835, 2004.

Failure of Layered Composites Subject to Impacts

129

[16] S.J. Julier, J. Uhlmann, and H.F. Durrant-Whyte. A new method for the nonlinear transformation of means and covariances in filters and estimators. IEEE Transactions on Automatic Control, 45:477–482, 2000. [17] T. Lefebvre, H. Bruyninckx, and J. De Schutter. Kalman filters for nonlinear systems: a comparison of performance. International Journal of Control, 77:639–653, 2004. [18] K. Ito and K. Xiong. Gaussian filters for nonlinear filtering problems. IEEE Transactions on Automatic Control, 45:910–927, 2000. [19] S. Mariani and A. Ghisi. Unscented Kalman filtering for nonlinear structural dynamics. Nonlinear Dynamics, 49:131–150, 2007. [20] A. Corigliano, S. Mariani, and A. Pandolfi. Numerical modeling of rate-dependent debonding processes in composites. Composite Structures, 61:39–50, 2003. [21] A. Corigliano, S. Mariani, and A. Pandolfi. Numerical analysis of rate-dependent dynamic composite delamination. Composites Science and Technology, 66:766–775, 2006. [22] R. Lund and J. Fish. Space-time multiscale laminated theory. International Journal of Multiscale Computational Engineering, 2:26–47, 2004. [23] S. Mariani, A. Pandolfi, and R. Pavani. Coupled space-time multiscale simulations of dynamic delamination tests. Materials Science, 23:509–519, 2005. [24] R.R. Talreja Y.W. Kwon, D.H. Allen, editor. Multiscale Modeling and Simulation of Composite Materials and Structures. Springer, 2007. [25] G.T. Camacho and M. Ortiz. Computational modelling of impact damage in brittle materials. International Journal of Solids and Structures, 33:2899–2938, 1996. [26] Y. Arun Roy and R.H. Dodds. Simulation of ductile crack growth in thin alluminum panels using 3-D surface cohesive elements. International Journal of Fracture, 110:21–45, 2001. [27] S. Mariani and U. Perego. Extended finite element method for quasi-brittle fracture. International Journal for Numerical Methods in Engineering, 58:103–126, 2003. [28] C. Comi and S. Mariani. Extended finite element simulation of quasi-brittle fracture in functionally graded materials. Computer Methods in Applied Mechanics and Engineering, 196:4013–4026, 2007. [29] S. Li, M.D. Thouless, A.M. Waas, J.A. Schroeder, and P.D. Zavattieri. Mixed-mode cohesive-zone models for fracture of an adhesively bonded polymer matrix composite. Engineering Fracture Mechanics, 73:64–78, 2006. [30] J.H. Rose, J. Ferrante, and J.R. Smith. Universal binding energy curves for metals and bimetallic interfaces. Physical Review Letters, 47:675–678, 1981.

130

Stefano Mariani

[31] J.H. Rose, J.R. Smith, and J. Ferrante. Universal features of bonding in metals. Physical Review B, 28:1835–1845, 1983. [32] X.-P. Xu and A. Needleman. Numerical simulation of fast crack growth in brittle solids. Journal of the Mechanics and Physics of Solids, 42:1397–1434, 1994. [33] A. Needleman and A.J. Rosakis. The effect of bond strength and loading rate on the conditions governing the attainment of intersonic crack growth along interfaces. Journal of the Mechanics and Physics of Solids, 47:2411–2449, 1999. [34] C.M. Landis, T. Pardoen, and J.W. Hutchinson. Crack velocity dependent toughness in rate dependent materials. Mechanics of Materials, 32:663–678, 2000. [35] O. C. Zienkiewicz and R. L . Taylor. The finite element method, volume II. McGrawHill, London, 1989. [36] N. Mo¨es, J. Dolbow, and T. Belytschko. A finite element method for crack growth without remeshing. International Journal for Numerical Methods in Engineering, 46:131–150, 1999. [37] T. Strouboulis, K. Copps, and I. Babuˇska. The generalized finite element method. Computer Methods in Applied Mechanics and Engineering, 190:4081–4193, 2001. [38] G.N. Wells and L.J. Sluys. A new method for modelling cohesive cracks using finite elements. International Journal for Numerical Methods in Engineering, 50:2667– 2682, 2001. [39] C. Comi, S. Mariani, and U. Perego. An extended FE strategy for transition from continuum damage to mode I cohesive crack propagation. International Journal for Numerical and Analytical Methods in Geomechanics, 31:213–238, 2007. [40] M. Jirasek and T. Zimmerman. Embedded crack model: II. Combination with smeared cracks. International Journal for Numerical Methods in Engineering, 50:1291–1305, 2001. [41] H.M. Hilber, T.J.R. Hughes, and R.L. Taylor. Improved numerical dissipation for time integration algorithms in structural dynamics. Earthquake Engineering and Structural Dynamics, 5:283–292, 1977. [42] T.J.R. Hughes. The finite element method. Linear static and dynamic finite element analysis. Dover Publications, 2000. [43] L. Ljung. System identification. Theory for the user. Prentice Hall, second edition, 1999. [44] A. Gelb. Applied optimal estimation. The M.I.T. Press, 1974. [45] E.A. Wan and A.T. Nelson. Dual extended Kalman filter methods. In S. Haykin, editor, Kalman filtering and neural networks, pages 123–173. John Wiley & Sons, Inc., 2001.

Failure of Layered Composites Subject to Impacts

131

[46] R. E. Kalman and R. S. Bucy. New results in linear filtering and prediction theory. ASME Journal of Basic Engineering, 83D:95–108, 1961. [47] L. Ljung. Asymptotic behavior of the extended Kalman filter as a parameter estimator for linear systems. IEEE Transactions on Automatic Control, AC-24:36–50, 1979. [48] K. Reif, S. G¨ unther, E. Yaz, and R. Unbehauen. Stochastic stability of the discretetime extended Kalman filter. IEEE Transactions on Automatic Control, 44:714–728, 1999. [49] S.J. Julier and J.K. Uhlmann. A general method for approximating nonlinear transformations of probability distributions. Technical report, RRG, Department of Engineering Science, University of Oxford, 1996. [50] S.J. Julier, J. Uhlmann, and H.F. Durrant-Whyte. A new approach for filtering nonlinear systems. In Proceedings of the American Control Conference, pages 1628–1632, Seattle, June 1995. [51] E.A. Wan and R. van der Merwe. The unscented Kalman filter. In S. Haykin, editor, Kalman filtering and neural networks, pages 221–280. John Wiley & Sons, Inc., 2001. [52] S.J. Julier. The scaled unscented transformation. In Proceedings of the American Control Conference, volume 6, pages 4555–4559, Anchorage, May 2002. [53] F. Yuan, L. Tsai, V. Prakash, A.M. Rajendran, and D.P. Dandekar. Spall strength of glass fiber reinforced polymer composites. International Journal of Solids and Structures, 44:7731–7747, 2007. [54] G. Alfano. On the influence of the shape of the interface law on the application of cohesive-zone models. Composites Science and Technology, 66:723–730, 2006.

In: Strength of Materials Editors: G. Mendes and B. Lago, pp. 133-155

ISBN: 978-1-60741-500-8 © 2009 Nova Science Publishers, Inc.

Chapter 4

CURRENT STATE OF THE ART OF THE CERAMIC COMPOSITE MATERIAL BIOLOX®DELTA Meinhard Kuntz1, Bernard Masson2 and Thomas Pandorf1 1

CeramTec AG, Plochington, Germany 2 CeramTec AG, Pechabou, France

Abstract An extensive overview about the state of the art of the ceramic composite material BIOLOX®delta is given. The unique properties rely on a well defined alumina based fine composite microstructure which is mainly achieved by high temperature solid body reaction of the different ceramic phases during sintering. Zirconia comprises 17 % of the total volume. The tetragonal phase of zirconia is stabilized chemically and mechanically. The high strength and toughness of the material depend on transformation toughening of the zirconia which is clearly shown by various experimental results. The excellent mechanical properties are reproduced batch by batch with a very low scatter. The outstanding properties of the material BIOLOX®delta support advantageous properties of the final product, e.g. ceramic hard-hard bearings for hip arthroplasty. The burst load of the components is significantly increased. It is shown that the design of the components is also very important for the reliability and the ultimate properties of the system. Wear properties at severe conditions are significantly improved by using the new composite material BIOLOX®delta in comparison to pure alumina. Phase transformation of zirconia from the tetragonal to the monoclinic phase due to hydrothermal aging is extensively discussed. Due to the particular distribution and stabilization of the zirconia particles instable aging effects are not possible in this material. After very long time of accelerated aging conditions an increase of monoclinic phase is found – however, it is shown that dynamic and static properties of BIOLOX®delta are not influenced by this effect.

1. Introduction Since 2001 more than 500.000 artificial hip joints with components of the new high performance ceramic composite BIOLOX®delta have been successfully implanted on a

134

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

global basis. Due to the unique strength and toughness of this material the risk of fracture has been substantially reduced when compared to conventional ceramic materials. The outstanding properties of BIOLOX®delta rely on complex reinforcing mechanisms. Therefore, it is necessary to assess if reinforcement is maintained throughout the life-time of the artificial joint which is anticipated to exceed more than 20 years. Furthermore, it is shown that the challenging production of BIOLOX®delta is reproduced at a high quality from batch to batch. Within the scope of this technical contribution the composite ceramic BIOLOX®delta is extensively described and analyzed. The composition and the material properties are presented based on data of regular production lots. It is shown that the advantageous properties of this material are based on the reinforcing mechanisms which are activated due to the unique composition of this material. The particular effect of monoclinic phase transformation and hydrothermal aging is described in detail based on general mechanisms and specific analysis of phase transformation in BIOLOX®delta. Furthermore, experimental data are provided which describe the long term properties of the material, in particular with respect to hydrothermal phase transformation of zirconia in combination with wear and cyclic load conditions.

2. International Material Standards BIOLOX®delta is a modern ceramic composite material for biomedical applications. The main components of the composite are alumina and zirconia. There are ISO standards available for bioceramics of high purity alumina (ISO 6474 - 1) and high purity zirconia (ISO 13356). However, these standards are not directly applicable for the composition of BIOLOX®delta. The ISO organisation is already on the way to prepare a new standard which is applicable for BIOLOX®delta and other similar composite materials (ISO 6474 - 2). The new standard will be released presumably in 2010. Meanwhile, it is helpful to refer and compare the properties of BIOLOX®delta to the draft of the new ISO 6474-2 and the other international material standards which are applicable for related high purity bioceramics.

ISO 6474 – 1 Implants for Surgery – Ceramic Materials - Part 1: Ceramic Materials Based on High Purity Alumina The current version of this standard was released in 1994. The material properties which are defined here reflect typical properties of high quality pure alumina. Strength and toughness which are required according to this standard are significantly lower than those which are available with the composite material BIOLOX®delta. Today, the experts of the ISO working group agree that some details of the current ISO 6474 do not represent the state of the art. Thus, a new version of ISO 6474 - 1 is being preparedwhich is already published as a Draft International Standard (ISO/DIS). Most technical details in this version are already finally implemented. Some details (fracture

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

135

toughness, microstructure) are still under discussion. Presumably, the final release of the new standard will be in 2009. Comment: There is a similar ASTM standard F 603 for the same application and material type. The required material properties are comparable.

ISO 6474 – 2. Implants for Surgery – Ceramic Materials - Part 2: Composite Materials Based on a High Purity Alumina Matrix with Zirconia Reinforcement A standard which is applicable for alumina zirconia composite materials is under preparation. Such composite materials are distinguished in those where the main phase is alumina (ZTA = zirconia toughened alumina) and those where zirconia is the dominating phase (ATZ= alumina toughened zirconia). Both material types are available for biomedical applications. The basic physical properties (e.g. hardness, thermal conductivity) of a composite are primarily derived from the main phase. It is thus useful to describe alumina based zirconia toughened materials parallel to pure alumina materials. Consequently, the new standard has been proposed as part 2 of the established standard ISO 6474 for pure alumina. This concept has been discussed at the ISO TC 150 meetings and was approved by the international experts. The new standard ISO 6474 - 2 is accepted as a Working Draft. It covers all material properties (except of Young´s modulus) which are defined in ISO 6474 - 1. Additionally, the specific subjects of hydrothermal aging and radioactivity, which are relevant for zirconia toughened materials is also included. ISO 6474 – 2 is defined such that a broad range of inorganic compositions are included. A composition of ≥ 60 wt. % alumina and ≥ 10 wt. % zirconia is required. Other ingredients are allowed. The new standard is not exclusively designated for BIOLOX®delta. So far there is no ASTM standard for alumina zirconia composite biomaterials available.

ISO 13 356. Implants for Surgery –Ceramic Materials Based on YttriaStabilized Tetragonal Zirconia (Y-TZP) This standard was revised and published in 2008 as an International Standard (ISO). In contrast to pure alumina, zirconia as a ceramic material can not be produced without a significant amount of other substances for phase stabilization. Several elements are known which are applicable. ISO 13356 is only focussed on Yttria as the stabilizing element. A specific range of Y content is predetermined. It should be noted that the typical range of Y in pure zirconia materials can be different to the required amount of Y in alumina zirconia composites. This issue is thoroughly discussed in chapter 4. Pure zirconia bioceramics can be applied either for biomedical bearings (e.g. hip or knee) or for dental applications. ISO 13 356 does not distinguish between these different applications. As a specific issue of zirconia a test for accelerated hydrothermal aging is required.

136

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

Table 1 gives an overview of the required properties of the 3 standards. The material properties according to the latest revised versions are chosen Table 1. Required material properties according to the ISO standards 6474 – 1 (pure alumina), ISO 6474 – 2 (alumina – zirconia composite) and ISO 13 356 (zirconia). ISO Standard Material Average Bulk density Chemical Composition

Grain Size

ISO 6474 - 1 Pure Alumina ≥ 3,94 g/cm3

ISO 13 356 Zirconia ≥ 6,00 g/cm3

ISO 6474 – 2 Alumina Zirconia ≥ 98,7 %

wt%

Al2O3 ≥ 99,7 MgO ≤ 0,2 Impurities ≤ 0,1

Al2O3 60 - 90 ZrO2+HfO2 10 - 30 Additives ≤ 10 Impurities ≤ 0,2

µm

MV ≤ 2,5 SD ≤ 40 %

ZrO2+HfO2+Y2O3 ≥ 99,0 Y2O3 4,5 – 6,0 HfO2 ≤ 5 Al2O3 ≤ 0,5 Others ≤ 0,5 MV ≤ 0,4

Unit

MPa Strength Weibull Modulus (4 pt bending) Young´s modulus GPa Fracture MPa Toughness m Hardness HV1 Wear Resistance Cyclic fatigue limit Amount of monoclinic phase Accelerated Aging

GPa

Radioactivity

Bq / kg

%

≥ 500 ≥8

≥ 800

Al2O3 MV ≤ 1,5 ZrO2 MV ≤ 0,6 SD ≤ 40 % ≥ 1000 ≥ 10

≥ 380 ≥ 2,5

≥ 4,0

≥ 18 Info No failure at 200 MPa

≥ 17 Info No failure at 400 MPa

No failure at 320 MPa ≤ 20 ≤ 25 % monocl. phase strength decrease not more than 20% ≤ 200

Accomplish requirements described above ≤ 100

Note: The values of ISO 6474 – 1 & 2 are not finally fixed at the date of this publication.

3. Description of BIOLOX®delta BIOLOX®delta is an alumina based composite ceramic. Approximately 80 vol.-% of the matrix consist of fine grained high purity alumina which is very similar to the well known material BIOLOX®forte (ISO 6474). As it is the case in any other composite material, the basic physical properties like stiffness, hardness, thermal conductivity etc. are mainly predetermined from the dominating phase. It was the basic idea for the development of the new material to preserve all the desirable properties of BIOLOX®forte - as an excellent

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

137

bioceramic with more than 30 years clinical experience - but to increase its strength and toughness. These properties are substantially improved by implementation of reinforcing elements. Figure 1 shows the microstructure of BIOLOX®delta.

Alumina matrix Zirconia Platelets

Figure 1. Microstructure of BIOLOX®delta.

Two reinforcing components are integrated into BIOLOX®delta. 17 vol.-% of the matrix consist of tetragonal zirconia particles. The average grain size of the zirconia is around 0.27 µm. As a further reinforcing element, approximately 3 vol.-% of the matrix are built by platelet shaped crystals of the ceramic composition strontium aluminate. The platelets stretch to a maximum length of approximately 5 µm with an aspect ratio of 5 – 10. The reinforcing ability of these ingredients is explained below. Additionally to the reinforcing components, there are also stabilizing elements doped to the material. Chromium is added which is soluble in the alumina matrix and increases the hardness of the composite. The minor amount of chromium is the reason for the pink color of the material, see Figure 2. Furthermore, some yttrium is added to the composite which is solved in the zirconia and supports the stabilization of the tetragonal phase. In Table 2, the composition is given: Table 2. Raw material specification for BIOLOX®delta Ingredient Yttrium oxide Chromium oxide Strontium oxide Zirconium oxide Other oxides Alumina

Formula Y2O3 Cr2O3 SrO ZrO2 TiO2, MgO, SiO2, CaO, Fe2O3, Na2O, K2O Al2O3

Weight percent 1,4 – 2,0 24,0 – 25,5 < 0,22 balance

138

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

During thermal treatment of the material the ingredients are transformed to the particular composition with the 3 components. The basic transformation equations are known as follows:

2 YCrO3 → Y2O3 + Cr2O3

(1)

SrZrO3 → SrO + ZrO2

(2)

Al2O3 + Cr2O3 → Al2O3 : Cr

(3)

SrO + 6 Al2O3 : Cr → SrAl12− x CrxO19

(4)

ZrO2 + Y2O3 → ZrO2 : Y

(5)

In Table 3 the volume fractions of the final products according to equations (3) – (5) are given. Table 3. Components of the final composite BIOLOX®delta Component of the composite Alumina, doped with Chromia Zirconia with Y-stabilization Strontiumaluminate (minor Cr-content)

Formula Al2O3:Cr ZrO2:Y SrAl12-xCrxO19

Figure 2. Ball heads and inserts of BIOLOX®delta.

Volume percent 80 % 17% 3%

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

139

4. Reinforcing Mechanism on BIOLOX®Delta Benefit of Phase Transformation The reinforcing elements, in particular zirconia, substantially increase fracture toughness and strength of the material. Fracture toughness (KIC) is a measure for the ability of the material to withstand crack extension. Strength (σc) is defined as the maximum stress within a structure at failure of the component. The correlation of strength and toughness is given in the fundamental equation of fracture mechanics:

K IC = σ c

ac Y

(6)

where ac is the size of a typical critical defect in the material and Y the shape factor. Consequently, when the fracture toughness of the alumina is increased also the strength is directly improved. This basic principle is the concept of the development of BIOLOX®delta. The microstructure is designed in order to provide an optimum of resistance against crack extension. The benefit in crack resistance which is obtained from incorporating zirconia into an alumina matrix (as shown in Figure 3) is well known in the science of high performance ceramics.

1 µm Figure 3. Reinforcing mechanism in BIOLOX®delta at crack initiation and propagation. Yellow particles represent tetragonal zirconia. Color change to red indicates monoclinic phase transformation. Arrows show the region of compressive stresses due to phase transformation.

The figure represents a realistic part of the microstructure. The gray particles refer to the alumina matrix, yellow to tetragonal zirconia. The phase transformation of zirconia is indicated by the change to red color. In the case of severe overloading crack initiation and crack extension will occur. High tensile stresses in the vicinity of the crack tip trigger the tetragonal to monoclinic phase transformation of the zirconia particles. The accompanied volume expansion leads to the formation of compressive stresses which are efficient for blocking the crack extension. The model as represented in Figure 3 has also been verified experimentally. Pezzotti et.al. [PezTBP] analyzed the monoclinic phase transformation in the vicinity of an artificial crack tip as shown in Figure 4.

140

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

As it is demonstrated in Figure 3 this reinforcing mechanism is fully activated within a region of a few micrometers. For the macroscopic performance of the material it is very important that immediately at the beginning of crack initiation also the reinforcing mechanisms are activated. Regarding Figure 3 one should keep in mind that the average distance between the reinforcing zirconia particles is approx. 0,3µm, i.e. similar to the grain size. Thus, the reinforcement is activated immediately when any microcrack is initiated. The reinforcing ability of zirconia particles is a consequence of the phase transformation, i.e. the spontaneous change from the tetragonal to the monoclinic phase [Han00]. The phase transformation is accompanied by a volume change of 4 % of the zirconia particle. Spontaneous phase transformation is a well known principle in material science. For example, the properties of high performance steels also rely on phase transformation from austenite to martensite.

Grey intensity proportional to monoclinic phase content

Raman Spectroscopy, G. Pezzotti.

Figure 4. Monoclinic phase transformation in the vicinity of an artificial crack tip.

It should be emphasized that the ability of phase transformation is the precondition for any benefit of the zirconia within the material. The composite is designed such that phase transformation occurs when it is needed, i.e. to prevent microcrack initiation and propagation at a high mechanical stress level.

Experiment: What Happens when Phase Transformation Is Suppressed? It has been shown experimentally that the ability of zirconia phase transformation in BIOLOX®delta is necessary for the excellent mechanical properties. The experiment has been designed such that the experimental material was identically produced to BIOLOX®delta but with a significant higher amount of Y2O3. Yttria is known for stabilizing the tetragonal phase of zirconia. Consequently, in the case of a too high amount of yttria, the ability of phase transformation is suppressed. This has been shown in the experiment. The experimental material W3530 has been produced equivalently to the production of BIOLOX®delta. In Figure 5 it is shown that the microstructure is identical. In Table 4 the properties of the two materials are compared.

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

®

BIOLOX delta

141

Experimental material W3530

Figure 5. Microstructure of regular BIOLOX®delta and experimental material W 3530

Table 4. Comparison of regular BIOLOX®delta and high stabilized experimental material Material properties Ratio Y2O3 / ZrO2 [mol %] Final density [g/cm3] Grain size [µm] Strength [MPa] Hardness [HV1] Monoclinic phase content [%] Fracture toughness

BIOLOX®delta 1,3 4,37 0,54 1392 1757 5 6,5

W3530 3,0 4,38 0,55 777 1747 ≤1 5,1

The basic properties of regular BIOLOX®delta and the experimental material W3530 are identical, i.e. microstructure, density, grain size and hardness. The fundamental difference is the ratio of Y2O3/ZrO2. In BIOLOX®delta the amount of yttria is significantly lower. As can be seen from the data, the higher amount of yttria in the experimental material leads - as expected - to a lower content of monoclinic phase, because phase transformation is suppressed. As a consequence the fracture toughness and the strength of the experimental material are much lower than the properties of BIOLOX®delta. In particular, the strength of the experimental material W3530 is only 55% of the normal strength of BIOLOX®delta. From this result it is immediately clear that the ability of phase transformation is necessary to obtain a high performance composite ceramic. The phase transformation can be easily suppressed by chemical stabilization (using yttria). However, suppressing phase transformation means loosing the excellent mechanical properties of the material.

142

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

Stabilization of the Zirconia Tetragonal Phase In BIOLOX®delta the content of yttria has been optimized during the material development. It should be noted that the Y2O3/ZrO2-ratio is lower than in normal pure zirconia materials (3Y-TZP), because the stabilization of the tetragonal phase in BIOLOX®delta is also influenced by “mechanical stabilization”, i.e. the embedding of zirconia in the stiff alumina matrix.

cub

temperature [°C]

2000

1500

tet + cub tet

1000

500 mon

mon + cub 2

4

6

8

Y2O3 [mol %]

Figure 6. Background of stabilizing effects: Y-doping and embedding of zirconia particles in a matrix.

As can be seen in Figure 6 doping of Y2O3 into ZrO2 shifts the temperature of tetragonal – to - monoclinic phase transformation towards lower temperatures. Thus, doping with Y means “chemical stabilization”. At Y2O3 content lower 10% the stable phase at room temperature is monoclinic. So additionally the embedding of the zirconia particles in a matrix as well as surface stresses in the small particles also act as stabilizing mechanisms. The surrounding material will oppose the transformation and it is the strain energy that is involved in this constraint that allows the tetragonal phase to be retained at room temperature [Gre89]. This effect is referred to as “mechanical stabilization”

5. Material Production and Properties BIOLOX®delta is a comparatively complex composite material where 4 different ingredients are mixed during powder preparation and undergo solid phase transformation at high temperature treatment as explained in chapter 2. The ability of reproducing such a material in high quantities with excellent quality batch by batch is the key qualification of CeramTec as manufacturer. It is the purpose of this section both to summarize the important material properties and to elucidate the reproducibility of the production. The important production and analytical steps are as follows:

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

143

Figure 7. Schematic description of processing and material data generation of a single batch.

As shown in Figure 7 the material data are obtained for every powder batch. In Table 5 the material data as obtained for all powder batches in 2007 are summarized.

144

Meinhard Kuntz, Bernard Masson and Thomas Pandorf Table 5. Material properties of BIOLOX®delta batches in 2007

Density g/cm3

4-pt. Weibull Hardness Monoclini Grain Size Fracture Bending Modulus HV 10 c content Alumina Toughness Strength MPa GPa % µm MPa m

Average

4,37

1411

14,9

17,2

4,4

0,54

6,4

Std. Dev.

0,007

50

3,1

0,09

1,1

0,027

0,20

The physical background of these parameters should be discussed. There are parameters which are almost invariable due to the physical nature of the property, in particular density and hardness. In the normal case of regular production there is only very little scatter with these data. However, it is important to analyze these parameters for every batch because any deviation of the expected results would indicate an insufficient production lot. On the other hand, it is worth highlighting the low alumina grain size and the very low scatter of this value. During sintering and final densification of any ceramic the particles build a dense matrix but simultaneously grain growth also occurs. It is the goal of adequate sintering to achieve full density but to suppress grain growth, as a fine microstructure is necessary for good mechanical properties. Obviously, the sintering of BIOLOX®delta is very well reproduced batch by batch. The grain size is low in comparison to pure alumina because the dispersed zirconia particles prevent grain growth of the alumina matrix. The fracture toughness is a measure for the reinforcing mechanisms in the material. As described in chapter 3 the high fracture toughness depends on the transformation mechanism of the zirconia particles. Obviously also this value shows very low scatter. The average fracture toughness is 6,4 MPa√m. In contrast, the “overstabilized” material W3530 described in chapter 3 has a significant lower fracture toughness K1c 5,1 MPa√m. Thus, it can be derived from the evaluation of fracture toughness from batch to batch that the desired transformation toughening is working properly. As explained in chapter 3 the fracture toughness should be discussed in context with the monoclinic phase content which is determined on a polished flat surface of a specimen. The monoclinic phase content [in %] as obtained from the regular X-ray diffraction is relative to the total zirconia content, not to the total volume of the material. Thus, in any case the monoclinic phase content of the total material can be determined by simply referring to the zirconia fraction of 17 vol.%. Example: 10% monoclinic phase content is equivalent to 1,7% relative to the total volume of the material. According to the materials specification the monoclinic phase content after polishing (intrinsic monoclinic phase content) is ≤ 10% of ZrO2 which is regularly determined by X-ray diffraction. The sensitivity of this technique is around 1% monoclinic phase content. As it is evident from the data the average intrinsic monoclinic content of ZrO2 of 4,4% is above the sensitivity limit. This indicates again that the sound material is in disposition of phase transformation. Note that the monoclinic content of the experimental material W3530 is below the sensitivity limit. In contrast to the other parameters discussed above the strength of the material shows significantly higher scatter. It is important to understand that failure in ceramics is always

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

145

triggered by imperfections of the microstructure. High performance ceramics can only be achieved when the natural defects in the material are very small. Typical relevant imperfections in BIOLOX®delta are within a range of 5 – 50µm. Accordingly, the scatter of natural defect size directly matches the scatter of strength which is described by the Weibull´s modulus. A high modulus indicates low scatter. For the high performance material BIOLOX®delta a Weibull’s modulus of ≥ 7 is tolerated in the specification. As can be seen from the data the normal scatter of the strength is much lower (i.e. higher modulus).

6. Correlation of Material and Component Properties In chapter 5 the extensive efforts of analyzing the material properties of BIOLOX®delta batch by batch have been discussed. These material properties are determined according to ISO 6474 which is applicable for pure alumina and currently being extended for aluminacomposite materials such as BIOLOX®delta (ISO 6474-2). This type of data is very familiar for evaluation of the performance of ceramics. In this chapter it is intended to discuss shortly how these material data correlate to component properties, e.g. the strength of ball heads and inserts. In general, the performance of any system depends on the intrinsic material properties, the design and manufacturing quality of the components and the system, the external load and the particular environment, and finally the quality of mounting and installation. The use of high performance materials inevitably promotes the performance of a system - however, the other factors may be even more decisive for the success of a system. These complex correlations must be necessarily evaluated by design analysis, modeling, simulations, risk analysis and many other tools. In order to eliminate any influences of design features most of the material testing has been performed using 4-point bending bars. In Figure 9 the setup of the regular 4-point bending test as recommended in ISO 6474-2 and the burst test according to ISO 7206 are shown. The bending test reveals the intrinsic strength of the material whereas the burst test is designed in order to simulate the in-vivo load of ceramic ball heads.

4-Point Bending Test

Burst Test

Figure 8. Schematic set-up of 4 point bending test and ball head burst test.

146

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

The strength measured with the bending test is – to a first approach - an intrinsic material parameter1, whereas the burst load as obtained from the burst test depends on the materials strength and the design of the ball head and the taper. This is directly shown by comparison of strength and burst load of different ball heads made of BIOLOX®forte and BIOLOX®delta, see Table 6. Table 6. Comparison of strength and burst load of BIOLOX®forte and BIOLOX®delta Parameter Strength Burst load Burst load

Test / Design 4-point bending 28-12/14 L 36-12/14 M

Unit

BIOLOX®forte

BIOLOX®delta

ratio delta / forte

MPa

620

1400

2,3

kN kN

54 110

85 131

1,6 1,2

All burst loads are far above the required value of 46kN. The maximum in vivo load at worst case conditions is approximately 10 kN. The data of the burst tests given in Table 6 are obtained from ball heads with identical geometry, Ti test taper and the same test setup. Thus, the advantage of BIOLOX®delta ball heads in the burst load only comes from the higher strength of the material in comparison to the pure alumina BIOLOX®forte. The strength of BIOLOX®delta is more than twice the strength of BIOLOX®forte, whereas the ratio of the burst strength values is lower. This is explained by the ductile deformation of the Ti taper during the burst test which steadily increases the contact area of the conical bore of the ceramic ball head and the metal taper. However, the burst load of identical ball heads is always higher when a high strength material is used. It is also seen that the burst strength strongly depends on the ball head size. A larger ball head shows a higher burst load. It is concluded that the benefit of using a high performance material is higher when applied to a challenging design, e.g. a ball head with lower wall thickness. Nevertheless, the use of the high strength material always increases the safety margin of the component.

7. Wear Performance of BIOLOX®Delta At normal wear conditions (e.g. standard wear simulator) the wear of a hard-hard couple of BIOLOX®delta is identical to the excellent performance of the well proven pure alumina BIOLOX®forte. There is only a minor difference in hardness of these both materials which does not compromise the normal wear behavior. However, a significant advantage of BIOLOX®delta is identified in the case of worst case wear simulation as shown in Figure 9. In this experiment microseparation of ceramic ball head and insert during each load cycle has been simulated which leads to highly localized 1

Due to the statistical nature the strength also slightly depends on the specimen size and the stress distribution. Size effects can be mathematically balanced. In order to obtain results which can be directly compared to each other the standardized set-up of the bending test should be used.

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

147

forces at the contact area. This experimental setup was supposed to simulate e.g. low tension of the soft tissue after surgery as it is discussed frequently by orthopedic experts. It was concluded from various retrievals that in some cases a well defined stripe-shaped area shows a more intense worn surface than the normal surface of the ball head. This phenomenon is known as “stripe wear”. In the experiment, heavy wear conditions were simulated due to the highly localized contact area. It was found after 5 mio microseparation load cycles that the wear volume of BIOLOX®delta couples (both ceramic ball head and insert were made of BIOLOX®delta) was 7 times lower than that with the coupling made of pure alumina BIOLOX®forte [Cla05]. The wear rate of the mixed couplings (either ball head or insert made of BIOLOX®delta, the remaining made of pure alumina BIOLOX®forte) ranged between those values. It is important to mention that due to the small differential hardness between BIOLOX®forte and BIOLOX®delta can be combined in a ceramic-ceramic coupling without running the risk of excessive wear or other adverse effects.

®

Figure 9. Wear performance of BIOLOX delta and BIOLOX®forte at simulated micro separation.

Obviously BIOLOX®delta shows an excellent “stripe wear tolerance”. The analysis as given in [Cla05] shows that in the stripe wear region the monoclinic phase content is strongly increased. This indicates the mechanism behind the excellent stripe wear tolerance of BIOLOX®delta. As a first approach it is assumed that at these special test conditions a very high localized stress acts in the contact area which may be able to introduce damage in the surface. In this case the reinforcing mechanism as described in Figure 3 is activated in BIOLOX®delta which supports maintaining the surface quality under these extreme conditions. This assumption is supported by the Raman analysis of the worn surface. In the stripe wear region a high monoclinic phase content was found which indicates that phase transformation for reinforcement took place.

148

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

8. Discussion of Hydrothermal Aging Mechanism of Hydrothermal Aging Aging is a relevant issue for all zirconia containing ceramics. The transformation from the tetragonal to the monoclinic phase can be triggered in a hydrothermal environment. “Hydrothermal” means that this particular aging effect only takes place in aqueous environment at elevated temperatures. A critical temperature range for hydrothermal aging is around 120 – 200°C. However, a very slow aging effect is potentially possible even at human body environment. The kinetics and the threshold of aging activation strongly depend on the grain size, volume fraction, amount and type of stabilizing elements (e.g. Y, Ce, Mg, Ca) and mechanical stabilization of the zirconia [Che99]. adsorption

1st step

H2O Zr

2nd step surface

Zr

Zr

O

OH

Zr

OH stress

O

O

O

O

vacancy

Zr

Y

3rd step

migration

Zr

OH

Y

OH

4th step

Zr

OH

migration

O

Zr

Y

Zr

O

Zr

OH

O lattice expansion

Zr

OH

O

Y

OH

Zr

Figure 10. Model of hydrothermal aging.

Albeit the hydrothermal aging is extensively studied in the literature, the exact mechanism behind this effect is still not perfectly described. Most of the available models refer to interaction of the hydroxide ions and oxygen vacancies in the zirconia lattice. The oxygen vacancies inevitably are introduced in the lattice at solution of Y2O3 in ZrO2 due to different valence of the cations. Figure 10 represents a model of the interaction of hydroxide ions with Y-doped zirconia with 4 steps: 1. Adsorption of water molecules at the surface 2. Dissolution of the oxygen bond

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

149

3. Migration of hydroxide ions to oxygen vacancy 4. Reorganisation of the atomic lattice The critical step within this model is the dissolution of the oxygen bond which is very strong in zirconia. Thus, a thermal activation at elevated temperatures is required.

Hydrothermal Aging in BIOLOX®delta Phase transformation caused by hydrothermal aging is an undesired effect. However, as it has been shown in the previous chapters, monoclinic phase transformation is necessary for the reinforcement and the high strength and toughness of the material BIOLOX®delta. Thus, a certain amount of phase transformation in hydrothermal environment is not a matter of concern. It depends on the specific composition of the material if there is a critical level of phase transformation where the material can be damaged. In the years 2001 – 2002 some batches of the pure zirconia material Prozyr® of the company Desmarquest showed catastrophic failure in-vivo due to monoclinic phase transformation at the surface [Che06]. It has to be emphasized that such a damage is impossible in BIOLOX®delta due to the fact that only 17vol% consist of zirconia. Consequently, the ultimate upper limit of monoclinic zirconia is only a total of 17% whereas 83% of the material remain not affected by phase transformation and hydrothermal aging. As mentioned above, hydrothermal aging is accelerated at elevated temperatures. For pure zirconia in biomedical applications a standardized accelerated aging test is recommended in ISO 13 356. The aging conditions are autoclaving at 134°C and 2 bar water steam for 5h. In the new standard ISO 6474-2 being prepared for alumina zirconia composites an aging time of 10h is recommended. As a rough estimate it is proposed that 1h autoclaving is equivalent to 2 – 4 years in human body environment. However, this transfer of aging kinetics depends on individual properties of a material. The aging behavior of BIOLOX®delta has been extensively analyzed using accelerated hydrothermal aging by autoclaving. Moreover, the aging has been combined with severe mechanical static and dynamic testing in order to understand if any material degradation occurs during aging. In fact, the monoclinic phase content in BIOLOX®delta is increased after long term aging. In Figure 11 quantitative analysis of monoclinic phase transformation using Raman spectroscopy are shown. The aging conditions (121°C, 1 bar) for this analysis were slightly different from the recommendation in the ISO standard. Equal to Figure 4 the gray intensity indicates monoclinic phase distribution. As can be seen the monoclinic content is increased after extreme long exposure time. After 300 h the monoclinic phase content reaches a relative value of 66,7%, i.e. 11,3% of the total volume of the composite are monoclinic zirconia.

150

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

Figure 11. Increase of monoclinic phase content after very long term hydrothermal aging in an autoclave. Autoclaving conditions 121°C, 1 bar. Pictures adopted from [Pez08]. Quantitative monoclinic phase content obtained by direct communication to the author.

The autoclaving time used in this study is extremely long, much longer than recommended in the ISO standard. The monoclinic phase content seems to reach a saturation since the increase from 200h to 300 h is only marginal.

Aging Kinetics of BIOLOX®delta As described above the aging effect of zirconia containing materials depends on the individual composition. It is of particular interest to estimate the aging effect of a bioceramic under in-vivo-conditions, i.e. 37°C in serum. As it was the case in the Prozyr® disaster a high amount of phase transformation occurred after a relatively short time in-vivo. On the other hand, it is well known that even pure zirconia is usually much more stable against hydrothermal aging when produced appropriately. For a given material, the long term aging (in years) at low temperatures can be predicted based on the assumption that nucleation and growth of phase transformation are thermally activated. The thermal activation can be assessed by a systematic variation of temperature and duration time in hydrothermal environment and measurement of monoclinic phase transformation before and after the test. The most common method for such a prediction is based on the model of Mehl-Avrami-Johnson (MAJ-theory), which was first applied to zirconia based materials by Prof. Chevalier (Lyon, France) [Che99]. For example, it was found that for a conventional zirconia material with 3 mol% Yttria content (3Y-TZP) one hour in autoclaving conditions (134°C, 2 bar water steam) is equivalent to 3-4 years in-vivo. For other zirconia materials, a correlation of only 2 years was found. It is important to understand that this relation is not a universal law for zirconia containing materials but instead the individual outcome of the particular ceramic composition. The aging kinetics of BIOLOX®delta was analyzed in close cooperation with Prof. Chevalier. The complete study will be accomplished and published in 2009. In the following, the preliminary results which are available at the current state are summarized. The accelerated aging tests were performed in water steam at 142°C, 134°C, 121°C, and 105°C. Additionally one test was performed at 90°C in water. It is assumed that steam and liquid hydrothermal environment are comparable by means of the effect on hydrothermal

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

151

aging. More tests have also been launched at 70°C and 50°C in water. However, due to the long duration time which is necessary to detect any effect at these temperatures results are expected within the next 2 years. The monoclinic phase content was determined using X-ray diffraction. In Figure 12 the results of the tests are shown on a logarithmic time scale. 80

90°C 105°C 121°C 134°C 142°C Pezzotti

monoclinic fraction (%)

70 60 50 40 30 20 10 0 0,1

1

10

100

1000

10000

time (h)

Figure 12.:Monoclinic phase transformation of BIOLOX®delta in hydrothermal environment. For comparison, also data from [Pez08] is included.

For evaluation of these data, the following modified MAJ equation was applied

[

(

Vm = Vm0 + (Vmax − Vm0 ) 1 − exp − (b t )

n

)]

(7)

0

where Vm is the monoclinic phase content, Vm is the initial monoclinic phase content prior to the test, Vmax is an apparent upper bound of the monoclinic phase, t is the time and n the time exponent. b is the factor which describes the temperature dependence of the aging effect. It is derived from fitting the data according to the following Arrhenius type equation:

⎛ Q ⎞ ⎟⎟ b = b0 exp⎜⎜ − ⎝ RT ⎠

(8)

where b0 is a material constant, Q is the activation energy, R the universal gas constant and T the temperature. Evaluation of the data given in Figure 12 reveals an activation energy Q of 108 kJ/mol. This is a particular high value in comparison to a similar material (alumina zirconia composite) which was discussed in [Pez08], where an activation energy of 78kJ/mol is referred. The reason for this discrepancy is, as discussed above, the low amount of oxygen

152

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

vacancies in BIOLOX®delta due to the unique chemical composition. High activation energy means strong influence of temperature on aging. Consequently at low temperatures the aging rate of in BIOLOX®delta is significantly lower. From the modified MAJ equations the hydrothermal aging effect under in-vivo conditions can be estimated. The following equivalence to the accelerated hydrothermal aging was found: 1 h at 134°C is equivalent to 3,9 years in-vivo According to the proposal of the new ISO standard 6474-2 hydrothermal aging is simulated under autoclaving conditions at 134°C for 10 hours. These conditions are thus equivalent to 39 years in-vivo for BIOLOX®delta which seems to be a realistic upper bound of the expected live time of an artificial joint. Several accelerated aging tests according to these conditions (134°C, 2 bar water steam, 10 h) have been performed with BIOLOX®delta. The initial monoclinic phase content prior to aging depends on the surface finishing. On a ground surface the initial monoclinic phase content is higher than on a polished surface due to the more intensive interaction of the ceramic surface to the diamond tool. There is no effect on strength of the higher initial monoclinic phase content - the test specimens for the regular evaluation of strength are ground, not polished. Table 7 gives the data of monoclinic phase increase after 10 h autoclaving Table 7. Analysis of zirconia phase transformation at accelerated aging Surface finishing 5% 21 %

Initial monoclinic phase content 8% 33 %

Monoclinic phase content after 10 h autoclaving

There is obviously a large difference of initial monoclinic phase content between polishing and grinding. However, the relative increase of monoclinic phase transformation does not depend on the surface condition. As discussed in chapter 5 the monoclinic phase content is given relative to the total amount of zirconia. When the effect of phase transformation shall be assessed, it is useful to refer the monoclinic content to the total volume of the material, i.e. taking into account the zirconia volume fraction of 17 vol %. Thus, after grinding and autoclaving the absolute monoclinic phase volume content is 5,6% (33% × 0,17). The accelerated aging according to Figure 11 was performed at 121°C 1 bar, i.e. a lower temperature and steam pressure than recommended in the ISO standards. It is also possible to evaluate the equivalence of this treatment to in-vivo conditions. 1 h at 121°C is equivalent to 1,3 years in-vivo. It should be noted that there is a strong discrepancy of this equivalence factor to the data which was used and discussed in [Pez08], because in this publication the activation energy of

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

153

a different material was used. It is evident that the aging kinetics must be carefully analyzed and discussed for the individual material.

Effect of Hydrothermal Aging on Strength of BIOLOX®delta It is necessary to examine if the phase transformation reveals any damage or loss in strength of the material. For this purpose experiments were designed in order to combine accelerated aging and mechanical loading at a very high stress level. The specimens were prepared according to the 4-point bending configuration as it is shown in Figure 9 (left). These bend bars were exposed to accelerated aging and then to loading-unloading cycles at high stresses. After aging and cyclic loading the residual strength was determined. Two stress levels (300 MPa and 600 MPa) were chosen for the cyclic loading tests. The lower stress level was applied for 20 Mio cycles, the higher stress level for 5 Mio cycles. All tests were performed in Ringer’s solution. The accelerated aging was simulated by 5 h and 100 h treatment in standard autoclaving conditions (134°C, 2 bar water steam). It should be noted that again an aging time much longer than required from the standard was used. For each step of the experiments (as received, after aging, after aging and cycling) the monoclinic phase content was measured using X-ray diffraction. As the most amazing result the yield of specimens surviving all the tests was 100 % in all cases. Even most severe conditions (i.e. 100 h autoclaving, 600 MPa cyclic load) did not reveal any premature failure. It should be recalled that this stress level represents 4 times the highest load level at worst case conditions in-vivo. We can thus conclude that the reliability of BIOLOX®delta exceeds by far the necessary requirements for reliable surgical components. Table 8. Residual strength and monoclinic phase content after diverse treatments. Monoclinic phase is given relative to the total volume of the material Autoclaving duration 0h 5h 100 h

no cyclic load Strength [MPa] Monoclinic phase content [%] Strength [MPa] Monoclinic phase content [%] Strength [MPa] Monoclinic phase content [%]

1346 18 1332 22 1234 30

300MPa, 600MPa, 20*106 cycles 5*106 cycles 1433 33 1248 35 1308 33

1284 43 1361 42 1300 47

Table 8 shows the results of the post – test analysis including residual strength and monoclinic phase content. There is –as expected - a marginal natural scatter in residual strength. However, statistical analysis using Student’s t-test did not reveal any significant deviation of all strength results.

154

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

Monoclinic Content [%]

50 40 30

100 h ageing 20

5 h ageing

10

No ageing

0

no cycling

300 MPa 20 Mio cycles

600 MPa 5 Mio cycles

Figure 13. Increase of monoclinic phase content at cyclic loading.

In contrast, there is a clear tendency of an increase in monoclinic phase content both, after autoclaving and after cyclic loading, which is illustrated in Figure 13. For example, the test series without autoclaving shows an increase of monoclinic phase content from 18 % in the initial state to 47 % after 5 Mio cycles at 600 MPa. It must be concluded that the cyclic mechanical loading at a high stress level (600 MPa) which represents already the strength of pure alumina activated the reinforcing ability of the material. As discussed under Figure 3, a high mechanical stress triggers localized phase transformation which prevents any further crack propagation. Obviously the increased amount of monoclinic phase content does not deteriorate the strength of the material. This important conclusion is independent from the source of the phase transformation. In other words, when the phase transformation is activated either by accelerated aging, cyclic fatigue or a combination of both, the residual strength remains at the initial level.

References [Che99]

Chevalier J., Cales B., and Drouin J.M., Low temperature aging of Y-TZP ceramics, J.Am.Cer.Soc. 82 (1999) 2150-54 [Che06] Chevalier J., What future for zirconia as a biomaterial, Biomaterials 27 (2006) 535-543 [Cla05] Clarke I.C., Pezzotti G., Green D.D., Shirasu H., and Donaldson T., Severe Simulation Test for run-in ear of all-alumina compared to alumina composite THR, Proceedings 10th BIOLOX Symposium, 11-20 (2005) [DeA02] De Aza, A.H., Chevalier J., Fantozzi G., Schehl M., and Torrecillas R., Crack growth resistance of alumina, zirconia and zirconia toughened alumina ceramics for joint prostheses, Biomaterials 23, 937-945 (2002) [Gre89] Green D.J., Hannink R.H.J., and Swain M.V., Tranformation Toughening of Ceramics, CRC Press Inc., Boca Raton, Florida (1989) ISBN 0-8493-6594-5 [Gre04] Gremillard L., Chevalier J., Epicier T., Deville S., and Fantozzi G., Modeling the ageing kinetics of zirconia ceramics, J.Eur.Cer.Soc., 24, 3483-3489 (2004)

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

155

[Han00] Hannink R.H.J., Kelly P.M., and Muddle B.C., Transformation Toughening in Zirconia-Containing Ceramics, J.Am.Cer.Soc. 83 [3] 461-87 (2000) [Ohm99] Ohmichi N., Kamioka K., Ueda K., Matsui K. and Ohgai M., Phase Transformation of Zirconia Ceramics by Annealing in Hot Water, J. Cer. Soc. Jap., 107 [2] 128-133 (1999) [Pez06] Pezzotti G. Environmental Phase Stability of Next Generation Ceramic composite for Hip Prostheses, Key Engineering Materials Vols. 309-311, 1223-1226 (2006) [Pez08] Pezzotti G. Yamada K., Sakakura S., and Pitto R.P., Raman Spectroscopic Analysis of Advanced Ceramic Composite for Hip Prosthesis, J.Am.Ceram.Soc. 91 [4] 1199-1206 (2008) [PezTBP] Pezzotti G. Yamada K., Porporati A., Kuntz M., and Yamamoto K., Raman Spectroscopic Analysis of Advanced Ceramic Composite for Hip Prosthesis: Part II Fracture Behavior (to be published)

In: Strength of Materials Editors: G. Mendes and B. Lago, pp. 157-182

ISBN: 978-1-60741-500-8 © 2009 Nova Science Publishers, Inc.

Chapter 5

PARTICLE MODELING AND ITS CURRENT SUCCESS IN THE SIMULATIONS OF DYNAMICS FRAGMENTATION OF SOLIDS G. Wang1*, A. Al-Ostaz1, A.H.D. Cheng1 and P. Radziszewski2 1

Department of Civil Engineering, University of Mississippi, Oxford, MS, 38677-1848, USA 2 Mechanical Engineering Department, McGill University, Montreal, QC, H3A 2T5, Canada

Abstract Particle modeling (PM) is an innovative particulate dynamics based modeling approach. It has been demonstrated as a robust tool for simulating fracture problems of solids with dynamic fragmentation under extreme loading conditions. These loading conditions can include situations of collapse, impact, blasting or high strain rate tension/compression, as well as thermally-induced breakage problems. Initially, PM was developed for the purpose of mimicking the microscopic material process at macroscopic level. This method can be conceptually illustrated by fully dynamic particles (or “quasi-particles”) placed at the nodes of a lattice network without explicitly considering their geometric size. The potential can be specified for particle-particle interactions via axial springs. Theoretically, PM is an upscale of the molecular dynamics (MD) model applicable to various length scale problems. This is possible if a proper equivalent macroscopic potential is found, and, in case of lattice spacing decreasing to a few Angstroms, a MD model at zero Kelvin with, say, Leonard-Jones potential is recovered. In its current form, PM has been developed as a tool applicable to real engineering problems. The advantages of PM over the existing discrete element based methods can be summarized as follows: (1) Sample in theory. Four conservative/equivalent rules (mass, potential energy, Young’s modulus and tensile/compression strength) are applied to preserve the equivalent material properties. (2) Easy for implementation. Since the physical size of each particle is ignored other than its equivalent mass, the algorithm of coding a PM computation is fairly easy. *

E-mail address: [email protected] Tel: + 662 915 5369, Fax: + 662 915 5523. Corresponding author: Ge Wang

158

G. Wang, A. Al-Ostaz, A.H.D. Cheng et al. Current research work has exhibited that PM is able to correctly predict dynamic fragmentation of materials with a good accuracy. In modeling an epoxy plate with randomly distributed holes in tension, the PM result of the final crack pattern compared favorably with the associate experiment; for the simulations of impact study of two polymeric materials (nylon, 6-6 and vinyl ester) subject to a rigid falling indenter, the modeling results of resistant force, energy, deflection and drop speed of indenter vs. time quantitatively agree fairly well with the according empirical observations.

1. Introduction The prompt development of modern computer technology and computational methods enables scientists, more easily than ever before, to numerically examine the nature of materials, to verify or modify the existing theories, and even to discover new phenomena. Dynamic fracture modeling also greatly benefits from this advancement. The dynamic fracture process itself is an exceedingly complex, multi-scale physical phenomenon. Material failure exhibits non-linearly, localized presence and a dependence on dynamic loading and loading conditions, etc. Hence, an ideal solver of dynamic fracture mechanics is required to be able to handle all the above-mentioned factors, especially to deal with the discontinuity of material that dominantly occurs in a dynamic fracture process which becomes an overwhelming difficulty to numerical approaches. At the microscopic level, fracturing is a process that material becomes separated due to the successive failures of atomic bonds. Since the intrinsic strength properties at atomic structure level are available, molecular dynamics (MD) analysis has been used in modern scientific research at nano-scale. However, although MD simulation has benefited from the rapid development of modern computer technology and is becoming increasingly popular, the present state of computational power is still far from being able to support simulation at the macroscopic level. For example, we currently still cannot simulate a 1 × 1 × 1 cm3 cubic copper body at atomic level because the body consists of 10 24 copper atoms, a number so large that no computer in the world can handle it. The second difficulty is its inability to reach the laboratory time scales. For instance, the laboratory fracture experiments generally last in microseconds ( 10 −12

−6

−9

second), while the MD model time steps are typically in the nano ( 10 )

or pico ( 10 ) second range. As such, MD is limited narrowly to solving nano- to micrometer scale problems. Hence modeling fracture problems directly at macroscopic scale is a prevalent pursuit. An all-round search to the existing optional modeling techniques reveals that the modern numerical methods for dynamic fracture simulations at macroscopic level can be generally classified into two categories of approaches. One is continuum mechanics based and the other is discrete element based. Examining the state-of-the-art of the research, we conclude that the continuum mechanics based approaches, such as the finite element method (FEM), have difficulty in solving dynamic fracture problems, particularly in dealing with the simulation of the collapse of structure and its fragmentation under extreme loading conditions. For this reason, another domain of alternative modeling approach —the discrete element based models, has become more and more popular. Discrete element models share a common concept of “discrete material”, which can still be further classified into two sub-categories. The first one is classified as a discrete element

Particle Modeling and Its Curent Success in the Simulations...

159

method, in which the physical size and shape of each element is considered in the computation, such as the applied element method (AEM) [Meguro & Tagel-Din, 2000], and particle finite element method (PFEM) [Oñate, et al., 2004] - another particle-related model. In practice, this type of models is complex and difficult to be implemented. For instance, AEM is laborious in keeping track of the instantaneous contact positions and the evolving geometry of all elements for a proper updating of the dynamic bonds; PFEM is expensive in remeshing and redefining boundaries at each time step. The second branch is named particle (or particulate) dynamics method, in which the physical size and shape of each discrete cell is not explicitly considered in the computation. Consequently, each cell is treated as a particle, with the equivalent mass lumped at its center. Smoothed particle hydrodynamics (SPH) [Monaghan, 2005], and particle modeling (PM) are currently the mainly two popular particulate based models. SPH adopts a kernel probability density function to define for each particle a reaction domain at each time step, in terms of a particle number density; it is therefore highly expensive in computation. In contrast, PM is rather simple in theory and easy for implementation; hence, it is attracting increasing interest, despite a good number of SPH codes. Particle modeling (PM) method was originally proposed by Greenspan [1981, 1997] for the purpose of mimicing the microscopic material process at macroscopic level. PM is fully dynamic with particles (or “quasi-particles”) placed at the nodes of a periodic (equilateral triangular) lattice. Conventionally, only the nearest neighboring particles are accounted for in the interaction via axial spring connections. Similar to MD, potential can be specified for particle-particle interactions, and, in the case of lattice spacing decreasing to a few Angstroms, we recover a molecular dynamics (MD) model at zero Kelvin with, say, a Leonard-Jones potential. This implies that PM is an upscaled MD and can be applied to various length scale problems if a proper equivalent macroscopic potential is used. Obviously, by making use of the similar processes as atomic interactions, it is possible to solve fracture problems at macro-scale level. However, as no direct link with the material properties was attempted by Greenspan, Greenspan’s PM method remains a conceptual model without a demonstrated success in fracture modeling. Wang and Ostoja-Starzewski [2005a] developed a newly modified PM with a conventional linkage pattern as shown in Figure 1. In this new PM, equivalent material properties are formulated using four physical conditions to determine continuum-level Young’s modulus and tensile strength, while maintaining the conservation of mass and energy of the particle system, and satisfying the interaction laws among all the particles. The theoretical foundations of the current PM can be outlined in the following four aspects: (a) Derivation is based on equivalence/equality of mass, energy, elastic moduli and tensile strengths between both atomic and quasi-particle systems. (b) Derivation is carried out in the setting of a 3-D face-centered cubic (f.c.c) lattice network (Figure 2) for both atomic and quasi-particle structures. (c) Either Lennard-Jones, polynomial or quadratic potentials can be employed for nonlinear or linear axial linkage. (d) In principle, it can be applied for various length scale problems of solids.

160

G. Wang, A. Al-Ostaz, A.H.D. Cheng et al.

Wang and Ostoja-Starzewski, 2006.

Figure 1. Lattice structure in PM.

Wang and Ostoja-Starzewski, 2005a.

Figure 2. Meshing system for a 3D material body.

In this paper, current PM modeling development is to be addressed. In the coming sections, first we will introduce the theory of PM; then report some significant success and also defects experienced through the applications. Meanwhile, the potential solutions to the modeling deficiencies are proposed; and finally, in the conclusion part, an outlook of futuregoing PM development is addressed.

2. Methodology of PM In particle modeling (PM), the nonlinear interaction force is considered between nearestneighbor (quasi-) particles and assumed to be of the same form as in MD:

Particle Modeling and Its Curent Success in the Simulations...

F =−

G H + r p rq

161

(1)

Here G, H, p and q are positive constants, and q > p ≥ 1 to obtain the repulsive effect that is necessarily (much) stronger than the attractive one, r being the distance between two particles. Ashby & Jones [1980] presented a simple method to evaluate continuum-type Young’s modulus E and tensile stress σ (r ) of the material from F (r ) , namely

E= and

S0 r0

σ ( r ) = NF (r )

(2) (3)

where S 0 = ( dF / dr ) r = r0 , and r0 is the equilibrium spacing between contiguous particles. N is the number of bonds/unit area, equal to 1 / r02 . Tensile strength, σ TS , results when

dF (rd ) / dr = 0 , that yields,

σ TS = NF (rd )

(4)

Just as in MD, the non-linear dynamical equation of motion for each particle Pi of the PM system is given by

G ⎡⎛ G H ⎞ rGji ⎤ d 2 ri mi 2 = ∑ ⎢⎜ − pi + qi ⎟ ⎥ i ≠ j ⎜ dt rij ⎟⎠ rij ⎦⎥ ⎣⎢⎝ rij ,

(5)

G

where mi and r ji are mass of Pi and the vector from Pj to Pi . Note that if an equilateral triangular lattice structure is adopted in 2-D, the resulting Poisson ratio equals 1/4 (or 1/3) when a 3-D (respectively, plane) elasticity formulation is adopted [Ostoja-Starzewski, 2002, 2007]. The derivation of four parameters in Equation (1) from MD structures is conducted on a cubic body with volume V (= A × B × C ), in Figure 2. A face-centered cubic (f.c.c) lattice for both atomic and quasi-particle structures is chosen. If p, q and r0

are given, then, by

conditions of mass and energy conservation, G and H can be derived. Consequently, Young’s modulus is evaluated by Equation (2) and tensile strength by Equation (4). To represent an expected material property, we would have to do many sets of testing until a unique ( p, q ) is

162

G. Wang, A. Al-Ostaz, A.H.D. Cheng et al.

found to match both Young’s modulus and tensile strength of the material. The complete derivation process is described below. First, for the atomic structure (MD model), we have:

⎛ Ga r 1− pa H a r 1−qa + interaction potential energy (ergs): φ a = ⎜⎜ 1 − qa ⎝ 1 − pa

⎞ ⎟ × 10 −8 ⎟ ⎠

(6)

Young’s modulus (GPa) is obtained from Equation (2) and tensile strength (MPa) from Equation (4). Total number of atoms in A × B × C cubic material body:

⎞ ⎞ ⎛ C × 10 8 ⎛ A × 10 8 ⎞ ⎛ B × 10 8 ⎜ ⎟ ⎟ + 1⎟⎟ × ⎜⎜ 1 1 + + × N * = ⎜⎜ 0 ⎟ ⎜ r 6 /3 ⎟ r sin 60 r a ⎝ ⎠ ⎝ a ⎠ ⎝ a ⎠

(7)

In Eqs. (6) and (7), ra is equilibrium position of the simulated material in atomic structure, and p a , q a are the exponential parameters in atomic structure. Note that, for a Lennard-Jones interaction case, pa = 7 and qa = 13 . Next, for the quasi-particle structure (PM model), we have interaction force (dynes) as in Equation (1). Interaction potential energy (ergs):

φ =

G r 1− p 1− p

+

H r 1− q 1− q

, for p > 1; φ = G ln r +

H r 1− q 1− q

total number of quasi-particles in PM system: N = imax × j max × k max

, for p =1

(8)

(9)

We now postulate the equivalence of MD and PM models. From the mass conservation, we calculate the mass of each quasi-particle m based on atomic mass m a :

m = N * × ma / N

(10)

From the energy conservation, we have:

(N × φ )r =r

0

under the requirement:

(

= N * × φa

)

r = ra

F (r0 ) = 0

From equations (11), (12), we now derive Young’s modulus E:

(11) (12)

Particle Modeling and Its Curent Success in the Simulations... for p = 1 : 1− q o

G = Hr

(N

, H =

*

× φa

)

r = ra

1− q 0

N (1 − q )r

(1 − q ) 1− q 0

ln r0 − r

, E = −Gr0−3 + qHr0− q − 2

163

(13)

for p > 1 :

(N ×φ ) *

1− q , o

G = Hr

H=

a r =ra

(1− p)(1− q)

N( p − q)

r0q−1 , E = − pGr0− p − 2 + qHr0− q − 2

(14)

Similarly, tensile strength can be obtained under dF ( rd ) / dr = 0 . Evidently, the four parameters ( p, q ) , r0 and V affect E and

σ TS .

We have established the equations for G, H, p and q, and carried out a parametric study to find the differing effects on p, q, V and r0 [Wang and Ostoja-Starzewski, 2005a]. Herein, we summarize the obtained rules as follows: (i) The larger the values of ( p, q ) are adopted, the larger is E generated. This is typically associated with the material becoming more brittle than ductile, albeit there is a range of toughness to choose from. Also, with E going up, there is a fragmentation into a larger number of pieces. (ii) In the case of p = 1 , the larger r0 spacing is adopted, the higher is Young’s modulus of the PM material. On the contrary, in the special case of p ≠ 1 , there is an opposite trend. In any case, this increase or decrease does not change very much. (iii) In the case of p ≠ 1 , while keeping the volume fixed, an increase of r0 produces a decrease of Young’s modulus. The situation is again opposite in the case of p = 1. (iv) A uniform augmentation of volume V by dilation in all three coordinate directions (xyz), at any ( p, q ) combination, results in Young’s modulus increasing first strongly and then leveling off. For brittle materials, a general format of linear dynamical equation is often employed [Wang, et al., 2008a],

− S (r − r0 ) for rc ≤ r ≤ rt F ={ 0 0 otherwise

(15)

with r being the distance between two particles, the stiffness S 0 = E • r0 by Equation (2), E the Young modulus and

rmax

the failure displacement of material, r0 the equilibrium

spacing between the contiguous particles.

164

G. Wang, A. Al-Ostaz, A.H.D. Cheng et al. In Equation (15), rc and rt are the fracture positions applied for compression and

tension, respectively, which need to be empirically determined. The leapfrog method, with second-order accuracy, is employed in all PM simulations. The leapfrog formulas relating position, velocity and acceleration for particles Pi ( i = 1,2,..., N ) [Greenspan, 1997] are

G G (Δt ) G Vi ,1 / 2 = Vi , 0 + ai , 0 2

(starter formula)

(16)

G G G Vi ,k +1 / 2 = Vi ,k −1 / 2 + (Δt )ai ,k , k = 1,2,3,...

(17)

G G G ri ,k +1 = ri ,k + (Δt )Vi ,k +1 / 2 G

G

k = 0,1,2,...

(18)

G

where Vi ,k , ai ,k and ri ,k are the velocity, acceleration and position vectors of particle i at

G

time t k = kΔt , Δt is the time step. Vi ,k +1 / 2 stands for the velocity of particle i at time

t k = (k + 1 / 2)Δt , and so on. Notably, the leapfrog method is of second-order 2

accuracy: O ((Δt ) ) . The safe time step is after the derivation result by Hockney & Eastwood [1999]:

ΩΔt

No part of this digital document may be reproduced, stored in a retrieval system or transmitted in any form or by any means. The publisher has taken reasonable care in the preparation of this digital document, but makes no expressed or implied warranty of any kind and assumes no responsibility for any errors or omissions. No liability is assumed for incidental or consequential damages in connection with or arising out of information contained herein. This digital document is sold with the clear understanding that the publisher is not engaged in rendering legal, medical or any other professional services.

STRENGTH OF MATERIALS

GUSTAVO MENDES AND

BRUNO LAGO EDITORS

Nova Science Publishers, Inc. New York

Copyright © 2009 by Nova Science Publishers, Inc. All rights reserved. No part of this book may be reproduced, stored in a retrieval system or transmitted in any form or by any means: electronic, electrostatic, magnetic, tape, mechanical photocopying, recording or otherwise without the written permission of the Publisher. For permission to use material from this book please contact us: Telephone 631-231-7269; Fax 631-231-8175 Web Site: http://www.novapublishers.com NOTICE TO THE READER The Publisher has taken reasonable care in the preparation of this book, but makes no expressed or implied warranty of any kind and assumes no responsibility for any errors or omissions. No liability is assumed for incidental or consequential damages in connection with or arising out of information contained in this book. The Publisher shall not be liable for any special, consequential, or exemplary damages resulting, in whole or in part, from the readers’ use of, or reliance upon, this material. Any parts of this book based on government reports are so indicated and copyright is claimed for those parts to the extent applicable to compilations of such works. Independent verification should be sought for any data, advice or recommendations contained in this book. In addition, no responsibility is assumed by the publisher for any injury and/or damage to persons or property arising from any methods, products, instructions, ideas or otherwise contained in this publication. This publication is designed to provide accurate and authoritative information with regard to the subject matter covered herein. It is sold with the clear understanding that the Publisher is not engaged in rendering legal or any other professional services. If legal or any other expert assistance is required, the services of a competent person should be sought. FROM A DECLARATION OF PARTICIPANTS JOINTLY ADOPTED BY A COMMITTEE OF THE AMERICAN BAR ASSOCIATION AND A COMMITTEE OF PUBLISHERS. LIBRARY OF CONGRESS CATALOGING-IN-PUBLICATION DATA Strength of materials / edited by Gustavo Mendes and Bruno Lago. p. cm. Includes bibliographical references. ISBN 978-1-61728-584-4 (E-Book) 1. Strength of materials. 2. Composite materials. I. Mendes, Gustavo. II. Lago, Bruno. TA405.S765 2009 620.1'12--dc22 2009013535

Published by Nova Science Publishers, Inc.

New York

CONTENTS Preface

vii

Chapter 1

High Temperature Mechanical Properties and Microstructure of Sic-Based Fibers under Severe Environments Jianjun Sha

Chapter 2

Ionomers as Candidates for Structural Materials Daniel J. Klein

61

Chapter 3

Failure of Layered Composites Subject to Impacts: Constitutive Modeling and Parameter Identification Issues Stefano Mariani

97

Chapter 4

Current State of the Art of the Ceramic Composite Material BIOLOX®delta Meinhard Kuntz, Bernard Masson and Thomas Pandorf

133

Chapter 5

Particle Modeling and Its Current Success in the Simulations of Dynamics Fragmentation of Solids G. Wang, A. Al-Ostaz, A.H.D. Cheng and P. Radziszewski

157

Chapter 6

Non-Oriented Electrical Steels: Materials for Saving Energy and Conserving the Environment Taisei Nakayama

183

Chapter 7

Influence of Luting Cement Application Technique on Quartz Fiber Post Regional Bond Strengths Camillo D’Arcangelo, Francesco De Angelis, Maurizio D’Amario, Simone Zazzeroni, Mirco Vadini and Sergio Caputi

217

Chapter 8

Microstructural Influence on Flexure Strength of a Ceromer Reinforced by Two Types of Fibers (Polyethylene and Glass) Silvana Marques Miranda Spyrides and Fernando Luiz Bastian

233

1

vi Chapter 9

Index

Contents Influence on Strength Properties of Anisotropy Planes in Slates Samples in the NW of Spain M.A. Rodríguez-Sastre, M. Gutiérrez-Claverol, M. Torres-Alonso and L. Calleja

247

261

PREFACE The strength of a material refers to the material's ability to withstand an applied stress without failure. The applied stress may be tensile, compressive, or shear. A material's strength is dependent on its microstructure. The engineering processes to which a material is subjected can alter this microstructure. This book provides a variety of material strength research including an extensive overview on the state of the art ceramic composite material BIOLOX delta which, since 2001, has successfully implanted more than 500,000 artificial hip joints. Due to the unique strength and toughness of this material, the risk of fracture has been substantially reduced when compared to conventional ceramic materials. Several different aspects of ionomer research from a physical property standpoint is discussed as well, including the history and current trends in ionomer research and a discussion on the immediate needs in this field. Furthermore, particle modeling (PM) as an innovative particulate dynamics based modeling approach is examined as a robust tool for simulating fracture problems of solids under extreme loading conditions, including situations of collapse, impact, blasting or high strain rate tension/compression. This book includes research on the ability of particle modeling to correctly predict dynamic fragmentation of materials with good accuracy. Ceramic-matrix composites (CMCs) have been considering as potential structural materials for advanced energy-generation systems and propulsion systems. SiC fibers with low oxygen content and high crystallinity, which derived from polycarbonsilane, are the backbone as reinforcements in load-bearing CMCs. For high temperature application, the most desired critical properties of SiC fibers are high strength and stiffness as well as the reliable retention of these properties throughout the service life of application. Low fiber strength and thermal stability could result in low fracture toughness and accelerate sub-critical crack propagation in CMCs. Thus, the mechanical durability and microstructure stability of SiC fibers are major concerns under severe environments. Furthermore, in practical service environments, rarely is one degradation mechanism operative, but several mechanisms operate simultaneously, leading to the environment-pertinent degradation mechanism is complex for the SiC materials. In order to enhance the understanding of reliability and durability of CMCs applied to high temperature and oxidative environments, the investigations on the high temperature mechanical properties and microstructure for SiCbased fibers subjected to severe environments were integrated into Chapter 1. The field of ionomers is an often overlooked and under-utilized branch of polymer research. Although ionomers can be broadly described as a class of polymers that contain any

viii

Gustavo Mendes and Bruno Lago

number of ionic groups, from a structural property standpoint only a low percent of ionic groups are necessary to impart significantly improved properties over the nonionic version of the same polymer. Current trends in the field of ionomers are highly focused on the field of fuel cell technology. There appears to be a significant hole remaining in the study of imparting strength to materials using ionic groups. This hole is very significant from an industrial point of view, and has a large commercial potential. There are very few commercially available ionomers, which shows how little this field has been explored to date. Chapter 2 will focus on several aspects of ionomer research from a physical property standpoint: 1) A history of ionomer research, 2) Current trends in ionomer research - a) standalone polymers, b) nanocomposites, c) blends; 3) A commentary on the immediate needs in the field of ionomer research. Layered composites subject to impacts can fail by delamination, i.e. by debonding between laminae, if the stress waves cause damaging phenomena to take place mainly within the resin-enriched interlaminar phases. To simulate delamination at the structural level, processes dissipating energy are lumped onto fictitious zero-thickness interlaminar surfaces, and softening interface constitutive laws are adopted to describe the progressive failure of the interlaminar phases. Since delamination occurs inside very narrow regions, results of experimental testing on whole composites need to be accurately and reliably filtered to calibrate the interface constitutive laws. To this aim, Chapter 3 proposes a sigma-point Kalman filter approach. The performances of the proposed methodology, in terms of constitutive parameter estimations and dynamic delamination tracking, are assessed through pseudoexperimental testings on a two-layer composite, and real testings on multi-layer glass fiber reinforced plastic composites. An extensive overview about the state of the art of the ceramic composite material BIOLOX®delta is given. The unique properties rely on a well defined alumina based fine composite microstructure which is mainly achieved by high temperature solid body reaction of the different ceramic phases during sintering. Zirconia comprises 17 % of the total volume. The tetragonal phase of zirconia is stabilized chemically and mechanically. The high strength and toughness of the material depend on transformation toughening of the zirconia which is clearly shown by various experimental results. The excellent mechanical properties are reproduced batch by batch with a very low scatter. As presented in Chapter 4, the outstanding properties of the material BIOLOX®delta support advantageous properties of the final product, e.g. ceramic hard-hard bearings for hip arthroplasty. The burst load of the components is significantly increased. It is shown that the design of the components is also very important for the reliability and the ultimate properties of the system. Wear properties at severe conditions are significantly improved by using the new composite material BIOLOX®delta in comparison to pure alumina. Phase transformation of zirconia from the tetragonal to the monoclinic phase due to hydrothermal aging is extensively discussed. Due to the particular distribution and stabilization of the zirconia particles instable aging effects are not possible in this material. After very long time of accelerated aging conditions an increase of monoclinic phase is found – however, it is shown that dynamic and static properties of BIOLOX®delta are not influenced by this effect.

Preface

ix

Chapter 5 studies particle modeling (PM), which is an innovative particulate dynamics based modeling approach. It has been demonstrated as a robust tool for simulating fracture problems of solids with dynamic fragmentation under extreme loading conditions. These loading conditions can include situations of collapse, impact, blasting or high strain rate tension/compression, as well as thermally-induced breakage problems. Initially, PM was developed for the purpose of mimicking the microscopic material process at macroscopic level. This method can be conceptually illustrated by fully dynamic particles (or “quasi-particles”) placed at the nodes of a lattice network without explicitly considering their geometric size. The potential can be specified for particle-particle interactions via axial springs. Theoretically, PM is an upscale of the molecular dynamics (MD) model applicable to various length scale problems. This is possible if a proper equivalent macroscopic potential is found, and, in case of lattice spacing decreasing to a few Angstroms, a MD model at zero Kelvin with, say, Leonard-Jones potential is recovered. In its current form, PM has been developed as a tool applicable to real engineering problems. The advantages of PM over the existing discrete element based methods can be summarized as follows: (1) Sample in theory. Four conservative/equivalent rules (mass, potential energy, Young’s modulus and tensile/compression strength) are applied to preserve the equivalent material properties. (2) Easy for implementation. Since the physical size of each particle is ignored other than its equivalent mass, the algorithm of coding a PM computation is fairly easy. Current research work has exhibited that PM is able to correctly predict dynamic fragmentation of materials with a good accuracy. In modeling an epoxy plate with randomly distributed holes in tension, the PM result of the final crack pattern compared favorably with the associate experiment; for the simulations of impact study of two polymeric materials (nylon, 6-6 and vinyl ester) subject to a rigid falling indenter, the modeling results of resistant force, energy, deflection and drop speed of indenter vs. time quantitatively agree fairly well with the according empirical observations. Electrical steels are the core materials for electrical motors or transformers. Those materials for motors are played an energy conversion roll from electricity to motion. However, energy losses are accompanied with this conversion. To minimize these losses is a key technology to conserve our environment. Numerous researches on the grain-oriented electrical steels reported. Those researches especially for transformers are focused on the reducing the losses at supplying the electricity from power plants. On the other hand, home or industrial appliances are the power consuming devices, and the most effective point on the energy loss reduction. These home appliances are used small motors using non-oriented electrical steels. In Chapter 6, several researches on the non-oriented electrical steels are discussed and focused on the metallurgical control of the steels to reduce the core loss for generating waste heats and motor building innovation technologies for decreasing the building factor of the core losses. In the metallurgical part, some additive elements as phosphorus, aluminum and manganese for improving magnetic properties reviewed. Moreover some contaminating elements as vanadium, titanium and zirconium are discussed especially for precipitation studies in the steels have been done. These precipitations are inhibited the grain growth at final annealing or stress relief annealing. These inhibited small grains increase the core losses.

x

Gustavo Mendes and Bruno Lago

For studying motor building technologies, compression stress effect, shearing stress effect are discussed. Even though the best core materials are used for manufacturing motors, those building deteriorations make worse for the motor efficiency. Therefore, those technologies are also important for reducing the carbon dioxide emission. The aim of Chapter 7 was to investigate regional root canal push-out bond strengths for a fiber-reinforced post system varying the application method of the luting agent. Recently extracted maxillary incisors (n=30) were sectioned transversally at the labial cemento-enamel junction, and the roots treated endodontically. Following post space preparations, fiber-reinforced posts (Endo Light-Post; RTD) were placed using adhesive system and resin cement provided by the manufacturer. Three equal groups (n=10) were assessed according to the technique used to place the luting agent into post space: using a lentulo spiral, applying the cement onto the post surface, injecting the material with a specific syringe. Each root was sliced into three discs (2 mm thick) representing the coronal, middle and apical part of the bonded fiber post. Push-out tests were performed for each specimen to measure regional bond strengths. Results were statistically analyzed using two-way ANOVA and Tukey tests (α = 0.05). All fractured specimens were observed using a scanning electron microscope to identify the types of failure. The results indicated that bond strength values were significantly affected by the application method of the resin cement (p < 0.05). The "syringe technique" and the "lentulo technique" showed higher bond strength values compared with the "post technique". No significant differences were recorded among the post space thirds. Microscopic analysis revealed a prevalence of post/cement and mixed failures. The best performance in terms of push-out bond strengths for the post system tested was obtained when the luting agent was applied into the post space either with a specific syringe or using a lentulo spiral. There were not differences in bond strength among root thirds. In Chapter 8, the microstructures of a ceromer (Artglass®) reinforced by either glass fibers (GlasSpan®) or polyethylene fibers (Connect®) were characterized and compared and the influence of the fiber reinforcement on the flexural strength of the resulting products evaluated. With this objective, seven bars of each material were produced. One bar of each material was separated for microstructural analysis. The microstructural samples were subjected to metallographic polishing and finishing, and then analyzed using optical microscopy at different magnifications. The images obtained were treated using an image processing computer program (Image Pro Plus) in order to quantify the microstructure by calculating the mean diameter and mean volume fraction of fibers. The flexure tests were made by three-point bending, using six samples of each material. After statistical analysis, the results showed that the mean diameter of the glass fibers (4μm) was smaller than the polyethylene ones (23.6 μm). The mean volume fraction of glass fibers (0.42) was larger than that of the polyethylene fibers (0.28) and the mean center-to-center distance between fibers was smaller in the glass fibers material (33 μm) than in the polyethylene fibers material (61 μm). The flexural strength of both glass and polyethylene fiber-reinforced materials was statistically equal, despite the fiber volume fraction being statistically larger in the fiber glass material. The purpose of Chapter 9 is to describe the influence of anisotropy on the geomechanical strength properties of two Spanish slates with different chemical and physical characteristics. From laboratory testing results of slates under point load and uniaxial compression and the use of indirect methods, as it is the measurement of P velocities, principal parameters were

Preface

xi

calculated for this rock material. As it is well known under uniaxial compressive strength slates are strong and also very strong rock when loading is parallel (90o) o perpendicular (0o) to the main anisotropic planes. In contrast it is a weak rock with minimum strength values for angles between 45 to 60o of inclination of anisotropy planes. The correlation equations were calculated between different parameters. Despite weak correlation between different geotechnical properties were found and when all lithologies are considered together correlation of geomechanical properties is weak. However when each lithology is considered separately the geomechanical properties can be coherently defined. Linear and polynomial equations were found for the point load and uniaxial strength correlations with the inclination of the anisotropy. Different strength fields were calculated when uniaxial strength and point load test plot and its comparison include the inclination of the anisotropy planes on slates. Uniaxial compressive strength and P wave velocity appears to be strongly influenced by uniaxial strength and good polynomial correlations resulted. Plots of slates with other sedimentary type of rocks from Cantabrian Zone, CZ, revealed the hardness and highest strength of slates when loading is perpendicular to the main anisotropy planes.

In: Strength of Materials Editors: G. Mendes and B. Lago, pp. 1-60

ISBN: 978-1-60741-500-8 © 2009 Nova Science Publishers, Inc.

Chapter 1

HIGH TEMPERATURE MECHANICAL PROPERTIES AND MICROSTRUCTURE OF SIC-BASED FIBERS UNDER SEVERE ENVIRONMENTS Jianjun Sha1,2* 1

Shool of Aeronautics and Astronautics, Dalian University of Technology 116024, Dalian, China 2 Ceramic Materials Engineering, University of Bayreuth, D-95440 Bayreuth, Germany

Abstract Ceramic-matrix composites (CMCs) have been considering as potential structural materials for advanced energy-generation systems and propulsion systems. SiC fibers with low oxygen content and high crystallinity, which derived from polycarbonsilane, are the backbone as reinforcements in load-bearing CMCs. For high temperature application, the most desired critical properties of SiC fibers are high strength and stiffness as well as the reliable retention of these properties throughout the service life of application. Low fiber strength and thermal stability could result in low fracture toughness and accelerate sub-critical crack propagation in CMCs. Thus, the mechanical durability and microstructure stability of SiC fibers are major concerns under severe environments. Furthermore, in practical service environments, rarely is one degradation mechanism operative, but several mechanisms operate simultaneously, leading to the environment-pertinent degradation mechanism is complex for the SiC materials. In order to enhance the understanding of reliability and durability of CMCs applied to high temperature and oxidative environments, the investigations on the high temperature mechanical properties and microstructure for SiC-based fibers subjected to severe environments were integrated into this review.

*

Corresponding address: School of Aeronautics and Astronautics, Dalian University of Technology, 116024, Dalian, China

2

Jianjun Sha

1. Introduction Non-oxide Ceramic-matrix Composites (CMCs), have been extensively studied during the last two decades. Currently, CMCs have been proposed to use as the structural materials in application of high temperature technologies, such as advanced nuclear energy systems [13], various stationary gas turbine engines and aerospace propulsion systems [4-6]. As structural engineering materials, one of the important advantages of CMCs is the significant improvement of toughness by using continuous ceramic fibers compared to their monolithic ceramics. In continuous ceramic fiber reinforced CMCs, the improved toughness is attributed to several energy dissipating mechanisms when the matrix crack is occurring under applied stress, such as crack deflection, fiber bridging and fiber sliding [7]. The energy dissipation procedure can be illustrated schematically in Figure 1. These energy dissipations enhanced the fracture toughness and resulted in a non-catastrophic failure mode. If the conditions for de-bonding are satisfied, fibers bridge the crack faces in the wake of the crack tip, subsequent to matrix cracking. The stress bore by bridge fibers applies traction forces to the crack faces that reduce the stress intensity at the crack tip. Under specific condition crack propagation does not occur without additional applied stress. The performance of CMCs could be improved through the optimization of fiber/interface/matrix, and now the fabrication process is still in developing and progressing.

σ

σ Fiber bridging

Fiber fracture

Interface Fibers

Crack tip Crack

crack

Crack deflection Matrix

σ Monolithic

σ composite

Figure 1. Schematic of crack propagation and principle for improved toughness in CMCs.

Based on the simple theory of mixture for the ultimate tensile strength (UTS) calculation of continuous fiber reinforced ceramic matrix composites [8], in the case of CMCs with I-D reinforcement alignment, when the reinforced fiber has a smaller modulus and a similar or even large strength, significant matrix cracks must be occurred before reaching the UTS of

High Temperature Mechanical Properties and Microstructure…

3

fiber. In other words, when the applied stress is beyond that of the crack initiation of matrix, the residual stress is mainly carried by the fiber alone. Pull out of the fiber can significantly improve the fracture toughness. The fibers are backbone in CMCs and play a very important role on the mechanical properties of CMCs. Among of CMCs, SiC fiber reinforced SiC matrix composite (SiC/SiC) has been considered as one of the most potential candidate materials, because it possessed many attractive properties for structural engineering applications under severe environments, such as excellent mechanical and chemical stability. It is well know, the fracture behavior of monolithic silicon carbide is brittle and fails catastrophically. However, if the SiC fibers with an appropriate coating as reinforcement are incorporated with the silicon carbide matrix by specific fabrication process to form the ceramic matrix composite, the fracture characteristics of silicon carbide materials can be significantly improved. Figure 2 shows the typical polished morphologies and the fracture surface of near-net shape SiC/SiC composite. It is apparent that reinforcing fibers incorporated with dense matrix through an appropriate interphase. The significant fibers pull out could improve the fracture toughness and result in a pseudo-ductile fracture behavior. The tough ceramics as structural materials have the potential for being used up to about 1500 °C which is much higher than the operation temperature of superalloy (maximum 1100 °C close to the melting point). In different fields, such as advanced nuclear energy system, gas turbines for power/steam co-generation, heat exchangers and so on, they give different requirements for materials performance, but common features for high temperature technologies are excellent mechanical performance and environmental durability.

Figure 2. Typical polished morphology of SiC/SiC composite and its fracture surface with long fiber pull out.

The major advantages for SiC/SiC composite applied to engineering are: (i) high specific strength, (ii) superior high temperature strength and creep resistance, (iii) low thermal expansion coefficient and high thermal conductivity, (iv) low neutron irradiation-induced radioactivity in nuclear environments.

4

Jianjun Sha

SiC fibers with low oxygen content and high crystallinity, which derived from polycarbonsilane, are the backbone as reinforcements in load-bearing CMCs. For high temperature application, the most desired critical properties of SiC fibers are high strength and stiffness as well as the reliable retention of these properties throughout the service life of application. Low fiber strength and thermal stability could result in low fracture toughness and accelerate sub-critical crack propagation in CMCs. The key to the successful application of high temperature ceramic matrix composites (CMC) is the judicious selection and incorporation of ceramic fiber reinforcement with the proper chemical, physical and mechanical properties. Thus, the mechanical durability and the microstructure stability of SiC fibers are major concerns under severe environments. In practical service environments, rarely is one degradation mechanism operative, but several mechanisms operate simultaneously, which leading to the environment-pertinent degradation mechanism is complex for the SiC materials. For understanding the environmental durability and describing the response of reinforced fibers to service environments and further evaluation of reliability of CMCs, the investigation of thermal mechanical properties on SiC-based fibers in complex situation is essential. In this chapter, the investigations on mechanical properties and microstructure of SiC-based fibers are reviewed in terms of varied environments; some issues concerning the environmentpertinent properties are discussed.

2. Materials System and Characterization Technique 2.1. Materials System The first SiC-based Nicalon fiber was produced by Nippon Carbon which allowed nonoxide ceramic matrix composites to be developed. It made possible to use the SiC fiber as the reinforcement for high temperature structural materials in very severe environments. In order to improve the flexibility and strength so that the preform can be woven in complex shape, the fine diameter SiC fibers were developed. However the first SiC-based fibers are inherently limited by oxidation at very high temperatures. As a result of this limitation a renewal of interest has occurred in oxide resistance of SiC fibers by approaching to the near stoichiometric composition or addition of small amount additives to improve thermal stability at elevated temperatures. Efforts have been made to improve the high temperature properties of fine diameter SiC fibers by making them with compositions increasingly approaching stoichiometry. Based on the chemical composition and the fabrication process, the development of SiC-based fibers could be categorized into three generations as illustrated in Figure 3. The first fine diameter SiC fiber (Nicalon NL200) was synthesized by Yajima in Japan in 1970 [9]. The Nicalon fiber could be viewed as the representative of the first generation of SiC fibers (Figure 3). This fiber is thermodynamically unstable at high temperature, because it consists of SiC-nanocrystals (average size: 1-2 nm) and free carbon embedded in an amorphous SiCxOy matrix. The amorphous SiCxOy phase decomposes at temperature beyond 1300 ˚C [10-11], with a significant gaseous species evolution and SiC crystal growth [11-12]. In order to improve the high temperature resistance of the Si-C-O fiber, a new fabrication

High Temperature Mechanical Properties and Microstructure…

5

process of the fiber, radiation curing method [13-15], has been developed. Irradiation curing with an electron beam was applied to make the fiber infusible and cross linking. β-SiC crystallite (~2 nm)

Amorphous (Si-C-O)

Stoichiometric Crystallized

Reduced oxygen

Low thermal stability Low strength Low stiffness

Amorphous Si-C-O Fibers NicalonTM TyrannoTM-LoxM, etc.

β-SiC crystallite (>20 nm)

β-SiC crystallite (~5 nm)

Improved thermal stability Modest oxidation resistance

Increased elastic modulus Enhanced creep resistance Enhanced oxidation resistance

Low-Oxygen Si-C Fibers Hi-NicalonTM TyrannoTM-ZMI, etc.

Crystalline SiC Fibers NicalonTM Type-S TyrannoTM-SA

Figure 3. Illustration of R&D of SiC-based Fibers.

To avoid the thermal instability caused by the decomposition of oxycarbide phase (SiCxOy), in 1990, a nearly oxygen-free SiC fiber, Hi-Nicalon (Nippon-Carbon) was developed by melt spinning, electron beam curing and pyrolysis of a polycarbosilane precursor (PCS) under anaerobic conditions [15-16]. This fiber had a much higher thermal stability than the standard Nicalon fiber and was viewed as the representative of the second generation. However, the Hi-Nicalon fiber consists of not only SiC nanocrystals (average crystal size: 5 nm) but also excess of free carbon which affects its oxidation and creep resistance. To reduce the free carbon content and eventually improve the high temperature properties of the fibers, extensive efforts have been devoted to develop near stoichiometric and high crystallized SiC fibers. The precursor fiber can be sintered at high temperatures that excess carbon and oxygen are lost as volatile species to yield polycrystalline and near-stoichiometric SiC fiber. These fibers are advanced SiC fibers and generally called the third generation of SiC fibers (Figure 3), including Hi-Nicalon type S fiber [17], Tyranno SA fibers [18] and Sylramic SiC fiber [19]. The third generation of SiC fibers is oxygen-free and nearstoichiometric (atomic ratio: C/Si=1.00–1.08). Furthermore, their grain size is relatively large (20–200 nm) and their thermal stability is excellent. For enhancing the environmental durability of CMCs, SiC-based fibers with high crystallinity and near stoichiometry would be preferential. Based on this standing point, the following SiC-based fibers were used for the work presented in this chapter (Table 1).

6

Jianjun Sha Table 1. SiC-based fibers used for the work in this chapter and their properties provided by manufacture

SiC fiber HNL HNLS TySA

C/Si

Oxygen (wt%)

Strength (Gpa)

Modulus (Gpa)

Density (g/cm3)

Diameter (μm)

1.39 1.05 1.07

0.5 0.2 [u]e

where ς is a model parameter that allows to match the slope of the softening branch just beyond the attainment of the peak traction τM . Sometimes, a smooth transition from the elastic regime to the softening one turns out to be more representative of the actual interphase response. The nonlinear binding model, originally proposed in [30, 31] for metals and bimetallic compounds and later adopted also in nonlinear fracture mechanics [20, 21, 32], allows to describe such smooth transition through the following exponential (EXP) law (see Figure 2(c)): [u] τ = K[u] exp − (14) [u]e Besides the effective stiffness K and strength τM , a full characterization of the nonlinear behavior of the interface has to match the fracture energy, or work of separation G. In terms of effective quantities, G is defined as the amount of energy required to annihilate the interaction between the opening/sliding crack faces, i.e.: G=

Z∞

τ d[u]

(15)

0

From a model calibration perspective, parameters Q and ς in (12) and (13) can be tuned to accurately match the actual G, since they do affect only the softening branch of the interface law. On the other hand, after having assigned K in (14), only [u]e can be adjusted: therefore, both τM and G can not be accurately matched. In the exponential law, in fact, the following constraint holds: s KG (16) 2 =e τM

104

Stefano Mariani

e being the Nepero number. To avoid problems related to this fictitious constraint, a modified exponential law is here formulated as follows (see Figure 3): [u] q τ = K[u] exp − (17) [u]e where q shows up as an additional constitutive parameter. In law (17): K still represents the initial elastic stiffness; [u]e is a reference effective displacement discontinuity, while peak traction τM is attained at [¯ u] ≡ (1/q)1/q [u]e . The effective peak traction and fracture energy are affected by q, according to: 1/q 1 1 exp − τM =K[u]e q q K 2 G = [u]2e γf q q

(18)

γf being the gamma function. The dependence of τM and G on the parameter q is depicted in Figure 4: it can be seen that G is a monotonically decreasing function of q, whereas τM is lower-bounded by the value corresponding to q = 1. Having tuned K, this law thus allows the calibration of both τM and G. All the above laws but the piecewise linear one, assume that the interaction between the opening interface sides continues up to [u] → ∞, which seems not physical at the macroscale. To simulate delamination growth a breakdown threshold therefore needs to be introduced [33, 34]: as soon as the current traction τ reduces to a small fraction (say 5-10 %) of the peak value τM , the interaction is suddenly assumed to vanish. When unloading from the tensile envelope occurs, i.e. when [u] ˙ < 0, the above interface models can be viewed as either reversible, if τ always belongs to the envelope (leading to interface healing if softening has already started), or irreversible, if τ decreases following a radial path to the origin of the τ − [u] plane. These two alternative constitutive assumptions lead to different entries in the interface tangent stiffness matrix E Γ , linking rates of τ and [u] in the local n − sj1 − sj2 reference frame according to: τ˙ = E Γ [u] ˙

(19)

For additional details, readers are referred to [27, 28].

2.3.

Finite Element Formulation

The weak form of the equilibrium equations (1)-(3) reads: Z

Ω\Γ

T

εv σ dΩ =

Z

Ω\Γ

¯ − ̺¨ v (b u) dΩ + T

Z

Γτ

T

v τ¯ dΓτ −

nΓ Z X j=1 Γ

[v]T τ dΓj

∀v ∈ U0 (20)

j

where: v is the test function; εv = Cv; U is the trial solution space, collecting displacement fields u continuous in Ω\Γ, possibly discontinuous along each Γj and fulfilling the boundary condition (5) on Γu ; U0 is the relevant variation space, with zero prescribed

Failure of Layered Composites Subject to Impacts

105

Figure 3. effect of q on the modified exponential traction-displacement discontinuity law (17).

(a)

(b)

Figure 4. modified exponential law (17). Effects of q on (a) the effective peak traction τM and on (b) the effective fracture energy G. displacements on Γu . In (20), in view of the assumed linearized kinematics, the relation − Γj ≡ Γ+ j ≡ Γj for each interface has been exploited. Allowing for the elastic bulk constitutive law (8), the following variational statement is arrived at: Z Z nΓ Z X T T ¨ dΩ + find u ∈ U : ̺v u εv E Ω ε dΩ + [v]T τ dΓj Ω\Γ

j=1 Γ

Ω\Γ

=

Z

Ω\Γ

j

T¯

v b dΩ +

Z

Γτ

T

v τ¯ dΓτ

(21)

∀v ∈ U0

106

Stefano Mariani

Now, let the finite element approximation of the displacement and deformation fields in Ω\Γ be (see [35] for the notation): u∼ = Φuh

(22)

ε∼ = CΦuh = B Ω uh

(23)

where matrix Φ gathers the nodal shape functions, and vector uh collects the nodal displacements. If delamination is allowed to occur only along element boundaries, the discrete displacement jump field can be written: [u]

Γj

∼ = B Γj uh

j = 1, ..., nΓ

(24)

Owing to the discrete interpolation fields defined above, the semi-discretized equations of motion of the composite turn out to be: ¨ h + K Ω uh + Mu

nΓ X

Rj = F

(25)

j=1

where the mass matrix M , the bulk stiffness matrix K Ω , the internal force vectors Rj and the external load vector F are, respectively: M=

Z

̺ ΦT Φ dΩ

Z

B TΩ E Ω B Ω dΩ

Ω\Γ

KΩ =

Ω\Γ

Rj =

Z

(26)

B TΓj τ dΓj

Γj

F =

Z

Ω\Γ

T¯

Φ b dΩ +

Z

ΦT τ¯ dΓτ

Γτ

Smarter finite element formulations, like the extended or generalized ones [36,37], have been recently formulated to simulate mixed-mode crack growth in homogeneous solids, see e.g. [27, 38, 39]. These methodologies allow cracks to propagate not only along interelement edges, but also inside the elements; possible constraints imposed by the mesh layout on crack trajectories, evidenced e.g. in [40], can be therefore alleviated. When dealing with delamination in layered continua, where debonding occurs only along the a-priori known interlaminar surfaces, crack description looks simple and the aforementioned feature of the extended finite element method looses much of its advantages.

Failure of Layered Composites Subject to Impacts

2.4.

107

Time Integration

In our previous works [11, 15] it was shown that the time integration scheme can strongly affect the stability of the filtering procedure and, therefore, the accuracy of model parameter estimates. In case of impact loadings, which cause the propagation of shock waves inside the composite, the time marching algorithm has to dump the spurious high frequency oscillations linked to space discretization. Otherwise, the numerically computed displacement and velocity fields do not prove reliable enough to be compared to the experimental data. We adopt here the explicit α−method [41, 42] to advance in time the solution of the equations of motion (25), see also [19]. After having partitioned the time interval of interest Nt −1 according to [t0 tN ] = ∪i=0 [ti ti+1 ], at the end of the generic time step [ti ti+1 ] the solution to (25) is obtained according to the following predictor-integrator-corrector splitting: • predictor: 1 ˜ i+1 =ui + ∆t u˙ i + ∆t2 ( − β)¨ u ui 2 ˜˙ i+1 =u˙ i + ∆t(1 − γ)¨ ui u

(27) (28)

where ∆t = ti+1 − ti ; • explicit integrator:

¨ i+1 = M −1 F i+1+α − (1 + α) K u ˜ i+1 + u

where: F i+1+α = F (ti + (1 + α)∆t); R T B Γj τ˜ i+1 dΓj ;

X

Rji

j

˜ j + α Kui + R i+1

=

R

Γj

B TΓj τ i dΓj

X j

Rji

(29) j ˜ and Ri+1 =

Γj

• corrector: ¨ i+1 ui+1 =˜ ui+1 + ∆t2 β u ˜ ¨ i+1 u˙ i+1 =u ˙ i+1 + ∆tγ u

(30) (31)

In the above equations α, β and γ are algorithmic coefficients. To get a non-oscillatory velocity field, α = −0.3 has been adopted in all the forthcoming simulations; furthermore, β and γ have been finely tuned around the values allowing second-order accuracy in linear elasto-dynamics. To ensure accuracy of the filtering procedure, the time step size ∆t has been always set so as to fulfill the Courant condition in the bulk of the composite. Moreover, to speed up the explicit integrator phase (29), the mass matrix M has been diagonalized by means of a standard row-sum lumping procedure [42].

108

Stefano Mariani

Account taken of the explicit format of the integrator stage, the space-time discretized equations of motion of the laminate (state equations) can be formally written: ui+1 (32) z i+1 = u˙ i+1 = f zi (z i ) ¨ i+1 u where z is the structural state vector, and mapping f z turns out to be nonlinear because of the softening interface behavior.

3. 3.1.

Constrained Sigma-point Kalman Filtering Parameter Identification via Joint Kalman Filtering

According to a standard methodology [43], the calibration of constitutive laws can be pursued by Kalman filtering if a state vector x is obtained by joining the structural state vector z (see Eq. 32) with a vector ϑ gathering all the model parameters to be tuned. At time ti this can be written: zi xi = (33) ϑi While the current structural state z is always at least partially observed, model parameters to be identified can not be directly measured; by joining z and ϑ, state tracking can consistently improve model calibration. In case of irreversible constitutive laws, internal state variables must be gathered by x too, see e.g. [12, 19]. Allowing for model and measurement errors, the state-space model describing the evolution within the time interval [ti ti+1 ] of the joint state vector and its link with observations turns out to be: ( xi+1 = f i (xi ) + v i (34) = Hxi + wi yi where: y is the observation vector, which collects the measured components of the state vector; v is the process noises; w is the measurement noise. v, w are assumed to be additive, uncorrelated white and Gaussian processes, with zero mean and covariances V and W [44, 45]. Since z is defined according to Eq. (32), the observation equation in (34) shows up as a linear relation between y and x. On the contrary, the interface behavior renders the evolution equation f nonlinear. By way of the EKF [12, 46], within the time step the nonlinear mapping f is expanded in Taylor series, up to the first order, around the current estimates of the state vector and of model parameters. Bounds on the required accuracy of the initialization of x, and on the statistics of noises v and w to assure filter stability were provided for linear systems in [47] and, more recently, for nonlinear systems in [48]. Even in the absence of filter instabilities, the softening response of the interlaminar surfaces does not always guarantee the achievement of an accurate model calibration, see [15, 19].

Failure of Layered Composites Subject to Impacts

109

Table 1. Sigma-point Kalman filter. • Initialization at t0 : ˆ 0 =E[x0 ] x ˆ 0 ) (x0 − x ˆ 0 )T ] P 0 =E[(x0 − x • At ti , for i = 0, ..., N 1. Predictor phase: χ ˆi,j =ˆ xi + ∆χi,j

j = 0, ..., Nχ

ˆ− ˆ i,j ) χ i+1,j =f i (χ ˆ− x i+1 P− i+1

=

Nχ X

ˆ− ωj χ i+1,j

j=0 =R− i+1

+V

where R− i+1

=

Nχ X j=0

T ˆ− ˆ− ˆ− ˆ− χ ωj χ i+1 i+1 i+1,j − x i+1,j − x

2. Corrector phase: U ˆ− ˆ i =ˆ x x− i i + Gi y i − H x

− U P i =P − i − Gi HRi

where − T T GU HR− i =Ri H i H +W

−1

To improve the results when nonlinearities become dominant, the SPKF has been recently proposed [16, 49–51]. At the beginning of the time step, the probability distribution of x is deterministically sampled through a set of sigma-points χ ˆj , j = 0, ..., Nχ . These sigma-points are then allowed to evolve according to the nonlinear mapping f . The statistics of x at the end of the time step are finally obtained through a proper weighted averaging scheme [18]. This filtering procedure is detailed in Table 1, where E[2] represents the expected value of 2. The number of sigma-points and their location in the state vector space are accurately chosen, so as to achieve high accuracy in the estimated probability distribution of x at the end of each time step; when compared to the EKF, a better performance of the SPKF, also in terms of model calibration, is therefore expected [16]. The enhanced accuracy of the

110

Stefano Mariani

SPKF is discussed next; even though these results have been already presented elsewhere, they are here collected to show how possible constraints on parameter estimates, not dealt with by the standard SPKF, can be managed.

3.2.

Accuracy of a Constrained Sigma-point Transformation

In this Section we focus on the time interval [ti ti+1 ], but we avoid using indexes i and i + 1 to simplify the notation. Let x be a random vector, featuring at the beginning of the time step mean x ˆ and covariance P . We conceive x as the sum of the mean x ˆ and a zero-mean disturbance ∆x = x − x ˆ. If x undergoes a nonlinear transformation, governed by a mapping f analytic everywhere so that it can be expanded in Taylor series about x ˆ, at the end of the time step we get: ∞ X 1 n x = f (x) = f (ˆ x + ∆x) =f (ˆ x) + D n! ∆x n=1 −

(35)

n in the series expansion is: where, with a slight abuse in notation, the n−th order term D∆x

n D∆x

≡

!n Nx X ∂f ∆xℓ ∂xℓ x=ˆ x

(36)

ℓ=1

Nx being the number of components of the state vector x. Since the derivatives of f in (36) are evaluated at x = x ˆ, they are not random variables. The expected value of x− therefore reads: "∞ # X 1 x ˆ− = E[x− ] =E [f (ˆ x)] + E Dn n! ∆x n=1 (37) ∞ X 1 n =f (ˆ x) + E D∆x n! n=1

The relevant error covariance matrix is: h T i P − =E x− − x ˆ − x− − x ˆ− ! ∞ X 1 n n D∆x − E D∆x =E n! n=1

∞ X m 1 m D∆x − E D∆x m!

m=1

∞ X ∞ i X n h m T i 1 1 h n m T E D∆xD∆x − E D∆x E D∆x = n! m!

!T

(38)

n=1 m=1

Now, let us suppose to sample the probability distribution of x through a set of sigmapoints χ ˆj , j = 0, ..., Nχ , chosen around the current mean x ˆ according to: χ ˆj = x ˆ + ∆χj ,

j = 0, ..., Nχ

(39)

Failure of Layered Composites Subject to Impacts

111

where the terms ∆χj need to be determined. Similarly to x, within the time step each sigma-point undergoes the transformation: χ ˆ− j

∞ X 1 n = f (χ ˆj ) = f (ˆ x) + D n! ∆χj n=1

(40)

where: Dn ∆χj

≡

!n Nx X ∂f ∆χj ℓ ∂xℓ x=ˆ x

(41)

ℓ=1

At the end of the time step, the information in the evolved sigma-points are collected via a weighted averaging procedure to obtain: x ˆ− SPT

=

Nχ X

ωj χ ˆ− j

j=0

=

Nχ X j=0

(42)

Nχ ∞ X X 1 ωj D n ωj f (ˆ x) + ∆χj n!

n=1

j=0

where ωj are the weights of the sigma-point transformation relevant to the mean of x. The corresponding error covariance matrix is given by: P− SPT

=

Nχ X j=0

=

Nχ X j=0

T − − − ωj⋆ χ ˆ− − x ˆ − x ˆ χ ˆ SPT SPT j j

T Nχ Nχ ∞ ∞ X X X X 1 1 n D m ωj⋆ D ∆χj − ωr D n ωs D m ∆χr ∆χj − ∆χs n! m! n=1 m=1 r=0

s=0

(43)

where ωj⋆ are the weights of the sigma-point transformation relevant to the covariance of x. If x is a Gaussian random vector, its probability distribution is symmetric with respect n , n = 1, 3, 5, ..., are zero. To be to the mean x ˆ; therefore, all the odd central moments D∆x compliant with this condition, couples of sigma-points are symmetrically placed around x ˆ, according to [16]: ∆χ0 ∆χk ∆χ Nχ +k 2

=0 √ = +ψ P 1k √ = −ψ P 1k

k = 1, ...,

Nχ 2

(44)

√ Here: P represents the square root of matrix P , computed e.g. through a Cholesky factorization; ψ is a scaling parameter; 1k is a unit vector aligned with component k in the

112

Stefano Mariani

state vector space. The series expansions (37) and (42) agree up to third order if: P Nχ j=0 ωj = 1 P χ 1 N j=0 ωj D ∆χj = 0 2 PNχ 2 j=0 ωj D ∆χj = E D∆x PNχ ωj D 3 = 0

(45)

∆χj

j=0

To simplify the matter, let us assume ωj = ω for j = 1, ..., Nχ ; relations involving the first and third order terms in (45) are then automatically satisfied. Relations involving the zeroth and second order terms in (45) then furnish: ( ω0 + Nχ ω = 1 (46) 2ψ 2 ω = 1 A further condition to set ω0 , ω and ψ can be furnished by matching the diagonal entries of the fourth order terms (kurtoses) in (37) and (42). This leads to [19]: ω0 = 1 −

Nχ , 6

1 ω= , 6

ψ=

√

3

(47)

Here we propose an alternative condition to determine ω0 , ω and ψ, partially exploiting the features of the so-called scaled unscented transformation [52]. Let us assume that model parameters have to satisfy the constraints: ϑm ≤ ϑ ≤ ϑM

(48)

where ϑm and ϑM respectively gather the minimum and maximum (if any) allowed values of model parameters. This requirement must be fulfilled by each sigma-point χ ˆ− j , j = ˆ (and, therefore, 0, ..., Nχ . For j = 0 the conditions (48) are automatically satisfied, since x ˆ is computed at the end of the previous time step by averaging sigma-points all fulfilling ϑ) the constraints. Further, if ϑ = B ϑ x, B ϑ being a Boolean matrix, conditions (48) are satisfied by all the sigma-points if: ( ) M −ϑ ˆℓ ϑˆℓ − ϑm ϑ Nχ ℓ ℓ ; ℓ = 1, ..., Nϑ (49) ψ ≤ min , , k = 1, ..., ℓ ℓ 2 ak ak √ where ak = B ϑ P 1k , and Nϑ is the√number of model parameters in ϑ. In the forthcoming examples, we initially assume ψ = 3 (according to what reported in 47) and reduce its value if necessary, according to relation (49). ⋆ As for the error covariance matrix P − SPT , by letting ωj = ωj = ω for j = 1, ..., Nχ , we get: Nχ Nχ Nχ ∞ X ∞ X X X X 1 1 T ⋆ m T P− ωk D m ωj D n ωj D n ∆χk ∆χj D ∆χj + (ω0 + Nχ ω − 2) ∆χj SPT = n! m! n=1 m=1 j=0

j=0

k=0

(50)

Failure of Layered Composites Subject to Impacts

113

In case of Gaussian random variables, independently of the value of ω0⋆ , (38) and (50) agree up to the third order. Weight ω0⋆ can be set by matching part of the fourth order terms T (specifically those involving D 2∆χj D 2∆χk in 50), thereby obtaining (see also [52]): ω0⋆ = 4 −

Nχ − ψ2 ψ2

(51)

In what precedes we have assumed the mapping f to be analytic everywhere in the x space. If f is not differentiable, low order terms of the Taylor series expansions of mean and covariance get affected. It is difficult to quantify the discrepancies with respect to the analytic case, because they depend on whether the sigma-points sample the loci of nondifferentiability. However, it can be generally said that the order of accuracy is detrimentally affected.

4.

Results

To assess the performances of the proposed filtering approach in calibrating the interlaminar constitutive law while detecting impact-induced delamination, we first study a simple problem consisting of a two-layer composite stricken by a homogeneous impactor. Hence, two different impact tests on GRP composites [14, 53] are considered to mainly show the accuracy in detecting delamination in real-time. In all the cases, it is assumed that the contact between specimen and impactor is perfect (i.e. distributed all over their approaching surfaces) and that failure of the laminate occurs because of the propagation of dilatational plane waves in the through-the-thickness direction: the interlaminar surfaces are therefore subject to pure mode I loading.

4.1.

Pseudo-experimental Testings

As a starting benchmark, a pseudo-experimental testing condition is conceived. The pseudo-experimental response of the laminate to the impact loading has been computed by adding a white noise (of assigned variance) to sampled outcomes of finite element analyses. Even though this approach is sometimes criticized, being not clear whether one is testing with it the filtering approach or its implementation, it helps in getting insights into the performance of the filter in terms of stability and convergence rate. Indeed, calibration of interlaminar constitutive models may become difficult if delamination occurs almost instantaneously: the filter has to be highly sensitive to model parameters to promptly react to the information conveyed by measurements. This requires a careful setting of filter parameters, like P 0 and V . It is worth mentioning that, to further complicate the problem, the effects of the shape of the tensile envelope of interlaminar laws (at assigned strength and toughness) on the overall response of a laminate subject to impacts have not been thoroughly understood yet: depending on the loading and boundary conditions, on the composite geometry and on the stacking sequence, in some circumstances the shape affects the response, whereas in others it does not [54]. The capabilities of the SPKF are therefore first assessed through a simple test: a twolayer composite is stricken by a homogeneous impactor. The laminae and the impactor are

114

Stefano Mariani

Figure 5. impact on a two-layer composite. Space-time diagram (the vertical dashed line here represents the possibly debonding surface when a brittle, homogeneous material is subject to the same impact). assumed to be isotropic and elastic, featuring Young’s modulus E = 10 GPa, Poisson’s ratio ν = 0.35 and mass density ̺ = 1500 kg/m3 (see also [11]). Each lamina and the impactor are 0.75 mm in thickness. Target mechanical properties of the interlaminar surfaces are assumed: 2K =277.09 (N/mm3 ) τM =75 G =0.15

(MPa)

(52)

(N/mm)

According to the space-time diagram of Figure 5, failure can occur only along the interlaminar surface because of the interaction of the two release waves propagating inwards from the free surfaces of impactor and specimen. Two different values of the velocity v of the impactor are considered. In a first case v = 10.19 m/s leads to the propagation in the through-the-thickness direction of a compressive/tensile wave of amplitude τ¯ = 50 MPa, which does not cause interface failure. In a second case v = 20.38 m/s causes laminate failure, i.e. whole delamination, because of the propagation of a compressive/tensile wave of amplitude τ¯ = 100 MPa. Outcomes of the two tests are respectively reported in Figures 6 and 7, in terms of time evolution of the free surface velocity velocity u˙ r at the rear laminate surface, of the opening displacement discontinuity [u] and of the normal traction τ (here and in what follows the subscript n has been dropped to simplify the notation). Results are shown for all the constitutive models described in Section 2.2., having assumed q = 1 for the modified exponential interface law (17). For comparison purposes, the response of an interface-free specimen is reported too; in such a case, the purely elastic behavior of the material leads to the propagation of sharp fronts of a shock wave. If delamination is not incepted (¯ τ = 50 MPa), the response is almost independent of the shape of the interface law. Only in the presence of an interface that behaves according to the exponential model, the pre-peak nonlinearity of the constitutive law (see Figure 2(a))

Failure of Layered Composites Subject to Impacts

115

(a)

(b)

(c)

Figure 6. impact on a two-layer composite, τ¯ = 50 MPa. Effects of the interlaminar laws on the time evolution of (a) the free surface velocity u˙ r , of (b) the displacement discontinuity [u] and (c) relevant traction τ along the interface. leads to a larger opening [u] of the interlaminar surface when subject to a tensile stress. For any constitutive model, the signature of the interface is shown in Figure 6(a) by the delay in the sudden changes of u˙ r with respect to the reference, interface-free solution. This delay, which grows in time, is caused by the compliance of the interface, that is additional to the bulk one. In case of failure (¯ τ = 100 MPa), the free surface velocity u˙ r is affected by the interface model only when the waves, traveling across the interlaminar surface while softening is taking place, reach the rear surface; this occurs in the present case around 1µs after the impact, see Figure 7(a). After failure, the rear lamina detaches from the front one and freely flies off, as testified by the diverging [u] history in Figure 7(b). Part of the shock waves then get confined inside the back lamina: this explains the subsequent doubling of the drops in the u˙ r evolution. It is worth noting that the time elapsed between softening

116

Stefano Mariani

(a)

(b)

(c)

Figure 7. impact on a two-layer composite, τ¯ = 100 MPa. Effects of the interlaminar laws on the time evolution of (a) the free surface velocity u˙ r , of (b) the displacement discontinuity [u] and (c) relevant traction τ along the interface. inception (t ∼ = 0.72 µs) and whole failure of the interface (t ∼ = 0.9 µs), see Figure 7(c), is very short; only the information on this failure event, constituting the so-called pull-back signal (PBS), conveyed by the shock waves to the free laminate surface, can be used by the filter to calibrate the interface law. The effects on the PBS of the shape of the tensile envelope and of the strength τM and toughness G values need to be assessed. In the absence of any dissipation mechanisms, in this test the free surface velocity u˙ r would drop to zero at t = 0.917 µs (see Figure 6(a)); in case of delamination, the minimum attained velocity after the arrival of the unloading tensile wave and the shape of the PBS do furnish information on the interface response. To understand the roles of interface law, strength and toughness, the results of a parametric analysis are shown in Figure 8: for any interface model, τM and G are varied by 20% at most with respect to the target values (52). The piecewise linear and linear-exponential

Failure of Layered Composites Subject to Impacts

(a)

(b)

(c)

(d)

(e)

(f)

117

Figure 8. impact on a two-layer composite, τ¯ = 100 MPa. Effects of the interface strength τM (left column) and toughness G (right column) on the pull-back signal. (a-b) piecewise linear law (12); (c-d) linear-exponential law (13); (e-f) exponential law (14).

118

Stefano Mariani

laws, having a common initial elastic phase in tension, lead to a common descending branch in the PBS. At variance, the local tangent stiffness of the exponential law in the hardening phase is affected by τM and G: the slope of the descending branch of the PBS is therefore affected by τM and G too. Independently of the interface law, τM turns out to affect the starting stage of debonding, whereas G affects its tail and the time needed to complete it; this is clearly evidenced by the PBS, since τM modifies the minimum attained velocity, whereas G influences only the ascending branch with no effects on the pull-back velocity. From a model calibration perspective, it is clear that the SPKF has chances to improve parameter estimates only in the time interval 0.9 ≤ t ≤ 1.2 µs. It is therefore hard to figure out from the previous plots whether the effects of tensile envelope, τM and G can be actually interpreted by the filter to improve model calibration. The performances of the SPKF are hence tested here not only looking at parameter estimates, but also checking its capability to detect whether a laminate is failing and, in case of delamination, where it actually takes place. Typical results of the filtering procedure are depicted in Figures 9 and 10; in this case the pseudo-experimental data, which consist in the free surface velocity alone, have been supposed very accurate, featuring a standard deviation δ = 0.33 m/s (the measurement error covariance matrix W becomes scalar-valued, with entry W = δ 2 ). As far as the process covariance matrix V is concerned, in case of pseudo-experimental testing it can be assumed to be vanishing, since the filter employs the same structural model adopted to get the pseudo-experimental data. Components of P 0 instead need to be finely tuned to enhance filter convergence [11, 15]. Figure 9 shows the obtained estimates of τM and G as a function of their initial guess in ˆ 0 (here respectively denoted by τM,0 and G0 ), for all the interface models. These estimates x evolve from τM,0 and G0 once the PBS is processed by the filter; after that, they become stationary. The tracked state of the laminate is shown in Figure 10 in terms of predicted interface opening [u] and free surface velocity u˙ r . Knowing the target response of the composite to the impact, here denoted by the dashed lines, allows to certify stability and convergence of the SPKF, no matter if displacement is diverging in a part of the system and what kind of interface constitutive law has been adopted. It can be seen that estimates get enhanced as soon as the filter senses the PBS: in fact, the sudden changes in the estimate of [u] show up only while processing the PBS, starting from t ∼ = 0.9 µs. These outcomes testify that the SPKF is very efficient in tracking the state of the laminate, i.e. in understanding whether the structure is failing or not. Model calibration is instead less accurately accomplished: independently of the interface law, τM is quite precisely estimated, provided the initial guess τM,0 is not too far from the target value, whereas G can be hardly inferred. These conclusions are in agreement with the results of the parametric analysis: while τM affects the whole PBS, G affects only its ascending branch. Therefore, filtering out from u˙ r the effects of G alone turns out to be extremely difficult. In case of a much higher scattering of pseudo-experimental data (δ = 3.3 m/s), see Figure 11, results loose accuracy as for the calibration task. Contrariwise, state tracking maintain accuracy: even though measurements contain poor information, the SPKF is again able to provide the evolution of the free surface velocity in the PBS.

Failure of Layered Composites Subject to Impacts

(a)

(b)

(c)

(d)

(e)

(f)

119

Figure 9. impact on a two-layer composite, τ¯ = 100 MPa (W=10−1 m2 /s2 ). Effects of the initialization values τM,0 and G0 on the converged estimates of τM (left column) and G (right column). (a-b) piecewise linear law; (c-d) linear-exponential law; (e-f) exponential law.

120

Stefano Mariani

(a)

(b)

(c)

(d)

(e)

(f)

Figure 10. impact on a two-layer composite, τ¯ = 100 MPa (W=10−1 m2 /s2 ). Evolution in time of interface opening [u] (left column) and free surface velocity u˙ r (right column), and comparison among tracked state (orange squares), actual state (dashed lines) and pseudoexperimental data (blue circles). (a-b) piecewise linear law; (c-d) linear-exponential law; (e-f) exponential law.

Failure of Layered Composites Subject to Impacts

(a)

(b)

(c)

(d)

(e)

(f)

121

Figure 11. impact on a two-layer composite, τ¯ = 100 MPa (W=10 m2 /s2 ). Evolution in time of interface opening [u] (left column) and free surface velocity u˙ r (right column), and comparison among tracked state (orange squares), actual state (dashed lines) and pseudoexperimental data (blue circles). (a-b) piecewise linear law; (c-d) linear-exponential law; (e-f) exponential law.

122

Stefano Mariani

(a)

(b)

Figure 12. impact on a 7-layer composite [53]. (a) space-time diagram (the vertical dashed line here represents the possibly debonding surface when a brittle, homogeneous material is subject to the same impact), and (b) experimentally measured free surface velocity.

4.2.

Actual Experimental Testings

To finally check the performances of the SPKF when dealing with multi-layered composites, we consider two of the experiments reported in [53] and [14]. In the first experiment (experiment FY06001 in [53]), the specimen is a 7-layer composite plate; each lamina is 1.37 mm in thickness, and is made of a balanced 5-harness satin weave E-glass and LY564 epoxy. The wave speed in the through-the-thickness direction is 3.34 km/s, while the mass density is ̺ = 1885 kg/m3 [53]. This laminate was subject to a plane impact, stricken by an aluminum impactor (12.5 mm thick) flying at velocity v = 71 m/s. The relevant space-time diagram is shown in Figure 12, along with the free surface velocity profile measured via a velocity interferometer for any reflector (VISAR). Account taken of the high accuracy of the experimentally measured u˙ r , the identification procedure have furnished the results reported in Figure 13 in terms of time evolution of estimates of τM and G as a function of their initialization values within the domain: Cϑ = {50 ≤ τM,0 ≤ 250 (MPa), 0.5 ≤ G0 ≤ 2.5 (N/mm)}

(53)

Failure of Layered Composites Subject to Impacts

(a)

(b)

(c)

(d)

(e)

(f)

123

Figure 13. impact on a 7-layer composite [53]. Evolution in time of the estimated values of τM (left column) and G (right column). (a-b) piecewise linear law; (c-d) linear-exponential law; (e-f) exponential law.

124

Stefano Mariani

(a)

(b)

(c)

(d)

(e)

(f)

(g)

Figure 14. impact on a 7-layer composite [53]. Evolution in time of (a) free surface velocity u˙ r and (b-g) estimated interface openings [u]1 − [u]6 .

Failure of Layered Composites Subject to Impacts

125

(a)

(b)

Figure 15. impact on a 11+11-layer composite [14]. (a) space-time diagram (the vertical dashed line here represents the possibly debonding surface when a brittle, homogeneous material is subject to the same impact), and (b) experimentally measured free surface velocity. Converged estimates of τM are in good agreement with the spall strength of 119.5 MPa reported in [53]; on the other hand, final estimates of G are well representative for this kind of composites. Figure 14 reports the estimated state of the specimen: the capability to track the measured free surface velocity and to foresee delamination along the third interlaminar surface away from the impact plane, is evidenced. This latter result, allowing also for wave dispersion caused by interlaminar surfaces and inner inhomogeneities of the composite, well agrees with the state-space diagram of Figure 12(a). In the second experiment (experiment 1 in [14]), a GRP specimen, 7.02 mm thick, is backed by another GRP plate, 6.91 mm thick; both laminates are made of 11 plies. The wave speed in the through-the-thickness direction now amounts to 3.19 km/s, and the mass density to ̺ = 1867 kg/m3 [14]. The specimen is stricken by a 5-layer GRP flyer, 2.96 mm in thickness, flying at velocity v = 85 m/s. The corresponding space-time diagram, and the free surface velocity profile measured via a VISAR are reported in Figure 15. Because of the test set-up, the release waves interact causing delamination inside the back plate.

126

Stefano Mariani

(a)

(b)

(c)

(d)

(e)

(f)

(g)

(h)

(i)

(j)

(k)

Figure 16. Impact on a 11+11-layer composite [14]. Evolution in time of (a) free surface velocity u˙ r and (b-k) estimated interface openings [u]1 − [u]10 in the back plate.

Results of the filtering process are reported in Figure 16 is terms of tracked free surface velocity and estimated displacement jumps along all the interfaces inside the back plate (sequence starts at the specimen-back plate contact surface). These estimations turn out once again to be independent of the interface law and of the initialization values of τM and

Failure of Layered Composites Subject to Impacts

127

G inside the domain: Cϑ = {25 ≤ τM,0 ≤ 100 (MPa), 0.1 ≤ G0 ≤ 0.6 (N/mm)}

(54)

While the free surface velocity is accurately tracked, delamination is foreseen to take place along the 7-th interlaminar surfaces, in agreement with the results of [11, 14]. As far as model calibration is concerned, outcomes turn out to be qualitatively in agreement with those already reported for the previous tests.

5.

Conclusion

In this Chapter we have addressed some issues related to constitutive modeling and parameter identification in finite element simulations of layered composites subject to impacts. Assuming the impact energy to be high enough to cause damage spreading inside the interlaminar resin-enriched phases, but not high enough to result in penetration of the impactor accompanied by intralaminar damage, a numerical scheme for structural-level analyses has been revised. Within this scheme the laminae are assumed to behave elastically, whereas dissipation mechanisms are lumped onto zero-thickness interlaminar surfaces. Along these interlaminar surfaces strength reduction, eventually leading to delamination, is governed by softening interface constitutive laws linking tractions to displacement jumps. Interface laws are known to be difficult to calibrate, since direct testing on a single interlaminar phase can not be devised. Here we have offered a sigma-point Kalman filtering approach to estimate uncertain model parameters of the aforementioned interface laws. This technique outperforms most of the customarily adopted ones, since it efficiently deals with nonlinearities, which are a result of interlaminar strength degradation in the case under study. The performances of the filtering procedure have been assessed through pseudoexperimental testings on a two-layer composite, and through real testings on multi-layer glass fiber reinforced plastic composites. It has been shown that the state of the composite, including delamination inception and growth, is always tracked with a noteworthy level of accuracy. Due to the fast failure events, model calibration is instead less accurately performed and sometimes requires initialization values of uncertain model parameters to be appropriately chosen to avoid biased estimates.

References [1] S. Abrate. Impact on composite structures. Cambridge University Press, 1998. [2] H.D. Espinosa, S. Dwivedi, P.D. Zavattieri, and G. Yuan. A numerical investigation of penetration in multilayered material/structure systems. International Journal of Solids and Structures, 35:2975–3001, 1998. [3] O. Allix and P. Ladev´eze. Interlaminar interface modelling for the prediction of delamination. Composite Structures, 22:235–242, 1992.

128

Stefano Mariani

[4] A. Corigliano. Formulation, identification and use of interface elements in the numerical analysis of composite delamination. International Journal of Solids and Structures, 30:2779–2811, 1993. [5] A. Corigliano and O. Allix. Some aspects of interlaminar degradation in composites. Computer Methods in Applied Mechanics and Engineering, 185:203–224, 2000. [6] A. Corigliano and S. Mariani. Simulation of damage in composites by means of interface models: parameter identification. Composites Science and Technology, 61:2299– 2315, 2001. [7] G. Alfano and M.A. Crisfield. Finite element interface models for the delamination analysis of laminated composites: mechanical and computational issues. International Journal for Numerical Methods in Engineering, 50:1701–1736, 2001. [8] A. Corigliano. Damage and fracture mechanics techniques for composite structures. In I. Milne, R.O. Ritchie, and B. Karihaloo, editors, Comprehensive Structural Integrity, volume 3, chapter 9, pages 459–539. Elsevier Science, 2003. [9] A. Corigliano and S. Mariani. Parameter identification of a time-dependent elasticdamage interface model for the simulation of debonding in composites. Composites Science and Technology, 61:191–203, 2001. [10] A. Corigliano and S. Mariani. Identification of a constitutive model for the simulation of time-dependent interlaminar debonding processes in composites. Computer Methods in Applied Mechanics and Engineering, 191:1861–1894, 2002. [11] S. Mariani and A. Corigliano. Impact induced composite delamination: state and parameter identification via joint and dual extended Kalman filters. Computer Methods in Applied Mechanics and Engineering, 194:5242–5272, 2005. [12] S. Bittanti, G. Maier, and A. Nappi. Inverse problems in structural elastoplasticity: a Kalman filter approach. In A. Sawczuk and G. Bianchi, editors, Plasticity today. Modelling, Methods and Applications, pages 311–329. Elsevier Applied Science Publishers, 1984. [13] A. Corigliano, S. Mariani, and B. Orsatti. Identification of Gurson-Tvergaard material model parameters via Kalman filtering technique - I. Theory. International Journal of Fracture, 104:349–373, 2000. [14] H.D. Espinosa, S. Dwivedi, and H.-C. Lu. Modeling impact induced delamination of woven fiber reinforced composites with contact/cohesive laws. Computer Methods in Applied Mechanics and Engineering, 183:259–290, 2000. [15] A. Corigliano and S. Mariani. Parameter identification in explicit structural dynamics: performance of the extended Kalman filter. Computer Methods in Applied Mechanics and Engineering, 193:3807–3835, 2004.

Failure of Layered Composites Subject to Impacts

129

[16] S.J. Julier, J. Uhlmann, and H.F. Durrant-Whyte. A new method for the nonlinear transformation of means and covariances in filters and estimators. IEEE Transactions on Automatic Control, 45:477–482, 2000. [17] T. Lefebvre, H. Bruyninckx, and J. De Schutter. Kalman filters for nonlinear systems: a comparison of performance. International Journal of Control, 77:639–653, 2004. [18] K. Ito and K. Xiong. Gaussian filters for nonlinear filtering problems. IEEE Transactions on Automatic Control, 45:910–927, 2000. [19] S. Mariani and A. Ghisi. Unscented Kalman filtering for nonlinear structural dynamics. Nonlinear Dynamics, 49:131–150, 2007. [20] A. Corigliano, S. Mariani, and A. Pandolfi. Numerical modeling of rate-dependent debonding processes in composites. Composite Structures, 61:39–50, 2003. [21] A. Corigliano, S. Mariani, and A. Pandolfi. Numerical analysis of rate-dependent dynamic composite delamination. Composites Science and Technology, 66:766–775, 2006. [22] R. Lund and J. Fish. Space-time multiscale laminated theory. International Journal of Multiscale Computational Engineering, 2:26–47, 2004. [23] S. Mariani, A. Pandolfi, and R. Pavani. Coupled space-time multiscale simulations of dynamic delamination tests. Materials Science, 23:509–519, 2005. [24] R.R. Talreja Y.W. Kwon, D.H. Allen, editor. Multiscale Modeling and Simulation of Composite Materials and Structures. Springer, 2007. [25] G.T. Camacho and M. Ortiz. Computational modelling of impact damage in brittle materials. International Journal of Solids and Structures, 33:2899–2938, 1996. [26] Y. Arun Roy and R.H. Dodds. Simulation of ductile crack growth in thin alluminum panels using 3-D surface cohesive elements. International Journal of Fracture, 110:21–45, 2001. [27] S. Mariani and U. Perego. Extended finite element method for quasi-brittle fracture. International Journal for Numerical Methods in Engineering, 58:103–126, 2003. [28] C. Comi and S. Mariani. Extended finite element simulation of quasi-brittle fracture in functionally graded materials. Computer Methods in Applied Mechanics and Engineering, 196:4013–4026, 2007. [29] S. Li, M.D. Thouless, A.M. Waas, J.A. Schroeder, and P.D. Zavattieri. Mixed-mode cohesive-zone models for fracture of an adhesively bonded polymer matrix composite. Engineering Fracture Mechanics, 73:64–78, 2006. [30] J.H. Rose, J. Ferrante, and J.R. Smith. Universal binding energy curves for metals and bimetallic interfaces. Physical Review Letters, 47:675–678, 1981.

130

Stefano Mariani

[31] J.H. Rose, J.R. Smith, and J. Ferrante. Universal features of bonding in metals. Physical Review B, 28:1835–1845, 1983. [32] X.-P. Xu and A. Needleman. Numerical simulation of fast crack growth in brittle solids. Journal of the Mechanics and Physics of Solids, 42:1397–1434, 1994. [33] A. Needleman and A.J. Rosakis. The effect of bond strength and loading rate on the conditions governing the attainment of intersonic crack growth along interfaces. Journal of the Mechanics and Physics of Solids, 47:2411–2449, 1999. [34] C.M. Landis, T. Pardoen, and J.W. Hutchinson. Crack velocity dependent toughness in rate dependent materials. Mechanics of Materials, 32:663–678, 2000. [35] O. C. Zienkiewicz and R. L . Taylor. The finite element method, volume II. McGrawHill, London, 1989. [36] N. Mo¨es, J. Dolbow, and T. Belytschko. A finite element method for crack growth without remeshing. International Journal for Numerical Methods in Engineering, 46:131–150, 1999. [37] T. Strouboulis, K. Copps, and I. Babuˇska. The generalized finite element method. Computer Methods in Applied Mechanics and Engineering, 190:4081–4193, 2001. [38] G.N. Wells and L.J. Sluys. A new method for modelling cohesive cracks using finite elements. International Journal for Numerical Methods in Engineering, 50:2667– 2682, 2001. [39] C. Comi, S. Mariani, and U. Perego. An extended FE strategy for transition from continuum damage to mode I cohesive crack propagation. International Journal for Numerical and Analytical Methods in Geomechanics, 31:213–238, 2007. [40] M. Jirasek and T. Zimmerman. Embedded crack model: II. Combination with smeared cracks. International Journal for Numerical Methods in Engineering, 50:1291–1305, 2001. [41] H.M. Hilber, T.J.R. Hughes, and R.L. Taylor. Improved numerical dissipation for time integration algorithms in structural dynamics. Earthquake Engineering and Structural Dynamics, 5:283–292, 1977. [42] T.J.R. Hughes. The finite element method. Linear static and dynamic finite element analysis. Dover Publications, 2000. [43] L. Ljung. System identification. Theory for the user. Prentice Hall, second edition, 1999. [44] A. Gelb. Applied optimal estimation. The M.I.T. Press, 1974. [45] E.A. Wan and A.T. Nelson. Dual extended Kalman filter methods. In S. Haykin, editor, Kalman filtering and neural networks, pages 123–173. John Wiley & Sons, Inc., 2001.

Failure of Layered Composites Subject to Impacts

131

[46] R. E. Kalman and R. S. Bucy. New results in linear filtering and prediction theory. ASME Journal of Basic Engineering, 83D:95–108, 1961. [47] L. Ljung. Asymptotic behavior of the extended Kalman filter as a parameter estimator for linear systems. IEEE Transactions on Automatic Control, AC-24:36–50, 1979. [48] K. Reif, S. G¨ unther, E. Yaz, and R. Unbehauen. Stochastic stability of the discretetime extended Kalman filter. IEEE Transactions on Automatic Control, 44:714–728, 1999. [49] S.J. Julier and J.K. Uhlmann. A general method for approximating nonlinear transformations of probability distributions. Technical report, RRG, Department of Engineering Science, University of Oxford, 1996. [50] S.J. Julier, J. Uhlmann, and H.F. Durrant-Whyte. A new approach for filtering nonlinear systems. In Proceedings of the American Control Conference, pages 1628–1632, Seattle, June 1995. [51] E.A. Wan and R. van der Merwe. The unscented Kalman filter. In S. Haykin, editor, Kalman filtering and neural networks, pages 221–280. John Wiley & Sons, Inc., 2001. [52] S.J. Julier. The scaled unscented transformation. In Proceedings of the American Control Conference, volume 6, pages 4555–4559, Anchorage, May 2002. [53] F. Yuan, L. Tsai, V. Prakash, A.M. Rajendran, and D.P. Dandekar. Spall strength of glass fiber reinforced polymer composites. International Journal of Solids and Structures, 44:7731–7747, 2007. [54] G. Alfano. On the influence of the shape of the interface law on the application of cohesive-zone models. Composites Science and Technology, 66:723–730, 2006.

In: Strength of Materials Editors: G. Mendes and B. Lago, pp. 133-155

ISBN: 978-1-60741-500-8 © 2009 Nova Science Publishers, Inc.

Chapter 4

CURRENT STATE OF THE ART OF THE CERAMIC COMPOSITE MATERIAL BIOLOX®DELTA Meinhard Kuntz1, Bernard Masson2 and Thomas Pandorf1 1

CeramTec AG, Plochington, Germany 2 CeramTec AG, Pechabou, France

Abstract An extensive overview about the state of the art of the ceramic composite material BIOLOX®delta is given. The unique properties rely on a well defined alumina based fine composite microstructure which is mainly achieved by high temperature solid body reaction of the different ceramic phases during sintering. Zirconia comprises 17 % of the total volume. The tetragonal phase of zirconia is stabilized chemically and mechanically. The high strength and toughness of the material depend on transformation toughening of the zirconia which is clearly shown by various experimental results. The excellent mechanical properties are reproduced batch by batch with a very low scatter. The outstanding properties of the material BIOLOX®delta support advantageous properties of the final product, e.g. ceramic hard-hard bearings for hip arthroplasty. The burst load of the components is significantly increased. It is shown that the design of the components is also very important for the reliability and the ultimate properties of the system. Wear properties at severe conditions are significantly improved by using the new composite material BIOLOX®delta in comparison to pure alumina. Phase transformation of zirconia from the tetragonal to the monoclinic phase due to hydrothermal aging is extensively discussed. Due to the particular distribution and stabilization of the zirconia particles instable aging effects are not possible in this material. After very long time of accelerated aging conditions an increase of monoclinic phase is found – however, it is shown that dynamic and static properties of BIOLOX®delta are not influenced by this effect.

1. Introduction Since 2001 more than 500.000 artificial hip joints with components of the new high performance ceramic composite BIOLOX®delta have been successfully implanted on a

134

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

global basis. Due to the unique strength and toughness of this material the risk of fracture has been substantially reduced when compared to conventional ceramic materials. The outstanding properties of BIOLOX®delta rely on complex reinforcing mechanisms. Therefore, it is necessary to assess if reinforcement is maintained throughout the life-time of the artificial joint which is anticipated to exceed more than 20 years. Furthermore, it is shown that the challenging production of BIOLOX®delta is reproduced at a high quality from batch to batch. Within the scope of this technical contribution the composite ceramic BIOLOX®delta is extensively described and analyzed. The composition and the material properties are presented based on data of regular production lots. It is shown that the advantageous properties of this material are based on the reinforcing mechanisms which are activated due to the unique composition of this material. The particular effect of monoclinic phase transformation and hydrothermal aging is described in detail based on general mechanisms and specific analysis of phase transformation in BIOLOX®delta. Furthermore, experimental data are provided which describe the long term properties of the material, in particular with respect to hydrothermal phase transformation of zirconia in combination with wear and cyclic load conditions.

2. International Material Standards BIOLOX®delta is a modern ceramic composite material for biomedical applications. The main components of the composite are alumina and zirconia. There are ISO standards available for bioceramics of high purity alumina (ISO 6474 - 1) and high purity zirconia (ISO 13356). However, these standards are not directly applicable for the composition of BIOLOX®delta. The ISO organisation is already on the way to prepare a new standard which is applicable for BIOLOX®delta and other similar composite materials (ISO 6474 - 2). The new standard will be released presumably in 2010. Meanwhile, it is helpful to refer and compare the properties of BIOLOX®delta to the draft of the new ISO 6474-2 and the other international material standards which are applicable for related high purity bioceramics.

ISO 6474 – 1 Implants for Surgery – Ceramic Materials - Part 1: Ceramic Materials Based on High Purity Alumina The current version of this standard was released in 1994. The material properties which are defined here reflect typical properties of high quality pure alumina. Strength and toughness which are required according to this standard are significantly lower than those which are available with the composite material BIOLOX®delta. Today, the experts of the ISO working group agree that some details of the current ISO 6474 do not represent the state of the art. Thus, a new version of ISO 6474 - 1 is being preparedwhich is already published as a Draft International Standard (ISO/DIS). Most technical details in this version are already finally implemented. Some details (fracture

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

135

toughness, microstructure) are still under discussion. Presumably, the final release of the new standard will be in 2009. Comment: There is a similar ASTM standard F 603 for the same application and material type. The required material properties are comparable.

ISO 6474 – 2. Implants for Surgery – Ceramic Materials - Part 2: Composite Materials Based on a High Purity Alumina Matrix with Zirconia Reinforcement A standard which is applicable for alumina zirconia composite materials is under preparation. Such composite materials are distinguished in those where the main phase is alumina (ZTA = zirconia toughened alumina) and those where zirconia is the dominating phase (ATZ= alumina toughened zirconia). Both material types are available for biomedical applications. The basic physical properties (e.g. hardness, thermal conductivity) of a composite are primarily derived from the main phase. It is thus useful to describe alumina based zirconia toughened materials parallel to pure alumina materials. Consequently, the new standard has been proposed as part 2 of the established standard ISO 6474 for pure alumina. This concept has been discussed at the ISO TC 150 meetings and was approved by the international experts. The new standard ISO 6474 - 2 is accepted as a Working Draft. It covers all material properties (except of Young´s modulus) which are defined in ISO 6474 - 1. Additionally, the specific subjects of hydrothermal aging and radioactivity, which are relevant for zirconia toughened materials is also included. ISO 6474 – 2 is defined such that a broad range of inorganic compositions are included. A composition of ≥ 60 wt. % alumina and ≥ 10 wt. % zirconia is required. Other ingredients are allowed. The new standard is not exclusively designated for BIOLOX®delta. So far there is no ASTM standard for alumina zirconia composite biomaterials available.

ISO 13 356. Implants for Surgery –Ceramic Materials Based on YttriaStabilized Tetragonal Zirconia (Y-TZP) This standard was revised and published in 2008 as an International Standard (ISO). In contrast to pure alumina, zirconia as a ceramic material can not be produced without a significant amount of other substances for phase stabilization. Several elements are known which are applicable. ISO 13356 is only focussed on Yttria as the stabilizing element. A specific range of Y content is predetermined. It should be noted that the typical range of Y in pure zirconia materials can be different to the required amount of Y in alumina zirconia composites. This issue is thoroughly discussed in chapter 4. Pure zirconia bioceramics can be applied either for biomedical bearings (e.g. hip or knee) or for dental applications. ISO 13 356 does not distinguish between these different applications. As a specific issue of zirconia a test for accelerated hydrothermal aging is required.

136

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

Table 1 gives an overview of the required properties of the 3 standards. The material properties according to the latest revised versions are chosen Table 1. Required material properties according to the ISO standards 6474 – 1 (pure alumina), ISO 6474 – 2 (alumina – zirconia composite) and ISO 13 356 (zirconia). ISO Standard Material Average Bulk density Chemical Composition

Grain Size

ISO 6474 - 1 Pure Alumina ≥ 3,94 g/cm3

ISO 13 356 Zirconia ≥ 6,00 g/cm3

ISO 6474 – 2 Alumina Zirconia ≥ 98,7 %

wt%

Al2O3 ≥ 99,7 MgO ≤ 0,2 Impurities ≤ 0,1

Al2O3 60 - 90 ZrO2+HfO2 10 - 30 Additives ≤ 10 Impurities ≤ 0,2

µm

MV ≤ 2,5 SD ≤ 40 %

ZrO2+HfO2+Y2O3 ≥ 99,0 Y2O3 4,5 – 6,0 HfO2 ≤ 5 Al2O3 ≤ 0,5 Others ≤ 0,5 MV ≤ 0,4

Unit

MPa Strength Weibull Modulus (4 pt bending) Young´s modulus GPa Fracture MPa Toughness m Hardness HV1 Wear Resistance Cyclic fatigue limit Amount of monoclinic phase Accelerated Aging

GPa

Radioactivity

Bq / kg

%

≥ 500 ≥8

≥ 800

Al2O3 MV ≤ 1,5 ZrO2 MV ≤ 0,6 SD ≤ 40 % ≥ 1000 ≥ 10

≥ 380 ≥ 2,5

≥ 4,0

≥ 18 Info No failure at 200 MPa

≥ 17 Info No failure at 400 MPa

No failure at 320 MPa ≤ 20 ≤ 25 % monocl. phase strength decrease not more than 20% ≤ 200

Accomplish requirements described above ≤ 100

Note: The values of ISO 6474 – 1 & 2 are not finally fixed at the date of this publication.

3. Description of BIOLOX®delta BIOLOX®delta is an alumina based composite ceramic. Approximately 80 vol.-% of the matrix consist of fine grained high purity alumina which is very similar to the well known material BIOLOX®forte (ISO 6474). As it is the case in any other composite material, the basic physical properties like stiffness, hardness, thermal conductivity etc. are mainly predetermined from the dominating phase. It was the basic idea for the development of the new material to preserve all the desirable properties of BIOLOX®forte - as an excellent

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

137

bioceramic with more than 30 years clinical experience - but to increase its strength and toughness. These properties are substantially improved by implementation of reinforcing elements. Figure 1 shows the microstructure of BIOLOX®delta.

Alumina matrix Zirconia Platelets

Figure 1. Microstructure of BIOLOX®delta.

Two reinforcing components are integrated into BIOLOX®delta. 17 vol.-% of the matrix consist of tetragonal zirconia particles. The average grain size of the zirconia is around 0.27 µm. As a further reinforcing element, approximately 3 vol.-% of the matrix are built by platelet shaped crystals of the ceramic composition strontium aluminate. The platelets stretch to a maximum length of approximately 5 µm with an aspect ratio of 5 – 10. The reinforcing ability of these ingredients is explained below. Additionally to the reinforcing components, there are also stabilizing elements doped to the material. Chromium is added which is soluble in the alumina matrix and increases the hardness of the composite. The minor amount of chromium is the reason for the pink color of the material, see Figure 2. Furthermore, some yttrium is added to the composite which is solved in the zirconia and supports the stabilization of the tetragonal phase. In Table 2, the composition is given: Table 2. Raw material specification for BIOLOX®delta Ingredient Yttrium oxide Chromium oxide Strontium oxide Zirconium oxide Other oxides Alumina

Formula Y2O3 Cr2O3 SrO ZrO2 TiO2, MgO, SiO2, CaO, Fe2O3, Na2O, K2O Al2O3

Weight percent 1,4 – 2,0 24,0 – 25,5 < 0,22 balance

138

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

During thermal treatment of the material the ingredients are transformed to the particular composition with the 3 components. The basic transformation equations are known as follows:

2 YCrO3 → Y2O3 + Cr2O3

(1)

SrZrO3 → SrO + ZrO2

(2)

Al2O3 + Cr2O3 → Al2O3 : Cr

(3)

SrO + 6 Al2O3 : Cr → SrAl12− x CrxO19

(4)

ZrO2 + Y2O3 → ZrO2 : Y

(5)

In Table 3 the volume fractions of the final products according to equations (3) – (5) are given. Table 3. Components of the final composite BIOLOX®delta Component of the composite Alumina, doped with Chromia Zirconia with Y-stabilization Strontiumaluminate (minor Cr-content)

Formula Al2O3:Cr ZrO2:Y SrAl12-xCrxO19

Figure 2. Ball heads and inserts of BIOLOX®delta.

Volume percent 80 % 17% 3%

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

139

4. Reinforcing Mechanism on BIOLOX®Delta Benefit of Phase Transformation The reinforcing elements, in particular zirconia, substantially increase fracture toughness and strength of the material. Fracture toughness (KIC) is a measure for the ability of the material to withstand crack extension. Strength (σc) is defined as the maximum stress within a structure at failure of the component. The correlation of strength and toughness is given in the fundamental equation of fracture mechanics:

K IC = σ c

ac Y

(6)

where ac is the size of a typical critical defect in the material and Y the shape factor. Consequently, when the fracture toughness of the alumina is increased also the strength is directly improved. This basic principle is the concept of the development of BIOLOX®delta. The microstructure is designed in order to provide an optimum of resistance against crack extension. The benefit in crack resistance which is obtained from incorporating zirconia into an alumina matrix (as shown in Figure 3) is well known in the science of high performance ceramics.

1 µm Figure 3. Reinforcing mechanism in BIOLOX®delta at crack initiation and propagation. Yellow particles represent tetragonal zirconia. Color change to red indicates monoclinic phase transformation. Arrows show the region of compressive stresses due to phase transformation.

The figure represents a realistic part of the microstructure. The gray particles refer to the alumina matrix, yellow to tetragonal zirconia. The phase transformation of zirconia is indicated by the change to red color. In the case of severe overloading crack initiation and crack extension will occur. High tensile stresses in the vicinity of the crack tip trigger the tetragonal to monoclinic phase transformation of the zirconia particles. The accompanied volume expansion leads to the formation of compressive stresses which are efficient for blocking the crack extension. The model as represented in Figure 3 has also been verified experimentally. Pezzotti et.al. [PezTBP] analyzed the monoclinic phase transformation in the vicinity of an artificial crack tip as shown in Figure 4.

140

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

As it is demonstrated in Figure 3 this reinforcing mechanism is fully activated within a region of a few micrometers. For the macroscopic performance of the material it is very important that immediately at the beginning of crack initiation also the reinforcing mechanisms are activated. Regarding Figure 3 one should keep in mind that the average distance between the reinforcing zirconia particles is approx. 0,3µm, i.e. similar to the grain size. Thus, the reinforcement is activated immediately when any microcrack is initiated. The reinforcing ability of zirconia particles is a consequence of the phase transformation, i.e. the spontaneous change from the tetragonal to the monoclinic phase [Han00]. The phase transformation is accompanied by a volume change of 4 % of the zirconia particle. Spontaneous phase transformation is a well known principle in material science. For example, the properties of high performance steels also rely on phase transformation from austenite to martensite.

Grey intensity proportional to monoclinic phase content

Raman Spectroscopy, G. Pezzotti.

Figure 4. Monoclinic phase transformation in the vicinity of an artificial crack tip.

It should be emphasized that the ability of phase transformation is the precondition for any benefit of the zirconia within the material. The composite is designed such that phase transformation occurs when it is needed, i.e. to prevent microcrack initiation and propagation at a high mechanical stress level.

Experiment: What Happens when Phase Transformation Is Suppressed? It has been shown experimentally that the ability of zirconia phase transformation in BIOLOX®delta is necessary for the excellent mechanical properties. The experiment has been designed such that the experimental material was identically produced to BIOLOX®delta but with a significant higher amount of Y2O3. Yttria is known for stabilizing the tetragonal phase of zirconia. Consequently, in the case of a too high amount of yttria, the ability of phase transformation is suppressed. This has been shown in the experiment. The experimental material W3530 has been produced equivalently to the production of BIOLOX®delta. In Figure 5 it is shown that the microstructure is identical. In Table 4 the properties of the two materials are compared.

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

®

BIOLOX delta

141

Experimental material W3530

Figure 5. Microstructure of regular BIOLOX®delta and experimental material W 3530

Table 4. Comparison of regular BIOLOX®delta and high stabilized experimental material Material properties Ratio Y2O3 / ZrO2 [mol %] Final density [g/cm3] Grain size [µm] Strength [MPa] Hardness [HV1] Monoclinic phase content [%] Fracture toughness

BIOLOX®delta 1,3 4,37 0,54 1392 1757 5 6,5

W3530 3,0 4,38 0,55 777 1747 ≤1 5,1

The basic properties of regular BIOLOX®delta and the experimental material W3530 are identical, i.e. microstructure, density, grain size and hardness. The fundamental difference is the ratio of Y2O3/ZrO2. In BIOLOX®delta the amount of yttria is significantly lower. As can be seen from the data, the higher amount of yttria in the experimental material leads - as expected - to a lower content of monoclinic phase, because phase transformation is suppressed. As a consequence the fracture toughness and the strength of the experimental material are much lower than the properties of BIOLOX®delta. In particular, the strength of the experimental material W3530 is only 55% of the normal strength of BIOLOX®delta. From this result it is immediately clear that the ability of phase transformation is necessary to obtain a high performance composite ceramic. The phase transformation can be easily suppressed by chemical stabilization (using yttria). However, suppressing phase transformation means loosing the excellent mechanical properties of the material.

142

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

Stabilization of the Zirconia Tetragonal Phase In BIOLOX®delta the content of yttria has been optimized during the material development. It should be noted that the Y2O3/ZrO2-ratio is lower than in normal pure zirconia materials (3Y-TZP), because the stabilization of the tetragonal phase in BIOLOX®delta is also influenced by “mechanical stabilization”, i.e. the embedding of zirconia in the stiff alumina matrix.

cub

temperature [°C]

2000

1500

tet + cub tet

1000

500 mon

mon + cub 2

4

6

8

Y2O3 [mol %]

Figure 6. Background of stabilizing effects: Y-doping and embedding of zirconia particles in a matrix.

As can be seen in Figure 6 doping of Y2O3 into ZrO2 shifts the temperature of tetragonal – to - monoclinic phase transformation towards lower temperatures. Thus, doping with Y means “chemical stabilization”. At Y2O3 content lower 10% the stable phase at room temperature is monoclinic. So additionally the embedding of the zirconia particles in a matrix as well as surface stresses in the small particles also act as stabilizing mechanisms. The surrounding material will oppose the transformation and it is the strain energy that is involved in this constraint that allows the tetragonal phase to be retained at room temperature [Gre89]. This effect is referred to as “mechanical stabilization”

5. Material Production and Properties BIOLOX®delta is a comparatively complex composite material where 4 different ingredients are mixed during powder preparation and undergo solid phase transformation at high temperature treatment as explained in chapter 2. The ability of reproducing such a material in high quantities with excellent quality batch by batch is the key qualification of CeramTec as manufacturer. It is the purpose of this section both to summarize the important material properties and to elucidate the reproducibility of the production. The important production and analytical steps are as follows:

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

143

Figure 7. Schematic description of processing and material data generation of a single batch.

As shown in Figure 7 the material data are obtained for every powder batch. In Table 5 the material data as obtained for all powder batches in 2007 are summarized.

144

Meinhard Kuntz, Bernard Masson and Thomas Pandorf Table 5. Material properties of BIOLOX®delta batches in 2007

Density g/cm3

4-pt. Weibull Hardness Monoclini Grain Size Fracture Bending Modulus HV 10 c content Alumina Toughness Strength MPa GPa % µm MPa m

Average

4,37

1411

14,9

17,2

4,4

0,54

6,4

Std. Dev.

0,007

50

3,1

0,09

1,1

0,027

0,20

The physical background of these parameters should be discussed. There are parameters which are almost invariable due to the physical nature of the property, in particular density and hardness. In the normal case of regular production there is only very little scatter with these data. However, it is important to analyze these parameters for every batch because any deviation of the expected results would indicate an insufficient production lot. On the other hand, it is worth highlighting the low alumina grain size and the very low scatter of this value. During sintering and final densification of any ceramic the particles build a dense matrix but simultaneously grain growth also occurs. It is the goal of adequate sintering to achieve full density but to suppress grain growth, as a fine microstructure is necessary for good mechanical properties. Obviously, the sintering of BIOLOX®delta is very well reproduced batch by batch. The grain size is low in comparison to pure alumina because the dispersed zirconia particles prevent grain growth of the alumina matrix. The fracture toughness is a measure for the reinforcing mechanisms in the material. As described in chapter 3 the high fracture toughness depends on the transformation mechanism of the zirconia particles. Obviously also this value shows very low scatter. The average fracture toughness is 6,4 MPa√m. In contrast, the “overstabilized” material W3530 described in chapter 3 has a significant lower fracture toughness K1c 5,1 MPa√m. Thus, it can be derived from the evaluation of fracture toughness from batch to batch that the desired transformation toughening is working properly. As explained in chapter 3 the fracture toughness should be discussed in context with the monoclinic phase content which is determined on a polished flat surface of a specimen. The monoclinic phase content [in %] as obtained from the regular X-ray diffraction is relative to the total zirconia content, not to the total volume of the material. Thus, in any case the monoclinic phase content of the total material can be determined by simply referring to the zirconia fraction of 17 vol.%. Example: 10% monoclinic phase content is equivalent to 1,7% relative to the total volume of the material. According to the materials specification the monoclinic phase content after polishing (intrinsic monoclinic phase content) is ≤ 10% of ZrO2 which is regularly determined by X-ray diffraction. The sensitivity of this technique is around 1% monoclinic phase content. As it is evident from the data the average intrinsic monoclinic content of ZrO2 of 4,4% is above the sensitivity limit. This indicates again that the sound material is in disposition of phase transformation. Note that the monoclinic content of the experimental material W3530 is below the sensitivity limit. In contrast to the other parameters discussed above the strength of the material shows significantly higher scatter. It is important to understand that failure in ceramics is always

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

145

triggered by imperfections of the microstructure. High performance ceramics can only be achieved when the natural defects in the material are very small. Typical relevant imperfections in BIOLOX®delta are within a range of 5 – 50µm. Accordingly, the scatter of natural defect size directly matches the scatter of strength which is described by the Weibull´s modulus. A high modulus indicates low scatter. For the high performance material BIOLOX®delta a Weibull’s modulus of ≥ 7 is tolerated in the specification. As can be seen from the data the normal scatter of the strength is much lower (i.e. higher modulus).

6. Correlation of Material and Component Properties In chapter 5 the extensive efforts of analyzing the material properties of BIOLOX®delta batch by batch have been discussed. These material properties are determined according to ISO 6474 which is applicable for pure alumina and currently being extended for aluminacomposite materials such as BIOLOX®delta (ISO 6474-2). This type of data is very familiar for evaluation of the performance of ceramics. In this chapter it is intended to discuss shortly how these material data correlate to component properties, e.g. the strength of ball heads and inserts. In general, the performance of any system depends on the intrinsic material properties, the design and manufacturing quality of the components and the system, the external load and the particular environment, and finally the quality of mounting and installation. The use of high performance materials inevitably promotes the performance of a system - however, the other factors may be even more decisive for the success of a system. These complex correlations must be necessarily evaluated by design analysis, modeling, simulations, risk analysis and many other tools. In order to eliminate any influences of design features most of the material testing has been performed using 4-point bending bars. In Figure 9 the setup of the regular 4-point bending test as recommended in ISO 6474-2 and the burst test according to ISO 7206 are shown. The bending test reveals the intrinsic strength of the material whereas the burst test is designed in order to simulate the in-vivo load of ceramic ball heads.

4-Point Bending Test

Burst Test

Figure 8. Schematic set-up of 4 point bending test and ball head burst test.

146

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

The strength measured with the bending test is – to a first approach - an intrinsic material parameter1, whereas the burst load as obtained from the burst test depends on the materials strength and the design of the ball head and the taper. This is directly shown by comparison of strength and burst load of different ball heads made of BIOLOX®forte and BIOLOX®delta, see Table 6. Table 6. Comparison of strength and burst load of BIOLOX®forte and BIOLOX®delta Parameter Strength Burst load Burst load

Test / Design 4-point bending 28-12/14 L 36-12/14 M

Unit

BIOLOX®forte

BIOLOX®delta

ratio delta / forte

MPa

620

1400

2,3

kN kN

54 110

85 131

1,6 1,2

All burst loads are far above the required value of 46kN. The maximum in vivo load at worst case conditions is approximately 10 kN. The data of the burst tests given in Table 6 are obtained from ball heads with identical geometry, Ti test taper and the same test setup. Thus, the advantage of BIOLOX®delta ball heads in the burst load only comes from the higher strength of the material in comparison to the pure alumina BIOLOX®forte. The strength of BIOLOX®delta is more than twice the strength of BIOLOX®forte, whereas the ratio of the burst strength values is lower. This is explained by the ductile deformation of the Ti taper during the burst test which steadily increases the contact area of the conical bore of the ceramic ball head and the metal taper. However, the burst load of identical ball heads is always higher when a high strength material is used. It is also seen that the burst strength strongly depends on the ball head size. A larger ball head shows a higher burst load. It is concluded that the benefit of using a high performance material is higher when applied to a challenging design, e.g. a ball head with lower wall thickness. Nevertheless, the use of the high strength material always increases the safety margin of the component.

7. Wear Performance of BIOLOX®Delta At normal wear conditions (e.g. standard wear simulator) the wear of a hard-hard couple of BIOLOX®delta is identical to the excellent performance of the well proven pure alumina BIOLOX®forte. There is only a minor difference in hardness of these both materials which does not compromise the normal wear behavior. However, a significant advantage of BIOLOX®delta is identified in the case of worst case wear simulation as shown in Figure 9. In this experiment microseparation of ceramic ball head and insert during each load cycle has been simulated which leads to highly localized 1

Due to the statistical nature the strength also slightly depends on the specimen size and the stress distribution. Size effects can be mathematically balanced. In order to obtain results which can be directly compared to each other the standardized set-up of the bending test should be used.

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

147

forces at the contact area. This experimental setup was supposed to simulate e.g. low tension of the soft tissue after surgery as it is discussed frequently by orthopedic experts. It was concluded from various retrievals that in some cases a well defined stripe-shaped area shows a more intense worn surface than the normal surface of the ball head. This phenomenon is known as “stripe wear”. In the experiment, heavy wear conditions were simulated due to the highly localized contact area. It was found after 5 mio microseparation load cycles that the wear volume of BIOLOX®delta couples (both ceramic ball head and insert were made of BIOLOX®delta) was 7 times lower than that with the coupling made of pure alumina BIOLOX®forte [Cla05]. The wear rate of the mixed couplings (either ball head or insert made of BIOLOX®delta, the remaining made of pure alumina BIOLOX®forte) ranged between those values. It is important to mention that due to the small differential hardness between BIOLOX®forte and BIOLOX®delta can be combined in a ceramic-ceramic coupling without running the risk of excessive wear or other adverse effects.

®

Figure 9. Wear performance of BIOLOX delta and BIOLOX®forte at simulated micro separation.

Obviously BIOLOX®delta shows an excellent “stripe wear tolerance”. The analysis as given in [Cla05] shows that in the stripe wear region the monoclinic phase content is strongly increased. This indicates the mechanism behind the excellent stripe wear tolerance of BIOLOX®delta. As a first approach it is assumed that at these special test conditions a very high localized stress acts in the contact area which may be able to introduce damage in the surface. In this case the reinforcing mechanism as described in Figure 3 is activated in BIOLOX®delta which supports maintaining the surface quality under these extreme conditions. This assumption is supported by the Raman analysis of the worn surface. In the stripe wear region a high monoclinic phase content was found which indicates that phase transformation for reinforcement took place.

148

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

8. Discussion of Hydrothermal Aging Mechanism of Hydrothermal Aging Aging is a relevant issue for all zirconia containing ceramics. The transformation from the tetragonal to the monoclinic phase can be triggered in a hydrothermal environment. “Hydrothermal” means that this particular aging effect only takes place in aqueous environment at elevated temperatures. A critical temperature range for hydrothermal aging is around 120 – 200°C. However, a very slow aging effect is potentially possible even at human body environment. The kinetics and the threshold of aging activation strongly depend on the grain size, volume fraction, amount and type of stabilizing elements (e.g. Y, Ce, Mg, Ca) and mechanical stabilization of the zirconia [Che99]. adsorption

1st step

H2O Zr

2nd step surface

Zr

Zr

O

OH

Zr

OH stress

O

O

O

O

vacancy

Zr

Y

3rd step

migration

Zr

OH

Y

OH

4th step

Zr

OH

migration

O

Zr

Y

Zr

O

Zr

OH

O lattice expansion

Zr

OH

O

Y

OH

Zr

Figure 10. Model of hydrothermal aging.

Albeit the hydrothermal aging is extensively studied in the literature, the exact mechanism behind this effect is still not perfectly described. Most of the available models refer to interaction of the hydroxide ions and oxygen vacancies in the zirconia lattice. The oxygen vacancies inevitably are introduced in the lattice at solution of Y2O3 in ZrO2 due to different valence of the cations. Figure 10 represents a model of the interaction of hydroxide ions with Y-doped zirconia with 4 steps: 1. Adsorption of water molecules at the surface 2. Dissolution of the oxygen bond

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

149

3. Migration of hydroxide ions to oxygen vacancy 4. Reorganisation of the atomic lattice The critical step within this model is the dissolution of the oxygen bond which is very strong in zirconia. Thus, a thermal activation at elevated temperatures is required.

Hydrothermal Aging in BIOLOX®delta Phase transformation caused by hydrothermal aging is an undesired effect. However, as it has been shown in the previous chapters, monoclinic phase transformation is necessary for the reinforcement and the high strength and toughness of the material BIOLOX®delta. Thus, a certain amount of phase transformation in hydrothermal environment is not a matter of concern. It depends on the specific composition of the material if there is a critical level of phase transformation where the material can be damaged. In the years 2001 – 2002 some batches of the pure zirconia material Prozyr® of the company Desmarquest showed catastrophic failure in-vivo due to monoclinic phase transformation at the surface [Che06]. It has to be emphasized that such a damage is impossible in BIOLOX®delta due to the fact that only 17vol% consist of zirconia. Consequently, the ultimate upper limit of monoclinic zirconia is only a total of 17% whereas 83% of the material remain not affected by phase transformation and hydrothermal aging. As mentioned above, hydrothermal aging is accelerated at elevated temperatures. For pure zirconia in biomedical applications a standardized accelerated aging test is recommended in ISO 13 356. The aging conditions are autoclaving at 134°C and 2 bar water steam for 5h. In the new standard ISO 6474-2 being prepared for alumina zirconia composites an aging time of 10h is recommended. As a rough estimate it is proposed that 1h autoclaving is equivalent to 2 – 4 years in human body environment. However, this transfer of aging kinetics depends on individual properties of a material. The aging behavior of BIOLOX®delta has been extensively analyzed using accelerated hydrothermal aging by autoclaving. Moreover, the aging has been combined with severe mechanical static and dynamic testing in order to understand if any material degradation occurs during aging. In fact, the monoclinic phase content in BIOLOX®delta is increased after long term aging. In Figure 11 quantitative analysis of monoclinic phase transformation using Raman spectroscopy are shown. The aging conditions (121°C, 1 bar) for this analysis were slightly different from the recommendation in the ISO standard. Equal to Figure 4 the gray intensity indicates monoclinic phase distribution. As can be seen the monoclinic content is increased after extreme long exposure time. After 300 h the monoclinic phase content reaches a relative value of 66,7%, i.e. 11,3% of the total volume of the composite are monoclinic zirconia.

150

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

Figure 11. Increase of monoclinic phase content after very long term hydrothermal aging in an autoclave. Autoclaving conditions 121°C, 1 bar. Pictures adopted from [Pez08]. Quantitative monoclinic phase content obtained by direct communication to the author.

The autoclaving time used in this study is extremely long, much longer than recommended in the ISO standard. The monoclinic phase content seems to reach a saturation since the increase from 200h to 300 h is only marginal.

Aging Kinetics of BIOLOX®delta As described above the aging effect of zirconia containing materials depends on the individual composition. It is of particular interest to estimate the aging effect of a bioceramic under in-vivo-conditions, i.e. 37°C in serum. As it was the case in the Prozyr® disaster a high amount of phase transformation occurred after a relatively short time in-vivo. On the other hand, it is well known that even pure zirconia is usually much more stable against hydrothermal aging when produced appropriately. For a given material, the long term aging (in years) at low temperatures can be predicted based on the assumption that nucleation and growth of phase transformation are thermally activated. The thermal activation can be assessed by a systematic variation of temperature and duration time in hydrothermal environment and measurement of monoclinic phase transformation before and after the test. The most common method for such a prediction is based on the model of Mehl-Avrami-Johnson (MAJ-theory), which was first applied to zirconia based materials by Prof. Chevalier (Lyon, France) [Che99]. For example, it was found that for a conventional zirconia material with 3 mol% Yttria content (3Y-TZP) one hour in autoclaving conditions (134°C, 2 bar water steam) is equivalent to 3-4 years in-vivo. For other zirconia materials, a correlation of only 2 years was found. It is important to understand that this relation is not a universal law for zirconia containing materials but instead the individual outcome of the particular ceramic composition. The aging kinetics of BIOLOX®delta was analyzed in close cooperation with Prof. Chevalier. The complete study will be accomplished and published in 2009. In the following, the preliminary results which are available at the current state are summarized. The accelerated aging tests were performed in water steam at 142°C, 134°C, 121°C, and 105°C. Additionally one test was performed at 90°C in water. It is assumed that steam and liquid hydrothermal environment are comparable by means of the effect on hydrothermal

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

151

aging. More tests have also been launched at 70°C and 50°C in water. However, due to the long duration time which is necessary to detect any effect at these temperatures results are expected within the next 2 years. The monoclinic phase content was determined using X-ray diffraction. In Figure 12 the results of the tests are shown on a logarithmic time scale. 80

90°C 105°C 121°C 134°C 142°C Pezzotti

monoclinic fraction (%)

70 60 50 40 30 20 10 0 0,1

1

10

100

1000

10000

time (h)

Figure 12.:Monoclinic phase transformation of BIOLOX®delta in hydrothermal environment. For comparison, also data from [Pez08] is included.

For evaluation of these data, the following modified MAJ equation was applied

[

(

Vm = Vm0 + (Vmax − Vm0 ) 1 − exp − (b t )

n

)]

(7)

0

where Vm is the monoclinic phase content, Vm is the initial monoclinic phase content prior to the test, Vmax is an apparent upper bound of the monoclinic phase, t is the time and n the time exponent. b is the factor which describes the temperature dependence of the aging effect. It is derived from fitting the data according to the following Arrhenius type equation:

⎛ Q ⎞ ⎟⎟ b = b0 exp⎜⎜ − ⎝ RT ⎠

(8)

where b0 is a material constant, Q is the activation energy, R the universal gas constant and T the temperature. Evaluation of the data given in Figure 12 reveals an activation energy Q of 108 kJ/mol. This is a particular high value in comparison to a similar material (alumina zirconia composite) which was discussed in [Pez08], where an activation energy of 78kJ/mol is referred. The reason for this discrepancy is, as discussed above, the low amount of oxygen

152

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

vacancies in BIOLOX®delta due to the unique chemical composition. High activation energy means strong influence of temperature on aging. Consequently at low temperatures the aging rate of in BIOLOX®delta is significantly lower. From the modified MAJ equations the hydrothermal aging effect under in-vivo conditions can be estimated. The following equivalence to the accelerated hydrothermal aging was found: 1 h at 134°C is equivalent to 3,9 years in-vivo According to the proposal of the new ISO standard 6474-2 hydrothermal aging is simulated under autoclaving conditions at 134°C for 10 hours. These conditions are thus equivalent to 39 years in-vivo for BIOLOX®delta which seems to be a realistic upper bound of the expected live time of an artificial joint. Several accelerated aging tests according to these conditions (134°C, 2 bar water steam, 10 h) have been performed with BIOLOX®delta. The initial monoclinic phase content prior to aging depends on the surface finishing. On a ground surface the initial monoclinic phase content is higher than on a polished surface due to the more intensive interaction of the ceramic surface to the diamond tool. There is no effect on strength of the higher initial monoclinic phase content - the test specimens for the regular evaluation of strength are ground, not polished. Table 7 gives the data of monoclinic phase increase after 10 h autoclaving Table 7. Analysis of zirconia phase transformation at accelerated aging Surface finishing 5% 21 %

Initial monoclinic phase content 8% 33 %

Monoclinic phase content after 10 h autoclaving

There is obviously a large difference of initial monoclinic phase content between polishing and grinding. However, the relative increase of monoclinic phase transformation does not depend on the surface condition. As discussed in chapter 5 the monoclinic phase content is given relative to the total amount of zirconia. When the effect of phase transformation shall be assessed, it is useful to refer the monoclinic content to the total volume of the material, i.e. taking into account the zirconia volume fraction of 17 vol %. Thus, after grinding and autoclaving the absolute monoclinic phase volume content is 5,6% (33% × 0,17). The accelerated aging according to Figure 11 was performed at 121°C 1 bar, i.e. a lower temperature and steam pressure than recommended in the ISO standards. It is also possible to evaluate the equivalence of this treatment to in-vivo conditions. 1 h at 121°C is equivalent to 1,3 years in-vivo. It should be noted that there is a strong discrepancy of this equivalence factor to the data which was used and discussed in [Pez08], because in this publication the activation energy of

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

153

a different material was used. It is evident that the aging kinetics must be carefully analyzed and discussed for the individual material.

Effect of Hydrothermal Aging on Strength of BIOLOX®delta It is necessary to examine if the phase transformation reveals any damage or loss in strength of the material. For this purpose experiments were designed in order to combine accelerated aging and mechanical loading at a very high stress level. The specimens were prepared according to the 4-point bending configuration as it is shown in Figure 9 (left). These bend bars were exposed to accelerated aging and then to loading-unloading cycles at high stresses. After aging and cyclic loading the residual strength was determined. Two stress levels (300 MPa and 600 MPa) were chosen for the cyclic loading tests. The lower stress level was applied for 20 Mio cycles, the higher stress level for 5 Mio cycles. All tests were performed in Ringer’s solution. The accelerated aging was simulated by 5 h and 100 h treatment in standard autoclaving conditions (134°C, 2 bar water steam). It should be noted that again an aging time much longer than required from the standard was used. For each step of the experiments (as received, after aging, after aging and cycling) the monoclinic phase content was measured using X-ray diffraction. As the most amazing result the yield of specimens surviving all the tests was 100 % in all cases. Even most severe conditions (i.e. 100 h autoclaving, 600 MPa cyclic load) did not reveal any premature failure. It should be recalled that this stress level represents 4 times the highest load level at worst case conditions in-vivo. We can thus conclude that the reliability of BIOLOX®delta exceeds by far the necessary requirements for reliable surgical components. Table 8. Residual strength and monoclinic phase content after diverse treatments. Monoclinic phase is given relative to the total volume of the material Autoclaving duration 0h 5h 100 h

no cyclic load Strength [MPa] Monoclinic phase content [%] Strength [MPa] Monoclinic phase content [%] Strength [MPa] Monoclinic phase content [%]

1346 18 1332 22 1234 30

300MPa, 600MPa, 20*106 cycles 5*106 cycles 1433 33 1248 35 1308 33

1284 43 1361 42 1300 47

Table 8 shows the results of the post – test analysis including residual strength and monoclinic phase content. There is –as expected - a marginal natural scatter in residual strength. However, statistical analysis using Student’s t-test did not reveal any significant deviation of all strength results.

154

Meinhard Kuntz, Bernard Masson and Thomas Pandorf

Monoclinic Content [%]

50 40 30

100 h ageing 20

5 h ageing

10

No ageing

0

no cycling

300 MPa 20 Mio cycles

600 MPa 5 Mio cycles

Figure 13. Increase of monoclinic phase content at cyclic loading.

In contrast, there is a clear tendency of an increase in monoclinic phase content both, after autoclaving and after cyclic loading, which is illustrated in Figure 13. For example, the test series without autoclaving shows an increase of monoclinic phase content from 18 % in the initial state to 47 % after 5 Mio cycles at 600 MPa. It must be concluded that the cyclic mechanical loading at a high stress level (600 MPa) which represents already the strength of pure alumina activated the reinforcing ability of the material. As discussed under Figure 3, a high mechanical stress triggers localized phase transformation which prevents any further crack propagation. Obviously the increased amount of monoclinic phase content does not deteriorate the strength of the material. This important conclusion is independent from the source of the phase transformation. In other words, when the phase transformation is activated either by accelerated aging, cyclic fatigue or a combination of both, the residual strength remains at the initial level.

References [Che99]

Chevalier J., Cales B., and Drouin J.M., Low temperature aging of Y-TZP ceramics, J.Am.Cer.Soc. 82 (1999) 2150-54 [Che06] Chevalier J., What future for zirconia as a biomaterial, Biomaterials 27 (2006) 535-543 [Cla05] Clarke I.C., Pezzotti G., Green D.D., Shirasu H., and Donaldson T., Severe Simulation Test for run-in ear of all-alumina compared to alumina composite THR, Proceedings 10th BIOLOX Symposium, 11-20 (2005) [DeA02] De Aza, A.H., Chevalier J., Fantozzi G., Schehl M., and Torrecillas R., Crack growth resistance of alumina, zirconia and zirconia toughened alumina ceramics for joint prostheses, Biomaterials 23, 937-945 (2002) [Gre89] Green D.J., Hannink R.H.J., and Swain M.V., Tranformation Toughening of Ceramics, CRC Press Inc., Boca Raton, Florida (1989) ISBN 0-8493-6594-5 [Gre04] Gremillard L., Chevalier J., Epicier T., Deville S., and Fantozzi G., Modeling the ageing kinetics of zirconia ceramics, J.Eur.Cer.Soc., 24, 3483-3489 (2004)

Current State of the Art of the Ceramic Composite Material BIOLOX®delta

155

[Han00] Hannink R.H.J., Kelly P.M., and Muddle B.C., Transformation Toughening in Zirconia-Containing Ceramics, J.Am.Cer.Soc. 83 [3] 461-87 (2000) [Ohm99] Ohmichi N., Kamioka K., Ueda K., Matsui K. and Ohgai M., Phase Transformation of Zirconia Ceramics by Annealing in Hot Water, J. Cer. Soc. Jap., 107 [2] 128-133 (1999) [Pez06] Pezzotti G. Environmental Phase Stability of Next Generation Ceramic composite for Hip Prostheses, Key Engineering Materials Vols. 309-311, 1223-1226 (2006) [Pez08] Pezzotti G. Yamada K., Sakakura S., and Pitto R.P., Raman Spectroscopic Analysis of Advanced Ceramic Composite for Hip Prosthesis, J.Am.Ceram.Soc. 91 [4] 1199-1206 (2008) [PezTBP] Pezzotti G. Yamada K., Porporati A., Kuntz M., and Yamamoto K., Raman Spectroscopic Analysis of Advanced Ceramic Composite for Hip Prosthesis: Part II Fracture Behavior (to be published)

In: Strength of Materials Editors: G. Mendes and B. Lago, pp. 157-182

ISBN: 978-1-60741-500-8 © 2009 Nova Science Publishers, Inc.

Chapter 5

PARTICLE MODELING AND ITS CURRENT SUCCESS IN THE SIMULATIONS OF DYNAMICS FRAGMENTATION OF SOLIDS G. Wang1*, A. Al-Ostaz1, A.H.D. Cheng1 and P. Radziszewski2 1

Department of Civil Engineering, University of Mississippi, Oxford, MS, 38677-1848, USA 2 Mechanical Engineering Department, McGill University, Montreal, QC, H3A 2T5, Canada

Abstract Particle modeling (PM) is an innovative particulate dynamics based modeling approach. It has been demonstrated as a robust tool for simulating fracture problems of solids with dynamic fragmentation under extreme loading conditions. These loading conditions can include situations of collapse, impact, blasting or high strain rate tension/compression, as well as thermally-induced breakage problems. Initially, PM was developed for the purpose of mimicking the microscopic material process at macroscopic level. This method can be conceptually illustrated by fully dynamic particles (or “quasi-particles”) placed at the nodes of a lattice network without explicitly considering their geometric size. The potential can be specified for particle-particle interactions via axial springs. Theoretically, PM is an upscale of the molecular dynamics (MD) model applicable to various length scale problems. This is possible if a proper equivalent macroscopic potential is found, and, in case of lattice spacing decreasing to a few Angstroms, a MD model at zero Kelvin with, say, Leonard-Jones potential is recovered. In its current form, PM has been developed as a tool applicable to real engineering problems. The advantages of PM over the existing discrete element based methods can be summarized as follows: (1) Sample in theory. Four conservative/equivalent rules (mass, potential energy, Young’s modulus and tensile/compression strength) are applied to preserve the equivalent material properties. (2) Easy for implementation. Since the physical size of each particle is ignored other than its equivalent mass, the algorithm of coding a PM computation is fairly easy. *

E-mail address: [email protected] Tel: + 662 915 5369, Fax: + 662 915 5523. Corresponding author: Ge Wang

158

G. Wang, A. Al-Ostaz, A.H.D. Cheng et al. Current research work has exhibited that PM is able to correctly predict dynamic fragmentation of materials with a good accuracy. In modeling an epoxy plate with randomly distributed holes in tension, the PM result of the final crack pattern compared favorably with the associate experiment; for the simulations of impact study of two polymeric materials (nylon, 6-6 and vinyl ester) subject to a rigid falling indenter, the modeling results of resistant force, energy, deflection and drop speed of indenter vs. time quantitatively agree fairly well with the according empirical observations.

1. Introduction The prompt development of modern computer technology and computational methods enables scientists, more easily than ever before, to numerically examine the nature of materials, to verify or modify the existing theories, and even to discover new phenomena. Dynamic fracture modeling also greatly benefits from this advancement. The dynamic fracture process itself is an exceedingly complex, multi-scale physical phenomenon. Material failure exhibits non-linearly, localized presence and a dependence on dynamic loading and loading conditions, etc. Hence, an ideal solver of dynamic fracture mechanics is required to be able to handle all the above-mentioned factors, especially to deal with the discontinuity of material that dominantly occurs in a dynamic fracture process which becomes an overwhelming difficulty to numerical approaches. At the microscopic level, fracturing is a process that material becomes separated due to the successive failures of atomic bonds. Since the intrinsic strength properties at atomic structure level are available, molecular dynamics (MD) analysis has been used in modern scientific research at nano-scale. However, although MD simulation has benefited from the rapid development of modern computer technology and is becoming increasingly popular, the present state of computational power is still far from being able to support simulation at the macroscopic level. For example, we currently still cannot simulate a 1 × 1 × 1 cm3 cubic copper body at atomic level because the body consists of 10 24 copper atoms, a number so large that no computer in the world can handle it. The second difficulty is its inability to reach the laboratory time scales. For instance, the laboratory fracture experiments generally last in microseconds ( 10 −12

−6

−9

second), while the MD model time steps are typically in the nano ( 10 )

or pico ( 10 ) second range. As such, MD is limited narrowly to solving nano- to micrometer scale problems. Hence modeling fracture problems directly at macroscopic scale is a prevalent pursuit. An all-round search to the existing optional modeling techniques reveals that the modern numerical methods for dynamic fracture simulations at macroscopic level can be generally classified into two categories of approaches. One is continuum mechanics based and the other is discrete element based. Examining the state-of-the-art of the research, we conclude that the continuum mechanics based approaches, such as the finite element method (FEM), have difficulty in solving dynamic fracture problems, particularly in dealing with the simulation of the collapse of structure and its fragmentation under extreme loading conditions. For this reason, another domain of alternative modeling approach —the discrete element based models, has become more and more popular. Discrete element models share a common concept of “discrete material”, which can still be further classified into two sub-categories. The first one is classified as a discrete element

Particle Modeling and Its Curent Success in the Simulations...

159

method, in which the physical size and shape of each element is considered in the computation, such as the applied element method (AEM) [Meguro & Tagel-Din, 2000], and particle finite element method (PFEM) [Oñate, et al., 2004] - another particle-related model. In practice, this type of models is complex and difficult to be implemented. For instance, AEM is laborious in keeping track of the instantaneous contact positions and the evolving geometry of all elements for a proper updating of the dynamic bonds; PFEM is expensive in remeshing and redefining boundaries at each time step. The second branch is named particle (or particulate) dynamics method, in which the physical size and shape of each discrete cell is not explicitly considered in the computation. Consequently, each cell is treated as a particle, with the equivalent mass lumped at its center. Smoothed particle hydrodynamics (SPH) [Monaghan, 2005], and particle modeling (PM) are currently the mainly two popular particulate based models. SPH adopts a kernel probability density function to define for each particle a reaction domain at each time step, in terms of a particle number density; it is therefore highly expensive in computation. In contrast, PM is rather simple in theory and easy for implementation; hence, it is attracting increasing interest, despite a good number of SPH codes. Particle modeling (PM) method was originally proposed by Greenspan [1981, 1997] for the purpose of mimicing the microscopic material process at macroscopic level. PM is fully dynamic with particles (or “quasi-particles”) placed at the nodes of a periodic (equilateral triangular) lattice. Conventionally, only the nearest neighboring particles are accounted for in the interaction via axial spring connections. Similar to MD, potential can be specified for particle-particle interactions, and, in the case of lattice spacing decreasing to a few Angstroms, we recover a molecular dynamics (MD) model at zero Kelvin with, say, a Leonard-Jones potential. This implies that PM is an upscaled MD and can be applied to various length scale problems if a proper equivalent macroscopic potential is used. Obviously, by making use of the similar processes as atomic interactions, it is possible to solve fracture problems at macro-scale level. However, as no direct link with the material properties was attempted by Greenspan, Greenspan’s PM method remains a conceptual model without a demonstrated success in fracture modeling. Wang and Ostoja-Starzewski [2005a] developed a newly modified PM with a conventional linkage pattern as shown in Figure 1. In this new PM, equivalent material properties are formulated using four physical conditions to determine continuum-level Young’s modulus and tensile strength, while maintaining the conservation of mass and energy of the particle system, and satisfying the interaction laws among all the particles. The theoretical foundations of the current PM can be outlined in the following four aspects: (a) Derivation is based on equivalence/equality of mass, energy, elastic moduli and tensile strengths between both atomic and quasi-particle systems. (b) Derivation is carried out in the setting of a 3-D face-centered cubic (f.c.c) lattice network (Figure 2) for both atomic and quasi-particle structures. (c) Either Lennard-Jones, polynomial or quadratic potentials can be employed for nonlinear or linear axial linkage. (d) In principle, it can be applied for various length scale problems of solids.

160

G. Wang, A. Al-Ostaz, A.H.D. Cheng et al.

Wang and Ostoja-Starzewski, 2006.

Figure 1. Lattice structure in PM.

Wang and Ostoja-Starzewski, 2005a.

Figure 2. Meshing system for a 3D material body.

In this paper, current PM modeling development is to be addressed. In the coming sections, first we will introduce the theory of PM; then report some significant success and also defects experienced through the applications. Meanwhile, the potential solutions to the modeling deficiencies are proposed; and finally, in the conclusion part, an outlook of futuregoing PM development is addressed.

2. Methodology of PM In particle modeling (PM), the nonlinear interaction force is considered between nearestneighbor (quasi-) particles and assumed to be of the same form as in MD:

Particle Modeling and Its Curent Success in the Simulations...

F =−

G H + r p rq

161

(1)

Here G, H, p and q are positive constants, and q > p ≥ 1 to obtain the repulsive effect that is necessarily (much) stronger than the attractive one, r being the distance between two particles. Ashby & Jones [1980] presented a simple method to evaluate continuum-type Young’s modulus E and tensile stress σ (r ) of the material from F (r ) , namely

E= and

S0 r0

σ ( r ) = NF (r )

(2) (3)

where S 0 = ( dF / dr ) r = r0 , and r0 is the equilibrium spacing between contiguous particles. N is the number of bonds/unit area, equal to 1 / r02 . Tensile strength, σ TS , results when

dF (rd ) / dr = 0 , that yields,

σ TS = NF (rd )

(4)

Just as in MD, the non-linear dynamical equation of motion for each particle Pi of the PM system is given by

G ⎡⎛ G H ⎞ rGji ⎤ d 2 ri mi 2 = ∑ ⎢⎜ − pi + qi ⎟ ⎥ i ≠ j ⎜ dt rij ⎟⎠ rij ⎦⎥ ⎣⎢⎝ rij ,

(5)

G

where mi and r ji are mass of Pi and the vector from Pj to Pi . Note that if an equilateral triangular lattice structure is adopted in 2-D, the resulting Poisson ratio equals 1/4 (or 1/3) when a 3-D (respectively, plane) elasticity formulation is adopted [Ostoja-Starzewski, 2002, 2007]. The derivation of four parameters in Equation (1) from MD structures is conducted on a cubic body with volume V (= A × B × C ), in Figure 2. A face-centered cubic (f.c.c) lattice for both atomic and quasi-particle structures is chosen. If p, q and r0

are given, then, by

conditions of mass and energy conservation, G and H can be derived. Consequently, Young’s modulus is evaluated by Equation (2) and tensile strength by Equation (4). To represent an expected material property, we would have to do many sets of testing until a unique ( p, q ) is

162

G. Wang, A. Al-Ostaz, A.H.D. Cheng et al.

found to match both Young’s modulus and tensile strength of the material. The complete derivation process is described below. First, for the atomic structure (MD model), we have:

⎛ Ga r 1− pa H a r 1−qa + interaction potential energy (ergs): φ a = ⎜⎜ 1 − qa ⎝ 1 − pa

⎞ ⎟ × 10 −8 ⎟ ⎠

(6)

Young’s modulus (GPa) is obtained from Equation (2) and tensile strength (MPa) from Equation (4). Total number of atoms in A × B × C cubic material body:

⎞ ⎞ ⎛ C × 10 8 ⎛ A × 10 8 ⎞ ⎛ B × 10 8 ⎜ ⎟ ⎟ + 1⎟⎟ × ⎜⎜ 1 1 + + × N * = ⎜⎜ 0 ⎟ ⎜ r 6 /3 ⎟ r sin 60 r a ⎝ ⎠ ⎝ a ⎠ ⎝ a ⎠

(7)

In Eqs. (6) and (7), ra is equilibrium position of the simulated material in atomic structure, and p a , q a are the exponential parameters in atomic structure. Note that, for a Lennard-Jones interaction case, pa = 7 and qa = 13 . Next, for the quasi-particle structure (PM model), we have interaction force (dynes) as in Equation (1). Interaction potential energy (ergs):

φ =

G r 1− p 1− p

+

H r 1− q 1− q

, for p > 1; φ = G ln r +

H r 1− q 1− q

total number of quasi-particles in PM system: N = imax × j max × k max

, for p =1

(8)

(9)

We now postulate the equivalence of MD and PM models. From the mass conservation, we calculate the mass of each quasi-particle m based on atomic mass m a :

m = N * × ma / N

(10)

From the energy conservation, we have:

(N × φ )r =r

0

under the requirement:

(

= N * × φa

)

r = ra

F (r0 ) = 0

From equations (11), (12), we now derive Young’s modulus E:

(11) (12)

Particle Modeling and Its Curent Success in the Simulations... for p = 1 : 1− q o

G = Hr

(N

, H =

*

× φa

)

r = ra

1− q 0

N (1 − q )r

(1 − q ) 1− q 0

ln r0 − r

, E = −Gr0−3 + qHr0− q − 2

163

(13)

for p > 1 :

(N ×φ ) *

1− q , o

G = Hr

H=

a r =ra

(1− p)(1− q)

N( p − q)

r0q−1 , E = − pGr0− p − 2 + qHr0− q − 2

(14)

Similarly, tensile strength can be obtained under dF ( rd ) / dr = 0 . Evidently, the four parameters ( p, q ) , r0 and V affect E and

σ TS .

We have established the equations for G, H, p and q, and carried out a parametric study to find the differing effects on p, q, V and r0 [Wang and Ostoja-Starzewski, 2005a]. Herein, we summarize the obtained rules as follows: (i) The larger the values of ( p, q ) are adopted, the larger is E generated. This is typically associated with the material becoming more brittle than ductile, albeit there is a range of toughness to choose from. Also, with E going up, there is a fragmentation into a larger number of pieces. (ii) In the case of p = 1 , the larger r0 spacing is adopted, the higher is Young’s modulus of the PM material. On the contrary, in the special case of p ≠ 1 , there is an opposite trend. In any case, this increase or decrease does not change very much. (iii) In the case of p ≠ 1 , while keeping the volume fixed, an increase of r0 produces a decrease of Young’s modulus. The situation is again opposite in the case of p = 1. (iv) A uniform augmentation of volume V by dilation in all three coordinate directions (xyz), at any ( p, q ) combination, results in Young’s modulus increasing first strongly and then leveling off. For brittle materials, a general format of linear dynamical equation is often employed [Wang, et al., 2008a],

− S (r − r0 ) for rc ≤ r ≤ rt F ={ 0 0 otherwise

(15)

with r being the distance between two particles, the stiffness S 0 = E • r0 by Equation (2), E the Young modulus and

rmax

the failure displacement of material, r0 the equilibrium

spacing between the contiguous particles.

164

G. Wang, A. Al-Ostaz, A.H.D. Cheng et al. In Equation (15), rc and rt are the fracture positions applied for compression and

tension, respectively, which need to be empirically determined. The leapfrog method, with second-order accuracy, is employed in all PM simulations. The leapfrog formulas relating position, velocity and acceleration for particles Pi ( i = 1,2,..., N ) [Greenspan, 1997] are

G G (Δt ) G Vi ,1 / 2 = Vi , 0 + ai , 0 2

(starter formula)

(16)

G G G Vi ,k +1 / 2 = Vi ,k −1 / 2 + (Δt )ai ,k , k = 1,2,3,...

(17)

G G G ri ,k +1 = ri ,k + (Δt )Vi ,k +1 / 2 G

G

k = 0,1,2,...

(18)

G

where Vi ,k , ai ,k and ri ,k are the velocity, acceleration and position vectors of particle i at

G

time t k = kΔt , Δt is the time step. Vi ,k +1 / 2 stands for the velocity of particle i at time

t k = (k + 1 / 2)Δt , and so on. Notably, the leapfrog method is of second-order 2

accuracy: O ((Δt ) ) . The safe time step is after the derivation result by Hockney & Eastwood [1999]:

ΩΔt

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close